2 / Aluminum Alloy Castings: Properties, Processes, and Applicationscasting process. Continuing technological improvements in alloy, An ability to produce near-net-shape parts with dimensionalcasting, and recycling technology have improved the competitive- accuracy, controlled surface ﬁnish, complex geometries includingness and enhanced the growth of aluminum castings markets. internal passages, and properties consistent with speciﬁed engi- neering requirements represents signiﬁcant manufacturing advan- tages (Fig. 1.1, 1.2):1.3 Advantages and Limitations of Aluminum Castings • In many cases, multicomponent welded or joined assemblies can be replaced with a single cast part. Aluminum castings are produced in a range of alloys demon- • Machining requirements are reduced.strating wide versatility in the characteristics than can be achieved. • Aluminum castings display controlled variations in as-castMore than 100 compositions are registered with the Aluminum ﬁnish.Association, and more than 300 alloys are in international use. • Contrasts between as-cast and machined ﬁnishes can be high-Properties displayed by these alloys, without considering the ex- lighted to create pleasing cosmetic effects.panded capabilities of metal-matrix and other composite structures, • Capital requirements are typically less than for wrought prod-include: ucts. • Tooling can range from simple patterns to complex tool steel dies depending on product requirements and production vol-Tensile strength, ksi (MPa) 10–72 (70–505) ume.Yield strength, ksi (MPa) 3–65 (20–455)Elongation, % <1–30 • Metallurgically or mechanically bonded bimetal parts can beHardness, HB 30–150 routinely cast.Electrical conductivity, %IACS 18–60Thermal conductivity, Btu · in./h · ft2 · °F at 77 °F 660–1155 (85–175) • Aluminum parts are routinely cast by every known process, (W/m · K at 25 °C) offering a broad range of volume, productivity, quality, mecha-Fatigue limit, ksi (MPa) 8–21 (55–145)Coefficient of linear thermal expansion 9.8–13.7 ϫ 10–6/°F nization, and specialized capabilities. at 68–212 °F (20–100 °C) (17.6–24.7) ϫ 10–6/°C) • Most aluminum casting alloys display solidiﬁcation character-Shear strength, ksi (MPa) 6–46 (42–325)Modulus of elasticity, 106 psi (GPa) 9.5–11.2 (65–80) istics compatible with foundry requirements for the productionSpeciﬁc gravity 2.57–2.95 of quality parts.Fig. 1.1 Casting applications include innovative and complex designs serving the needs of diverse industries. (a) Aircraft stabilizer. (b) Golf irons. (c) Crankcase for small engine. (d) Cross member for a minivan. (e) Cellular phone casing. Source: Ref 1
Chapter 1: Introduction / 3• Many aluminum casting alloys display excellent ﬂuidity for the incentives to reduce fuel consumption while preserving product casting thin sections and ﬁne detail. performance and cost objectives.• Aluminum casting alloys melt at relatively low temperatures. The most cost-effective means of addressing these challenges• Aluminum casting processes can be highly automated. has been the substitution of lightweight materials in existing and projected automotive designs. The U.S. automotive industry in Many limitations do apply. Very thin sections may not be castable. collaboration with suppliers and the U.S. Department of EnergyThere are practical limitations in size for speciﬁc casting processes. formed coalitions, including USAMP, which focused on materialsThe solidiﬁcation behavior of some alloys precludes casting in characterization, and USCAR, which focused on materials devel-difficult engineered conﬁgurations or in speciﬁc casting processes. opment and process capabilities. Their objective has been to fa-The casting process is simpler and less capital intense than pro- cilitate the transition to lighter-weight materials and more fuel-cesses for producing forgings, extrusions, and rolled products. How- efficient performance without sacriﬁce in safety and with minimalever, solidiﬁcation in complex geometrical shapes, as with other impact on costfabrication options, can result in surface discontinuities and inter- The emphasis placed on improved efficiency in energy-nal microstructure features with varying degrees of quality that consuming applications has resulted in a steady increase in theaffect properties and performance. production and use of aluminum castings. The recent pattern of Aluminum alloy castings can display the tensile properties of growth in aluminum casting shipments in the United States, in-most forgings, extrusions, and rolled plate. Because wrought prod- cluding projections through the year 2005 is (Ref 2):ucts are normally characterized by ﬁnely recrystallized grain struc-tures with speciﬁc anisotropy and highly textured microstructural Casting shipments in the United Statesfeatures, ductility in longitudinal directions is typically greater than Year 106 lb 106 kgin castings that contain coarser grain structures. Conversely, thetypically uniaxial grain structure and absence of anisotropy in cast 1994 2880 1306 1995 2990 1356structures do not present design engineers with the challenges 1996 3260 1479associated with transverse property limitations. 1997 3380 1533 1998 3490 1583 1999 3550 1610 2000 3640 1651 2001 3800 17241.4 Major Trends Inﬂuencing 2202 4100 1860 2003 4500 2041 Increased Use of Aluminum Castings 2004 4900 2223 2005 5160 23411.4.1 Technology The importance of improved energy efficiency in recent decadesreﬂects the effects of increased gasoline and oil costs to the con- Cast aluminum has been used or demonstrated successfully for many decades in power-train applications including engine blocks,sumer and graduated government-mandated fuel-efficiency stan-dards for automobile and truck manufacturers. Environmental con- cylinder heads, pistons, transmission cases, and oil pans. In the ﬁrst wave of light-weighting, aluminum was extensively adopted forcerns, global competitiveness, and raw-material concerns reinforce these parts. For maximum impact on fuel efficiency, this expansion in the role of cast aluminum necessitated substitutions in more critical structural parts requiring the qualiﬁcation of new compo- nent designs, materials, and production methods. These applica- tions include traditionally cast iron, malleable iron, nodular iron and steel cross members, suspension and control arms, brackets, brake valves, rotors, and calipers. The commercialization of alu- minum-intense automobile designs can result in 20 lb less engine emissions over the life of an automobile for each pound of iron or steel replaced by lower-density aluminum with correspondingly signiﬁcant reductions in fuel consumption (Ref 3). New aluminum- intensive automotive construction concepts include cast ﬁttings or nodes for extruded stringers in monocoque assemblies and the development of energy-absorbing thin-wall cast space frames. Fig- ures 1.3 through 1.6 summarize the results of a study performed for the Aluminum Association showing the growth in cast alumi- num as well as total aluminum products in North American light vehicle production. The most signiﬁcant barrier to the acceptance of cast alumi- num in these and many other structural applications has been itsFig. 1.2 One-piece cast missile tail cone. A cost-effective and reliable reputation for variability. Overcoming this barrier required the alternative to what had been a multicomponent assembly demonstration of integrity and reliability derived from the evolu-
4 / Aluminum Alloy Castings: Properties, Processes, and Applications tion of manufacturing processes and effective process controls. To be economic, casting results must be consistent and predictable without reliance on extensive inspection and nondestructive evalu- ation. Each step in these developments has been the product of close collaboration between aluminum casting suppliers and the auto- motive industry. Not only are speciﬁc engineering criteria to be met for each new component, process designs and controls must reli- ably demonstrate capability and consistent product quality in theFig. 1.3 North American light vehicle change in aluminum content, 1991 high volumes that are required. New casting processes, alloys, to 2002 composite compositions, thermal treatments, process control meth- odologies, and the sensors and controls they require have contrib- uted to an accelerated evolution of technologies that has been facilitated by research and development programs, many of which were sponsored by USCAR and USAMP in cooperation with na- tional laboratories, colleges, and universities and with supplier industries. Aluminum castings will play an important future role when in- evitable electric, hybrid, or fuel-cell technologies are developed to combine materials, design, and construction methods for maximum efficiency. Technological progress achieved in automotive programs affects all phases of aluminum foundry operations and all casting appli- cations. Technology is also being broadly advanced by the activi- ties of the U.S. Department of Energy that has identiﬁed metal casting as one of nine important “Industries of the Future.” Beneﬁts have been the development of a technology roadmap (Ref 4) that includes many of the challenges and technical barriers facing the aluminum castings industry and the funding of research and de- velopment programs in casting, aluminum, sensors, automation, and industrial materials of the future to meet or overcome them.Fig. 1.4 North American light vehicle change in aluminum content, 1991 The product of these efforts has been greater versatility and to 2002. (a) Passenger cars. (b) Trucks improved capability in consistently and economically meeting even the most severe engineering challenges in automotive and other industries. Understanding the material and process changes that areAluminum product form 1999 lb/vehicle Percent of total 2002 lb/vehicle Percent of total Percent change 1999 vs 2002Die castings 95.76 38.2% 101.42 37.1% ϩ5.9% or 5.66 lbPermanent mold castings 92.43 36.9% 100.58 36.8% ϩ8.8% or 8.15 lbFlat rolled products 27.24 10.9% 29.39 10.7% ϩ7.9% or 2.15 lbExtruded and drawn products 16.83 6.7% 18.49 6.8% ϩ9.9% or 1.66 lbForgings and impacts 6.34 2.5% 6.10 2.2% –3.8% or –0.24 lbSand, lost foam, squeeze, and semisolid castings 11.94 4.8% 17.52 6.4% ϩ46.7% or 5.58 lbTotal 250.54 100% 273.50 100% ϩ9.2% or 22.96 lbFig. 1.5 North American light vehicle change in aluminum content by product form and metal source, 1999 to 2002
Chapter 1: Introduction / 5taking place to further increase the comfort of design engineers in with competing materials, the advantage of aluminum in life-cyclethe use of aluminum castings is essential for deﬁning material analysis can be signiﬁcant.advantages for any new application. 1.5 Selecting the Right1.4.2 Recycling Aluminum Alloy and Casting Process Recycling and its impact in life-cycle studies are increasinglyimportant considerations in materials selection (Ref 5). The manner The succeeding chapters review the substantial portfolio of alu-in which energy efficiency can be directly and indirectly affected minum casting alloys available; Chapter 2 illustrates the charac-is important, but so are environmental and competitive consider- teristics that have made certain alloys the ﬁrst choice for speciﬁcations. While the production of aluminum is energy-intensive, it applications. Chapters 3 through 7 focus on the process and thermalcan be efficiently recovered from scrap at 5% of the energy required treatment variables that inﬂuence the metallurgical structure offor reduction. Corrosion resistance preserves metal value, and new aluminum alloys and, in turn, how the combination of processtechnologies are being developed for the segregation of scrap variables and metallurgical structure inﬂuence their properties andstreams by alloy and product form for essentially closed-loop re- performance. Finally, Chapter 8 provides a broad range of physicalcycling. and mechanical property data, a substantial amount of which has Virtually all aluminum forms classiﬁed as old scrap (end of never been published before, certainly not all in a single resource.cycle) and new scrap (turnings, borings, gates and risers, rejec- This wide range of information contained herein is provided astions) are recyclable. With appropriate recycling processes, recov- a reference for aluminum alloy casting producers, heat treaters,eries typically exceed 90%. designers, and users with the intent of aiding them in the selection Many casting compositions are compatible with the alloy con- of the right alloy, temper, and processing needed to achieve thetent of even mixed scrap. The cost of ingot produced from scrap performance required of cast components. The authors believe itis typically less than that of primary metal. As a consequence, most is clear that, as suggested above, aluminum casting alloys providealuminum alloy castings are produced from recycled metal. a broad range of capabilities including—when appropriate, process- The use of aluminum in energy-consuming applications pro- optimization and quality-control procedures are applied—compo-vides efficiencies with calculable beneﬁts for prolonging product nents suitable for challenging applications where soundness,life, conserving raw materials, reducing energy consumption in strength, and toughness are critical. The authors hope it will also bemanufacturing and service, reducing levels of environmental pol- clear that there are great advantages for designers and castinglution and the costs of environmental control, and lowering ma- suppliers working closely with their customers on the selection ofterial cost through recycling. When factored into cost comparisons alloys, tempers, and casting processes capable of meeting manu-Fig. 1.6 North American light vehicle change in aluminum content, 1973 to 2002
6 / Aluminum Alloy Castings: Properties, Processes, and Applicationsfacturing objectives, component performance criteria, and eco- • Aluminum, the Magic Metal, National Geographic, Aug 1978nomic targets. • Aluminum Permanent Mold Handbook, American Foundry So- This reference volume is not intended as a guide to producing ciety, 2001, 216 pagesaluminum alloy castings; for example, it does not cover the details • R.J. Anderson and H. Carey, The Metallurgy of Aluminium andof how to design and build molds, inject the molten alloys, and Aluminium Alloys, Baird and Company, 1925sequence the ﬁnishing process. For more information on such mat- • L. Arnberg, L. Bäckerud, and A. Dahle, Castability of Alumi-ters, the reader is referred to the excellent aluminum casting in- num Foundry Alloys, AFS Research Report, American Found-dustry publications of the American Foundry Society and similar rymen’s Society, 1999, 111 pagesorganizations (Ref 1, 6–9) plus those of the Aluminum Association • C.C. Carr, Alcoa, An American Enterprise, Rinehart and Com-(Ref 10–12). For those interested in a broader overview of the pany, 1941entire aluminum industry, D.G. Altenpohl’s volume (Ref 13) is • Casting, Vol 15, ASM Handbook, ASM International, 1988recommended. • S. Das, The Life Cycle Impacts of Aluminum Body-in-White Automotive Material, JOM, Aug 2000REFERENCES • J.R. Davis, Ed., ASM Specialty Handbook: Aluminum and Alu-1. Principles of Purchasing Castings, CD-ROM, American minum Alloys, ASM International, 1993 Foundry Society, 2002 • Design and Procurement of High-Strength Structural Alumi-2. U.S. Department of Commerce num Castings, American Foundrymen’s Society, 1995, 48 pages3. S. Das, The Life Cycle Impacts of Aluminum Body-in-White • J.D. Edwards, F.C. Frary, and Z. Jeffries, The Aluminum In- Automotive Material, JOM, Vol 52 (No. 8), Aug 2000, p 41–44 dustry, McGraw Hill, 19304. “Metalcasting Industry Technology Roadmap,” Cast Metal • Forgings and Castings, Vol 5, 8th ed., Metals Handbook, Ameri- Coalition, American Foundrymen’s Society, North American can Society for Metals, 1970 Die Casting Association, and Steel Founders’ Society of • M.B.W. Graham and B.H. Pruitt, R&D for Industry: A Century America, Jan 19985. “U.S. Energy Requirements for Aluminum Production,” The of Technical Innovation at Alcoa, Cambridge University Press, U.S. Dept. of Energy, Jan 2003 19906. D. Zalenas, Ed., Aluminum Casting Technology, 2nd ed., • J.E. Hatch, Ed., Aluminum: Properties and Physical Metal- American Foundrymen’s Society, 1993 lurgy, American Society for Metals, 19847. “NADCA Product Speciﬁcation Standards for Die Casting,” • J.G. Kaufman, Introduction to Aluminum Alloys and Tempers, 5th ed., North American Die Casting Association (NADCA), ASM International, 2000 2003 • Melting and Recycling of Aluminum Alloys, American Found-8. “Product Design for Die Casting in Recyclable Aluminum, rymen’s Society, 1997, 66 pages Magnesium, Zinc, and ZA Alloys,” Die Casting Development • The Physical Metallurgy of Aluminum Alloys, American Soci- Council, 19969. “The NFFS Guide to Aluminum Casting Design: Sand and ety for Metals, 1949 Permanent Mold,” Non-Ferrous Founders Society, 1994 • Properties and Selection: Nonferrous Alloys and Special-10. “Designations and Chemical Composition Limits for Alumi- Purpose Materials, Vol 2, ASM Handbook, ASM International, num Alloys in the Form of Castings and Ingot,” The Aluminum 1990 Association Alloy and Temper Registrations Records, The Alu- • E.L. Rooy, Scrap Recycling and Its Impact on the Metal Cast- minum Association, Jan, 1996 ings Industry, AFS Trans., l98511. “Aluminum Standards & Data (Standard and Metric Edi- • G.D. Smith, From Monopoly to Competition, Cambridge Uni- tions),” The Aluminum Association, published periodically versity Press, 198812. “Standards for Aluminum Sand and Permanent Mold Cast- • Solidiﬁcation Characteristics of Aluminum Alloys, Vol 2, ing,” The Aluminum Association, Dec 199213. D.G. Altenpohl, Aluminum: Technology, Applications and En- Foundry Alloys, American Foundrymen’s Society, 1990, 266 vironment, The Aluminum Association and TMS, 1999 pages • Solidiﬁcation Characteristics of Aluminum Alloys, Vol 3, Den-SELECTED REFERENCES drite Coherency, American Foundrymen’s Society, 1996, 258 pages• Aluminum and Aluminum Alloys, The Pittsburgh Reduction • K.R. Van Horn, Ed., Aluminum, Vol 1–3, American Society for Company, 1897 Metals, 1967
8 / Aluminum Alloy Castings: Properties, Processes, and Applications• Major alloying elements deﬁne the ranges of elements that Variations in the composition limits that are too small to require control castability and property development. a change in numeric designation are indicated by a preceding letter• Minor alloying elements control solidiﬁcation behavior, modify (A, B, C, etc). The ﬁrst version of an alloy, say 356.0, contains no eutectic structure, reﬁne primary phases, reﬁne grain size and letter preﬁx; the ﬁrst variation has an A, e.g., A356.0, the second form, promote or suppress phase formation, and reduce oxi- a B, for example, B356.0, and so forth. dation. The ﬁrst digit deﬁnes the major alloying constituent or constitu-• Impurity elements inﬂuence castability and the form of in- ents, with the following categories being deﬁned: soluble phases that at times limit or promote desired properties. • lxx.x, pure aluminum (99.00% or greater)Preferred major, minor, and impurity element concentrations and • 2xx.x, aluminum-copper alloysrelationships may not be deﬁned by alloy speciﬁcations. Optimal • 3xx.x, aluminum-silicon ϩ copper and/or magnesiumresults are not implied by nominal chemistries. The addition of • 4xx.x, aluminum-siliconstructure-controlling elements or combinations of elements can be • 5xx.x, aluminum-magnesiumcontained within chemistry limits when not otherwise speciﬁed • 7xx.x, aluminum-zincunder “Other Elements Each.” • 8xx.x, aluminum-tin Stoichiometric ratios for favored phase formation can be speci- • 9xx.x, aluminum ϩ other elementsﬁed, but also may not be controlled or deﬁned. • 6xx.x, unused series Concentration limits allow biasing of composition for castabilityand property development. For maximum strength, the concen- In designations of the 1xx.x type, the second and third digits in-tration of elements that form hardening phases can be maximized. dicate minimum aluminum content (99.00% or greater); these dig-Improved ductility results from ﬁner structures, restricting in- its are the same as the two to the right of the decimal point in thesoluble-element concentrations, and by controlling the concentra- minimum aluminum percentage expressed to the nearest 0.01%.tions of impurities in ratios that favor the formation of the least For example, alloy 170.0 contains a minimum of 99.70% Al.detrimental intermetallic constituents. Composition biasing can be In 2xx.x through 8xx.x designations for aluminum alloys, thespeciﬁed in ingot procurement or can result from alloying adjust- second and third digits have no numerical signiﬁcance, but onlyments in the foundry. arbitrarily identify individual alloys in the group. In all casting alloy designations, the fourth digit, that to the right of the decimal point, indicates product form:2.3 Alloy Designations • 0 denotes castings • 1 denotes standard ingot Designation systems and alloy nomenclature for aluminum cast- • 2 denotes ingot having composition ranges narrower than buting alloys are not internationally standardized. Many nations have within those of standard ingotdeveloped and published their own standards. Individual ﬁrmshave also promoted alloys by proprietary designations. In NorthAmerica, the most commonly used system is that developed and Designations in the form xxx.1 and xxx.2 include the compositionmaintained by the Aluminum Association. General procurement of speciﬁc alloys in remelt ingot form suitable for foundry use.speciﬁcations issued through government agencies and technical Designations in the form xxx.0 in all cases deﬁne compositionassociations and societies typically reference this nomenclature. limits applicable to castings. Further variations in speciﬁed com- positions are denoted by preﬁx letters used primarily to deﬁne differences in impurity limits. Accordingly, one of the most com-2.3.1 The Aluminum Association (AA) Casting Alloy mon gravity cast alloys, 356, has variations A356, B356, and C356; Designation System each of these alloys has identical major alloy contents, but has The most widely used casting alloy designation system in the decreasing speciﬁcation limits applicable to impurities, especiallyUnited States is the Aluminum Association (AA) alloy and temper iron content.systems (Ref 1), which are described below. Regrettably, the AA Alloying-element and impurity limits for ingot are usually thesystem is not universally used, and some of its earlier modiﬁcations same as those for castings of the same alloy. When the ingot isare still widely quoted. Therefore, subsequent sections discuss the remelted, iron and silicon contents tend to increase and magnesiumearlier variations as well as other rather widely used designations. content decreases. For these reasons, ingot chemistry for some In the AA alloy designation, there are four numeric digits, with alloys may be somewhat different from those speciﬁed for castings.a period between the third and fourth. The meanings of the four Despite the broad acceptance of the AA casting alloy designationdigits are: system, including recognition by the American National Standards Institute (ANSI), it remains relatively common to see the alloys• First digit: Principal alloying constituent(s) listed with only the ﬁrst three digits of the alloy designation, for• Second and third digits: Speciﬁc alloy designation (number has example, for 356.0, one may see simply 356 (see Section 2.3.3 in no signiﬁcance but is unique) this chapter). Technically, this is obsolete usage of the designation• Fourth digit: Casting (0) or ingot (1, 2) designation system, and for cast components the “.0” should always be utilized.
Chapter 2: Aluminum Casting Alloys / 9 The nominal compositions and composition limits of aluminum formal basis. They cause confusion because there is no obvious linkalloys in commercial use today are presented in Table 2.1. to the current system if one does not have a conversion guide such as Table 18.104.22.168.2 Aluminum Association Casting Temper The other fairly often seen variation is the result of the signiﬁcant Designation System revision of the Aluminum Association system in around 1990, The Aluminum Association Casting Temper Designation System when the guidelines for registering the alloys including copper and(Ref 1) uses letters and numbers to indicate the major types of magnesium were changed. The result was that some alloys shiftedthermal treatments applicable to engineered castings: classiﬁcation; for example, alloy 195.0 became 295.0 and alloy 214.0 became 514.0.• F, as-cast• O, annealed 2.3.4 The UNS Alloy Designation System• T4, solution treated and aged Another rather widely known alloy classiﬁcation system is the• T5, precipitation hardened Uniﬁed Numbering System (UNS) (Ref 2). The UNS system has• T6, solution heat treated, quenched, and precipitation hardened the advantage of covering all metallic alloy systems.• T7, solution heat treated, quenched, and overaged For aluminum alloys, as illustrated in Table 2.2, this system is essentially an adaptation of the Aluminum Association alloy des- Temper designation is presented immediately following the alloy ignation system to ﬁt the UNS format. UNS numbers are obtaineddesignation. Thus, for a 356.0 alloy casting that has been solution by taking the three digits to the left of the decimal point in theheat treated, quenched, and artiﬁcially aged, the full alloy and Aluminum Association system and adding A9 (meaning aluminumtemper designation would be shown as 356.0-T6. Examples of alloys) and a digit reﬂecting the letter preﬁx to the alloy desig-registered temper variations are A357.0-T61, 242.0-T571, and nation. For alloys with no letter preﬁx, the next numeric digit after355.0-T71. A9 is a 0; for those with A, the next digit is 1, for B, it is 2, and Other variations of temper designations are permitted by the so forth.Aluminum Association Temper Designation System (Ref 1), the Thus, in the UNS system, 356.0 becomes A90356, A356.0 be-most common being the use of “P” added to a standard temper comes A91356, C356.0 becomes A93356; and so forth.designation (e.g., T6P) indicating a producer variation of the stan- The UNS system is not as widely used for aluminum alloys asdard processing treatment. There is further discussion of temper for certain other classes of alloys. An example would be copperdesignations in Chapter 7, “Heat Treatment of Aluminum Cast- alloys, for which the UNS designations have been selected as theings.” U.S. standards.2.3.3 Evolution of Designation System; 2.3.5 International Casting Alloy Designations Cross-Reference to Older Designations Unlike the case for wrought aluminum alloys, there is no inter- As noted previously, over the years there have been several national accord on casting alloy designations, and other systems areevolutionary steps in the development of the Aluminum Associa- rather universally used overseas (Ref 3). Most systems employtion casting alloy designation system, with the result that it is not some system based on identifying the major alloying elements, butuncommon to ﬁnd variations of the current designations appearing regrettably there are many variations of these.on drawings and in publications from not too many years ago, and One of the mostly widely used international systems is the Eu-in some cases even in current publications. To assist in dealing with ronorm designation, and so, where applicable, designations of thatsuch variations, Table 2.2 illustrates a number of the variations in type have been included in Table 2.2. There are no comparablecasting alloy designations over the past 50 years. Euronorm designations for about half of the alloys registered in the The overall most common variation is clearly the omission of the United States, nor is there any simple guide to generate them.decimal point and the fourth digit, always a .0 for a foundry prod-uct. While inconsistent with current Aluminum Association stan-dards, this variation is not usually a problem resulting in confusion, 2.3.6 Nomenclature System for Aluminumas for example it is relatively clear that an alloy designated 354 may Metal-Matrix Compositessafely be assumed to be 354.0 by today’s standard system. Aluminum casting alloys are now regularly used as the matrix While the most common variation is the omission of the decimal material in metal-matrix composites (MMC). The Aluminum As-point and the fourth digit in the designation, there are two other sociation, Inc, and ANSI H35.5 (Ref 4) have published a standardtypes of variations reﬂected in Table 2.2 that are also seen fre- nomenclature system for such composites that builds on the stan-quently and can be more confusing. One variation is simply a dard casting alloy designation system as outlined below. Althoughproprietary designation that has become rather widely known in the this standard nomenclature has been established, some MMC sup-past, for example, Hiduminium, Frontier 40E, Precedent 71, and pliers have preferred their own designations. One reason is thatAlmag 35. These designations originated before the alloy compo- matrix alloys may not coincide exactly with Aluminum Associationsitions were registered with the Aluminum Association and had no ranges.
Chapter 2: Aluminum Casting Alloys / 13 The designation system for aluminum metal-matrix composites Many alloys containing 4 to 5% Cu have been developed, usuallyconsists of four parts: with varying amounts of magnesium. Silver accelerates aging re- sponse and reduces the risk of stress corrosion. These heat treatable• The matrix alloy designation employs the Aluminum Associa- compositions represent the highest-strength capabilities of any com- tion alloy designation as described in Section 2.1 in this chapter. mercial casting alloys. With controlled impurities, excellent duc- It is immediately followed by a slash that separates it from the tilities are also achieved. The combination of tensile properties and rest of the composite designation. ductility provide exceptional toughness.• The composition of the reinforcement is shown immediately Alloys of this type are susceptible to solidiﬁcation cracking and after the slash, using the appropriate chemical designation, with to interdendritic shrinkage. Exacting foundry techniques are re- the exception that no subscripts or superscripts are used. Some quired to avoid these conditions. In permanent mold or other rigid common examples cited in the standard are: C for graphite, SiC mold casting methods, excellent grain reﬁnement and selective for silicon carbide, and Al2O3 for aluminum oxide (alumina). chilling are essential. This reinforcement designation is also followed without space Copper-containing aluminum alloys are less resistant to corro- by a slash. sion, and certain compositions and material conditions may be• The volume percent of the reinforcement is shown immediately susceptible to stress corrosion. after the second slash. It is always presented as two digits, for Copper is typically the alloy basis for improved mechanical example, 05 for 5%, 10 for 10%, 20 for 20%, and so forth. properties at elevated temperature, often with nickel additions.• Immediately following the percentage is a single lower-case 2.4.2 Aluminum-Silicon-Copper letter for the type of reinforcement: c for cut or chopped ﬁbers, ﬁlaments, or monoﬁlaments; f for continuous ﬁbers, ﬁlaments, Among the most widely used aluminum casting alloys are those or monoﬁlaments; p for particles (particulate); and w for whis- that contain silicon and copper. The amounts of both additions vary kers. widely, so that copper predominates in some alloys and silicon in others. Copper contributes to strengthening and machinability, and Some common illustrations of cast aluminum metal-matrix com- silicon improves castability and reduces hot shortness. Alloys con-posite designations are: taining higher hypoeutectic concentrations of silicon are normally better suited for more complex castings and for permanent mold• A356.0/Al2O3/05f: Alloy A356.0 reinforced with 5% alumi- and die casting processes. num ﬁlaments Aluminum-silicon-copper alloys with less than 5.6% Cu are heat• 360.0/C/20c: Alloy 360.0 reinforced with 20% chopped ﬁbers treatable, but the more important alloys of this family are those also• 380.0/SiC/10p: Alloy 380.0 reinforcement 10% silicon carbide containing magnesium. Heat treatment response is enhanced, lead- particulate ing to a very attractive range of properties including premium- strength capabilities. Many hypereutectic silicon alloys (12 to 30% Si) also contain2.4 Composition Groupings copper. The primary silicon phase imparts excellent wear resis- tance, and copper contributes to matrix hardening and elevated- Although a large number of aluminum casting alloys have been temperature strength.developed, there are seven basic families: 2.4.3 Aluminum-Silicon• Aluminum-copper (2xx) Binary aluminum-silicon alloys exhibit excellent ﬂuidity, cast-• Aluminum-silicon-copper (3xx) ability, and corrosion resistance. These alloys display low strength• Aluminum-silicon (4xx) and poor machinability. Ductility, which can be exceptional, is a• Aluminum-silicon-magnesium (3xx) function of low impurity concentrations and microstructural fea-• Aluminum-magnesium (5xx) tures. The strength, ductility, and castability of hypoeutectic alu-• Aluminum-zinc-magnesium (7xx) minum-silicon alloys can be further improved by modiﬁcation of• Aluminum-tin (8xx) the aluminum-silicon eutectic. Modiﬁcation is particularly advan- tageous in sand castings and can be effectively achieved through2.4.1 Aluminum-Copper the controlled addition of sodium and/or strontium. Calcium is a Aluminum-copper alloys have been used extensively in cast and weak eutectic modiﬁer and a more lamellar eutectic can be achievedwrought form where strength and toughness are required. These with antimony. Higher solidiﬁcation rates also promote a ﬁneralloys exhibit high strength and hardness at room and elevated unmodiﬁed eutectic microstructure.temperatures. Aluminum-silicon alloys exhibit low speciﬁc gravity and coef- The ﬁrst signiﬁcant aluminum casting alloys contained copper at ﬁcients of thermal expansion.concentrations up to 10%. With no understanding of heat treatment, In hypereutectic aluminum-silicon alloys, reﬁnement of thethese alloys displayed signiﬁcantly improved strengths and hard- proeutectic silicon phase by phosphorus additions is essential fornesses in the as-cast state. casting and product performance.
14 / Aluminum Alloy Castings: Properties, Processes, and Applications2.4.4 Aluminum-Silicon-Magnesium Machinability and resistance to general corrosion is usually good. The addition of magnesium to aluminum-silicon alloys forms the The chemistry of most alloys is controlled to minimize stress-basis for an extremely important and useful family of compositions corrosion susceptibility.that combines outstanding casting characteristics with excellent The castability of Al-Zn-Mg alloys is poor, and good foundryproperties after heat treatment. Corrosion resistance is also excel- practices are required to minimize hot tearing and shrinkage de-lent, and a low level of thermal expansion is retained. fects. While not as strong as high-strength Al-Cu and Al-Si-Cu alloys,the mechanical properties of several Al-Si-Mg alloys provide me- 2.4.7 Aluminum-Tinchanical properties in the premium-strength range. Beryllium ad-ditions improve strength and ductility by affecting the morphology Tin is the major alloying element in compositions developed forand chemistry of the iron-containing intermetallic. bearing applications. It has also been employed with bismuth, lead, Eutectic modiﬁcation remains important as a means of improv- and cadmium at lower concentrations to provide free-machininging strength, substantially increasing elongation, and improving properties. The 850-series alloys can often be substituted for 660casting results. or similar bronzes. Their light weight minimizes loads in recip- rocating applications, and heat dissipation improves bearing life.2.4.5 Aluminum-Magnesium Alloys containing 5.0 to 7.0% Sn are broadly used in bearings and bushings in which low friction, compressive strength, fatigue These are essentially single-phase binary alloys with moderate strength, and resistance to corrosion are important criteria. Addi-to high strength and toughness. Their most important characteristic tions of copper, nickel, and magnesium contribute to hardness andis corrosion resistance, including exposure to seawater and marine strength, and silicon is added to improve castability, reduce hotatmospheres. This characteristic is also the basis for extensive use shortness, and increase compressive yield strength.in food and beverage processing. Aluminum-magnesium alloys Most bearings are produced by the permanent mold process.offer excellent weldability and are often used in architectural and Higher-solidiﬁcation rates promote the ﬁner, more uniform dis-other decorative applications. Aluminum-magnesium alloys have persion of tin. Larger, special-design, and low-volume bearings aregood machinability, weldability, and an attractive appearance nevertheless cast successfully in sand molds. Because most bear-whether as-cast, machined, polished, or anodized. ings are simple hollow or solid cylinders, the direct chill (DC) In comparison with aluminum-silicon alloys, all aluminum- casting process has also been used for production.magnesium alloys require more care in gating, larger risers, and Aluminum-tin alloys are unique among signiﬁcant composi-greater control of temperature gradients. tions. Aluminum and tin are essentially immiscible. Before and Magnesium in aluminum alloys increases oxidation rates. In the after solidiﬁcation, tin is present in dispersed form. Mechanicalmolten state, magnesium losses can be signiﬁcant and oxides of agitation is required initially to achieve suspension of tin, and,aluminum and magnesium can affect casting quality. Spinels of because of density differences, gravity segregation may occur overaluminum and magnesium oxides form with unprotected exposure time in the molten state.at high molten metal temperatures. The potential for inclusions is Aluminum-tin alloys containing copper are conventionally pre-especially important because many applications involve polishing cipitation hardened and may be fully heat treated. Because mostand/or ﬁne surface ﬁnishing. bearings are cast in simple solid or hollow cylindrical shapes, parts Alloys containing >7.0% Mg are heat treatable, although thermal may be plastically cold worked to improve compressive yieldtreatments are more typically used to stabilize properties that could strength. Solidiﬁcation and thermal stresses are also relieved byotherwise change, in some compositions, over long periods of time. axial compression resulting in 4% permanent deformation. 2.4.6 Aluminum-Zinc-Magnesium Many alloys of this type naturally age, achieving full strengthwithin 20 to 30 days at room temperature after casting. Solution 2.5 Effects of Alloying Elementsheat treatment is not typically necessary for property development.Rapid solidiﬁcation in these alloys can result in microsegregation 2.5.1 Antimonyof magnesium-zinc phases that reduces hardening potential. Con- At concentration levels equal to or greater than ϳ0.10%, anti-ventional solution heat treatments can be used when adequate prop- mony reﬁnes the aluminum-silicon eutectic. The effect is essen-erty development does not occur through natural aging. tially that of modiﬁcation, but a distinctly lamellar eutectic rather Since high-temperature solution heat treatment and quench are than a ﬁne ﬁbrous form results. The effectiveness of antimony innot normally required, the cost of heat treatment, high residual altering the eutectic structure depends on an absence of phosphorusstress levels and distortion are avoided. and on an adequately rapid rate of solidiﬁcation. Antimony also Artiﬁcial aging treatments can be used to accelerate the hard- reacts with either sodium or strontium to form coarse intermetallicsening process, and annealing treatments accomplish the same pur- with adverse effects on castability and metallurgical structure.pose with improved dimensional and structural stability. Antimony is classiﬁed as a heavy metal with potential toxicity These alloys typically display moderate to good tensile proper- and hygiene implications, especially associated with stibine gasties in the as-cast condition. The melting temperatures of alloys of (SbH3) formation and the effects of human exposure to other an-this group are high, an advantage in castings that are to be brazed. timony compounds.
Chapter 2: Aluminum Casting Alloys / 152.5.2 Beryllium compositions, but it is rarely encountered in gravity casting alloys. Additions of a few parts per million beryllium can be effective Chromium improves corrosion resistance in certain alloys and in-in reducing oxidation losses and associated inclusions in magne- creases quench sensitivity at higher concentrations.sium-containing compositions. 2.5.8 Copper At higher concentrations (>0.04%), beryllium affects the formand composition of iron-containing intermetallics, markedly im- Copper substantially improves strength and hardness in the as-proving strength and ductility. In addition to changing the mor- cast and heat treated conditions. Alloys containing 4 to 5.5% Cuphology of the insoluble phase from script or plate to nodular form, respond most strongly to thermal treatment and display relativelyberyllium changes its composition, rejecting magnesium from the improved casting properties. Copper generally reduces resistanceAl-Fe-Si complex and thus permitting its full use for hardening to general corrosion and in speciﬁc compositions and materialpurposes. conditions increases stress-corrosion susceptibility. Conversely, low Beryllium-containing compounds are, however, known carcino- concentrations of copper in aluminum-zinc alloys inhibit stressgens that require speciﬁc precautions in melting, molten metal corrosion.handling, dross handling, dross disposition, and welding. Copper reduces hot tear resistance and increases the potential for interdendritic shrinkage.2.5.3 Bismuth 2.5.9 Iron Bismuth additions improve the machinability of cast aluminum Iron improves hot-tear resistance and decreases the tendency foralloys at concentrations greater than 0.1%. die sticking or soldering in die casting. Increases in iron content2.5.4 Boron are accompanied by substantially decreased ductility. Iron reacts to form a number of intermetallic phases, the most common of which Boron combines with other metals to form borides, such as AlB2 are FeAl3, FeMnAl6, and ␣AlFeSi. These essentially insolubleand TiB2. Titanium boride forms stable nucleation sites that interact phases are responsible for improvements in strength, especially atwith active grain-reﬁning phases such as TiAl3 for grain reﬁne- elevated temperature, but also the embrittlement of the micro-ment. structure. As the fraction of insoluble phases increases with in- Metallic borides reduce tool life in machining operations and creased iron content, casting considerations such as feeding char-form coarse or agglomerated inclusions with detrimental effects on acteristics are adversely affected. Iron participates in the formationmechanical properties and ductility. Borides also contribute to of sludging phases with manganese, chromium, and other ele-sludging, the precipitation of intermetallics from liquid solution in ments.furnaces and troughing. Boron treatment of aluminum-containing peritectic elements such 2.5.10 Leadas titanium, zirconium, and vanadium is practiced to improve pu- Lead is used at concentrations greater than 0.1% to improverity and conductivity in electrical applications. Rotor alloys may machinability.specify boron to exceed titanium and vanadium contents to ensureeither the complexing or precipitation of these elements for im- 2.5.11 Magnesiumproved electrical performance. Magnesium is the basis for strength and hardness development2.5.5 Cadmium in heat treated aluminum-silicon alloys and is commonly used in more complex aluminum-silicon alloys containing copper, nickel, In concentrations exceeding 0.1%, cadmium improves machin- and other elements for the same purpose. The hardening-phaseability. Precautions that acknowledge volatilization of cadmium at Mg2Si displays a useful solubility limit corresponding to approxi-1413 ºF (767 ºC) are essential. mately 0.70% Mg, beyond which either no further strengthening occurs or matrix softening takes place. Common high-strength2.5.6 Calcium aluminum-silicon compositions specify magnesium in the range of Calcium is a weak aluminum-silicon eutectic modiﬁer. It in- 0.40 to 0.070%.creases hydrogen solubility and is often responsible for casting Binary aluminum-magnesium alloys are widely used in appli-porosity at trace concentration levels. Calcium greater than ap- cations requiring a bright surface ﬁnish, excellent response toproximately 0.005% also adversely affects ductility in aluminum- chemical ﬁnishing, corrosion resistance, and attractive combina-magnesium alloys. tions of strength and ductility. Common compositions range from 4 to 10% Mg, and compositions containing more than 7% Mg are2.5.7 Chromium heat treatable. Instability and long-term room-temperature aging at Additions of chromium are commonly made in low concentra- higher magnesium concentrations can be avoided by heat treat-tions to room-temperature aging and thermally unstable compo- ment.sitions in which germination and grain growth are known to occur.Chromium typically forms the compound CrAl7, which displays 2.5.12 Manganeseextremely limited solid-state solubility and is therefore useful in Normally considered an impurity in casting compositions, man-suppressing grain-growth tendencies. Sludge that contains iron, ganese is controlled to low levels in most gravity cast composi-manganese, and chromium is sometimes encountered in die casting tions. Manganese is an important element in work-hardened
16 / Aluminum Alloy Castings: Properties, Processes, and Applicationswrought alloys through which secondary foundry compositions relationship between cooling rate and ﬂuidity and the effect ofmay contain higher manganese levels. In the absence of work percentage of eutectic on feeding as solidiﬁcation progresses.hardening, manganese offers no signiﬁcant beneﬁts in cast alumi- Silicon combines with magnesium to form Mg2Si in heat treat-num alloys. Some evidence exists, however, that a high-volume able alloys. It combines with iron and other elements to formfraction of MnAl6 in alloys containing more than 0.5% Mn may complex insoluble phases.beneﬁcially inﬂuence internal soundness (Ref 5). Manganese can Silicon also reduces speciﬁc gravity and coefficient of thermalalso be employed to alter response in chemical ﬁnishing and an- expansion.odizing. Iron and manganese may be considered isomorphous, andalloy chemistry may reﬂect stoichiometries favoring the least det- 2.5.17 Silverrimental insoluble Al-Fe-Mn phases. Used in only a limited range of aluminum-copper premium-2.5.13 Mercury strength alloys at concentrations of 0.5 to 1.0%. Silver contributes to precipitation hardening and stress-corrosion resistance. Compositions containing mercury were developed as sacriﬁcialanodes for cathodic protection systems, especially in marine en-vironments. The use of these optimally electronegative alloys, 2.5.18 Sodiumwhich do not passivate in seawater, was severely restricted for Sodium modiﬁes the aluminum-silicon eutectic. In the absenceenvironmental reasons. of phosphorus, recovered concentrations of 0.01% are effective. Sodium interacts with phosphorus to reduce its effectiveness in2.5.14 Nickel modifying the eutectic and that of phosphorus in the reﬁnement of Nickel is commonly used with copper to enhance elevated- the primary silicon phase.temperature properties. It also reduces coefficient of thermal ex- Sodium at less than 0.005% is embrittling in aluminum-pansion. magnesium alloys. Sodium is rapidly lost in molten aluminum through its high vapor2.5.15 Phosphorus pressure so that modifying effects are transient. Periodic additions are required to maintain modiﬁcation levels. As AlP3, phosphorus nucleates and reﬁnes primary silicon-phase Sodium increases surface tension and through addition methodsformation in hypereutectic aluminum-silicon alloys. At parts per can increase hydrogen content. Overmodiﬁcation increases misrunmillion concentrations, phosphorus coarsens the eutectic structure tendencies in gravity casting.in hypoeutectic aluminum-silicon alloys and diminishes the effec- Unlike some other modiﬁers, sodium provides effective alumi-tiveness of common eutectic modiﬁers, sodium and strontium. num-silicon eutectic modiﬁcation under all solidiﬁcation condi- tions.2.5.16 Silicon The outstanding effect of silicon in aluminum alloys is the im- 2.5.19 Strontiumprovement of casting characteristics. Additions of silicon dramati-cally improve ﬂuidity, hot tear resistance, and feeding character- Strontium modiﬁes the aluminum-silicon eutectic. Effectiveistics. The most prominently used compositions in all aluminum modiﬁcation can be achieved at very low addition levels, but acasting processes are those in which silicon plays a major role. range of recovered strontium of 0.008 to 0.04% is commonly used.Commercial alloys span the hypoeutectic and hypereutectic ranges Lower concentrations are effective with higher solidiﬁcation rates.up to about 30% Si. Higher addition levels are associated with casting porosity. De- Increasing silicon content improves ﬂuidity for ﬁlling thin walls gassing efficiency may also be adversely affected at higher stron-and for reproducing more intricate designs and details. Aluminum- tium levels.silicon alloys are typically more resistant to solidiﬁcation cracking Strontium has been regarded as ineffective as a modiﬁer at slowand display excellent castability and feeding characteristics. solidiﬁcation rates, but some investigators report beneﬁcial effects Percent liquid in the solidiﬁcation range is dictated by the initial in AFS Level 4 and 5 structures in 319.0 and 356.0 alloys whencomposition and by the degree of nonequilibrium cooling. For >200 ppm Sr is present.higher-solidiﬁcation-rate processes such as pressure die and per-manent mold casting and for thinner sections in which more rapid 2.5.20 Tinsolidiﬁcation takes place, shrinkage porosity is strongly affected by Tin is effective in improving antifriction characteristics and isthe temperature at which mass feeding from liquid to partially therefore useful in bearing applications. Casting alloys may containsolidiﬁed structures no longer occurs. Feeding to minimize shrink- up to 25% Sn. Additions of tin also improve machinability.age porosity improves as the volume fraction solidiﬁed is increasedat the temperature at which mass feeding ceases. For this reason,the most desirable silicon content of aluminum-silicon alloys cor- 2.5.21 Titaniumresponds to the characteristic process solidiﬁcation rate. For slow Titanium is extensively used to reﬁne the grain structure ofcooling rate processes such as plaster, investment, and sand, the aluminum casting alloys, often in combination with smallerpreferred range is 5 to 7%, for permanent mold 7 to 9%, and for amounts of boron. The operable phase is TiAl3 with lattice spacingdie casting 8 to 12%. The bases for these recommendations are the closely matched to that of aluminum. Titanium in excess of the
Chapter 2: Aluminum Casting Alloys / 17stoichiometry of TiB2 is necessary for effective grain reﬁnement. and lower resistance to corrosion. These and similar general-Titanium is often employed at concentrations greater than those purpose alloys are often produced in the as-cast condition. Artiﬁcialrequired for grain reﬁnement to reduce cracking tendencies in aging can improve hardness, stability, and machinability. Typicalhot-short compositions. applications include:2.5.22 Zinc • Machinery • Transmission cases (Fig. 2.2) Zinc offers no signiﬁcant beneﬁts in aluminum casting. Accom- • Engine blockspanied by the addition of copper and/or magnesium, however, zinc • Gas meters and regulatorsresults in attractive heat treatable or naturally aging compositions. • Gear blocksA number of such compositions are in common use. Zinc is also • Gear casescommonly found in secondary gravity and die casting composi- • Fuel pumpstions. In these alloys, tolerance for up to 3% Zn allows the use of • Impellerslower-grade and wrought alloy scrap. • Instrument cases • Lawnmower decks • Intake manifolds2.6 Alloy Groupings by Application or • Cylinder heads Major Characteristic • Clutch housings • Oil pans2.6.1 General-Purpose Alloys • Outboard motor propellers, motor parts and housings Alloys with silicon as the major alloying constituent are the mostimportant commercial casting alloys, primarily because of theirsuperior casting characteristics. The large number of alloys of thistype that have been developed displays a broad range of properties. Binary aluminum-silicon alloys (443.0, 444.0, 413.0, and A413.0)are low-density, weldable, and resistant to corrosion. Althoughcastings of these alloys are somewhat difficult to machine, goodresults are obtained with cutting ﬂuids, sintered carbide tools, andchip breakers. Alloy 443.0 is used with all casting processes for parts in whichstrength is less important than ductility, resistance to corrosion, andpressure tightness. Permanent mold alloys 444.0 and A444.0 display high ductilityand are used where impact resistance is a primary consideration. Alloys 413.0 and A413.0 are close to the eutectic compositionand, as a result, have very high ﬂuidity. They are useful in diecasting and where large-area, thin-walled parts with cast-in let-tering or other high-deﬁnition details are required. Representative applications for these alloys are:• Architectural panels and spandrels• Outdoor lamp housings• Lawn mower decks• Outdoor grills• Marine components• Cooking utensils• Parts used in food, dairy, and beverage processing• Medical and dental equipment• Electronic cabinet frames and components• Tire molds• Escalator and moving sidewalk tread plates and parts• Highway railing posts (Fig. 2.1); alloy A444.0 being the stan- dard for this application Fig. 2.1 Example of one of the many highway railing post designs utilizing Aluminum-silicon-copper alloys such as 308.0, 319.0, 360.0, aluminum castings that have been developed. The alloy is A444.0-380.0, and 384.0 offer good casting characteristics, higher strength T4 with minimum elongation in permanent mold castings of 20% in frontand hardness, and improved machinability with reduced ductility ﬂanges for maximum energy absorption during impact.
18 / Aluminum Alloy Castings: Properties, Processes, and Applications Aluminum-silicon-magnesium alloys including 356.0 and • Industrial beam headsA356.0 have excellent casting characteristics and resistance to • Brake cylinderscorrosion. Heat treatment provides combinations of tensile and • Automobile cross members and suspension componentsphysical properties that make them attractive for many applicationsincluding machinery, automotive, military, and aerospace parts. Aluminum-silicon-copper-magnesium alloys such as 328.0.Higher tensile properties are obtained with 357.0, A357.0, 358.0, 333.0, 354.0, 355.0, and C355.0 offer excellent strength and hard-and 359.0 alloys. The high properties of these alloys, attained by ness with some sacriﬁce in ductility and corrosion resistance. Cast-heat treatment to the fully hardened condition, are of special in- ing characteristics are good, but inferior to those displayed byterest in structural applications. Developments in high-integrity die copper-free aluminum-silicon alloys. Properties in the as-cast con-casting have resulted in low-iron, manganese-containing Al-Si-Mg dition can be acceptable for some applications, but these alloys arealloys such as 365.0 and AlMg3Mn. Some typical uses include: typically heat treated for optimal properties. Alloy C355.0 with low iron is a higher-strength version of 355.0. When premium-strength• Automotive space frames casting processes are used, even higher tensile properties can be• Automotive wheels obtained with heat treated Alloy 354.0. Alloys of this type are• Truck wheels routinely cast in sand and permanent mold.• Axle and differential housings (Fig. 2.3)• Pump bodies• Meter bodies• Compressor bodies• Intake manifolds• Cylinder heads• Dies for plastic injection molding• Machine parts• Truck and bus frames and chassis components• Suspension saddles (Fig. 2.4)• Aircraft pylons, canopies, ﬂaps, speed-brakes hatch covers, and other ﬁttings• Impellers• Wave guides• Electronic cases• Fuel pumps• Missile bodies, ﬁns, and other structural parts Fig. 2.3 Die cast alloy 380.0 rear axle housingFig. 2.2 Die cast alloy 380.0 transmission case Fig. 2.4 Alloy A356.0 trailer suspension saddle
Chapter 2: Aluminum Casting Alloys / 19 Applications include: More complex aluminum-silicon alloys have been developed to meet the demands of high speciﬁc output, fuel-efficient engines that• Engine cooling fans operate at higher temperatures. Some of these alloys retain yield• Clutch housings strengths over 10 ksi (70 MPa) at temperatures exceeding 500 °F• Crankcases (260 °C).• High-speed rotating parts such as fans and impellers Piston alloys for heavy-duty and diesel engines include low-• Structural aerospace components expansion alloys 332.0-T5 and 336.0-T551. Alloy 242.0-T571 of-• Air compressor pistons fers higher thermal conductivity and superior properties at elevated• Fuel pumps (Fig. 2.5) temperatures.• Compressor cases Other applications of aluminum alloys for elevated-temperature• Rocker arms use include air-cooled cylinder heads for aircraft and motorcycles.• Timing gears Alloy 220.0-T61 was once used extensively for this purpose, but• Machine parts has been largely replaced by more castable 242.0 and 243.0 alloys with superior elevated-temperature properties.2.6.2 Elevated-Temperature Alloys Alloys 295.0, 355.0, and C355.0 have been extensively used in applications requiring strength and hardness at temperatures up to Many aluminum alloys have been developed to provide strength, 350 °F (175 °C). They include aircraft motor and gear housings.wear resistance, and hardness at elevated temperatures. The re- Alloy A201.0 and 204.0/206.0 type alloys have also been used intention of these properties as temperature increases is an advantage this temperature range when the combination of high strength atin many applications. room temperatures and elevated temperatures is required. Cast aluminum alloy pistons featuring low speciﬁc gravity, low Applications include:thermal expansion, elevated-temperature strength, wear resistance,and high thermal conductivity are the international standard for • Cylinder headsinternal combustion engines. Lower inertial forces permit higher • Motorcycle engine partsengine speeds, reduced bearing requirements, and lighter, simpler • Gear housingscrankshaft designs. • Pistons Aluminum pistons are usually permanent mold castings. Wrist • Structural parts exposed to elevated temperaturespin bore struts and compression ring-groove inserts can be cast-in;in large diesel engine pistons, integral cooling passages can be 2.6.3 Wear Resistant Alloysincorporated through copper coils or coring methods. The alloy most commonly used for pistons in passenger cars, Alloys containing greater-than-eutectic silicon concentrationssports-utility vehicles, and light trucks, 332.0-T5, demonstrates a display low speciﬁc gravity and elevated-temperature strength anddesirable combination of foundry, mechanical, and physical char- are often used in applications requiring a high degree of wearacteristics, including low thermal expansion. Precipitation hard- resistance. While wear resistance is usually associated with surfaceening from air or water quenching from the mold improves hard- hardness resulting from matrix properties or anodized coatings,ness for improved machinability and eliminates or reduces changes wear resistance in these alloys results from the presence of a largein dimensions from residual growth at operating temperatures. volume fraction of hard primary silicon particles in the micro- structure. Growth in the popularity of these alloys has accelerated in recent years. Alloys include 390.0, 392.0, and 393.0. Hypereutectic aluminum-silicon alloys are relatively more dif- ﬁcult to cast and machine, but are used in all casting processes. Matrix-hardening alloys also provide improved wear resistance. Alloys of the 2xx.0 and 355.0 family are considered wear resistant. Applications include: • Brake rotors • Cylinder blocks • Cylinder liners • Marine engines • Pistons 2.6.4 Moderate-Strength Alloys with Low Residual Stresses A number of casting compositions have been developed to pro- vide strength and hardness without heat treatment through natural aging. These alloys offer dimensional stability that reduces dis-Fig. 2.5 Alloy C355.0 fuel pump housing tortion during machining and simpliﬁes straightening to close tol-
20 / Aluminum Alloy Castings: Properties, Processes, and Applicationserances. The cost of heat treatment is avoided or reduced and • Automotive suspension systems and cross-memberspostweld heat treatment is typically not required. • Fuel pumps In many cases, properties in the as-cast condition approach • Brake valvesthose of higher-strength heat treated alloys. Castability is dis- • Armored cupolastinctly inferior, and full properties may not be realized for days, • Aerospace structural partsweeks, or longer periods of room-temperature hardening. Stabilitycan be an issue addressed by artiﬁcial aging or heat treatment REFERENCESwithout quenching. Alloys of this type include selected Al-Mg, Al-Zn-Mg, and Al- 1. Aluminum Standards & Data, The Aluminum Association,Zn-Mg-Cu alloys such as 535.0, 712.0, 771.0, and 772.0. Washington, DC (updated periodically), and American Na- Typical applications include: tional Standards Institute ANSI H35.1 2. Metals and Alloys in the Uniﬁed Numbering System, 9th ed.,• Tooling plate SAE and ASTM, 2001• Complex thin-walled shapes such as impellers and cooling fans 3. J. Datta, Ed., Aluminium Schlüssel: Key to Aluminium Alloys,• Explosion-proof enclosures 6th ed., Aluminium Verlag, Düsseldorf, Germany, 2002• Electrical ﬁttings 4. “American National Standard Nomenclature System for Alu-• Brazed parts minum Metal Matrix Composite Materials,” ANSI H35.5-• Machinery 2000, The Aluminum Association, May 25, 2000• Instrument cases 5. E.L. Rooy, Aluminum Scrap Recycling and Its Impact on the• Marine components Metal Castings Industry, AFS Trans., 1985, p 179• Pistol frames• Food and beverage processing SELECTED REFERENCES• Decorative parts• Reﬂectors • Alcoa Alloys for Use in Induction Motor Rotors, The Aluminum• Optical systems Company of America, 1974 • Aluminum Alloys, Canadian Institute of Mining and Metallurgy,2.6.5 Bearings 1986, p 249 • Aluminum Brazing Handbook, The Aluminum Association, Aluminum-tin alloys 850.0, 851.0, 852.0, and 853.0 are spe- 1990cialized compositions displaying excellent bearing characteristics • J. Frick, Ed., Woldman’s Engineering Alloys, 9th ed., ASMunder moderate loads and with effective lubrication. Castability, International, 2000hardness, compressive yield strength, and other properties are in- • D.A. Granger, W.G. Truckner, and E.L. Rooy, Aluminum Al-ﬂuenced by alloy variations involving silicon and copper additions. loys for Elevated Temperature Application, AFS Trans., 1986 The principal applications for these alloys are bushings and bear- • Handbook of International Alloy Compositions and Designa-ings. tions, Vol III, Metals and Ceramics Information Center, 1980 • M. Holt and K. Bogardus, The “Hot” Aluminum Alloys, Prod.2.6.6 High-Strength Alloys Eng., Aug 1965 • H.Y. Hunsicker, Aluminum Alloy Bearings—Metallurgy, De- High-strength alloys include compositions designed to provide sign and Service Characteristics, Sleeve Bearing Materials,high strength and ductility and in the case of premium engineered American Society for Metals, 1949castings also imply high levels of internal soundness and micro- • W.F. Powers, Automotive Materials in the 21st Century, Adv.structural reﬁnement. Alloys considered premium strength by deﬁ- Mater. Proc., May 2000nition and speciﬁcation (AMS-A-21180) are A201.0, A206.0, 224.0, • Registration Record of Aluminum Association Alloy Designa-249.0, 354.0, A through D356.0, A through D357.0, 358.0, and tions and Composition Limits for Aluminum Alloys in the Form359.0. Other alloys displaying high strength are 204.0, 206.0, of Castings and Ingot, The Aluminum AssociationC355.0, and metal-matrix composite compositions. • E. Rooy, Summary of Technical Information on Hypereutectic Applications include: Al-Si Alloys, AFS Trans., 1968 • E.L. Rooy, The Metallurgy of Rotors, Society of Die Casting Engineers, 1986• Missile bodies • J. Tirpak, “Elevated Temperature Properties of Cast Aluminum• Missile ﬁns Alloys A201-T7 and A357-T6,” AFWAL-TR-85-4114, Air• Aircraft pylons Force Wright Aeronautical Laboratories, 1985• Aircraft canopies • K.R. Van Horn, Ed., Fabrication and Finishing, Vol 3, Alu-• Wing ﬂaps minum, American Society for Metals, 1967• Speed brakes • D.B. Wood, Solid Aluminum Bearings, Prod. Eng., 1960• Hatch covers • Worldwide Guide to Equivalent Nonferrous Metals and Alloys,• Hydraulic pumps 4th ed., ASM International, 2001
22 / Aluminum Alloy Castings: Properties, Processes, and Applicationscharacteristics also vary as a function of cooling rates and solidi- before wear, heat checking caused by thermal fatigue, or otherﬁcation conditions imposed by differing casting processes. An alloy conditions that affect their acceptability for continued production.selection imposed by speciﬁed requirements and metallurgical con- Sections 3.4 and 3.5 describe casting technologies under ex-siderations often dictates the casting process. pendable and nonexpendable mold processes.3.2.3 Volume of Production 3.3.2 Pressure versus Gravity The number of castings that are estimated to be required is a A second important factor in categorization of aluminum castingmajor factor in the choice of casting method. Loose or simple processes is whether molten metal ﬂows by gravity into the die orpatterns may be used for sand cast prototypes or when only one or mold cavity or is forced under pressure. Casting by injection undera few parts are required. When production is limited, tooling cost pressure requires nonexpendable dies and is commonly referred todominates. For larger production volumes, tooling costs, though as pressure die casting. Countergravity processes that employ low-signiﬁcant, become less important. As volume requirements in- pressure differentials such as low pressure, displacement, or pumpedcrease, the trend is toward automated molding processes, perma- systems for mold ﬁlling are considered variations of either ex-nent molds, and die casting. For extended production in die and pendable or gravity permanent mold processes.permanent mold operations, more expensive, difficult-to-machine 3.3.3 Gating and Riseringtool steels provide improved life. Recent developments for reduc-ing tooling costs include near-net-shape forming of dies, composite There is a commonality in practices and terminologies for gravitydie materials, the deposition of hard, wear-resistant die surfaces, casting in both expendable and nonexpendable molds. Molten metaland in situ bonding of dissimilar materials by laser and high- is normally introduced to the mold cavity in an arrangement re-intensity infrared technologies. ferred to as the gating system (Fig. 3.1, 3.2). It consists of a pouring basin leading to a downsprue through which molten metal is de-3.2.4 Costs livered to the parting plane of the mold. From the base of the Costs are strongly inﬂuenced by process choice. Tooling costs downsprue, metal is conveyed along the casting periphery in run-associated with die and permanent mold casting are justiﬁed by ners that supply metal to in-gates from which metal enters thehigher levels of production and product reproducibility. The use of casting cavity. Risers—volumes of heat and pressure-differentiatedhigh-speed molding machines in volume sand casting improvesproduction rates with increased capital and maintenance costs.Low-volume investment castings require precise patterns, handmold assembly, and pouring practices that are justiﬁed by theextreme detail, accuracy, and ﬁnish of the ﬁnal product. Premiumengineered castings are typically low volume and high cost. Whentwo or more casting processes are capable of satisfying part re-quirements, selection is dictated by unit cost.3.2.5 Quality Quality factors are also important in the selection of the castingprocess. Quality refers to the degree of internal soundness and tothe mechanical properties and performance characteristics that area reﬂection of alloy chemistry, molten-metal quality, solidiﬁcationconditions, microstructural features, and soundness. The casting Fig. 3.1 Typical sand mold gating. Source: Ref 1process dictates solidiﬁcation conditions and, to a large extent,variations in microstructural features and soundness. The selectedcasting process must be competent to deliver the required level ofquality.3.3 Casting Process Technology3.3.1 Expendable and Nonexpendable Mold Processes Casting processes for aluminum may be categorized as involvingexpendable or nonexpendable molds. In sand casting, for example,the mold is destroyed when the casting is produced. Similarly,plaster and investment castings are made in molds that cannot bereused. Permanent molds and dies are reused, although each hasﬁnite life based on the number of castings that can be produced Fig. 3.2 Typical permanent mold gating. Source: Ref 2
Chapter 3: Aluminum Casting Processes / 23molten metal—are strategically located external to the mold cavity 3.4 Expendable Mold Gravity-Feedto compensate for volumetric shrinkage as solidiﬁcation of the Casting Process and Its Variationscasting progresses. The gating system is comprehensively designedto minimize turbulence and prevent aspiration. 3.4.1 Sand Casting Pressure die castings are ﬁlled through runners and in-gates, but Green and Dry Sand. Sand casting involves the forming of arisers are not normally used because solidiﬁcation rate limits their geometrically dimensioned impression in sand. The process in-effectiveness (Fig. 3.3). Instead, internal soundness is promoted by cludes green sand and dry sand casting. Green sand refers to thedie design features, elaborate mold cooling, and pressure intensi- use of uncured bonding systems, usually a blended mixture of sand,ﬁcation during the shot cycle. clay, and water. In the dry sand process, resins, oil, or other chemi- Most sand castings are produced in molds with a horizontal cal binding agents are used to precoat the molding sand. The dryparting plane, while the parting plane in most permanent mold sand mold is then thermally or chemically cured. Another dry sandcasting is vertically oriented. Pressure die castings are produced method reacts carbon dioxide (CO2) gas with sodium silicate in thewith both horizontal and vertical parting-plane orientation. In hori- sand blend to form a silica gel bond.zontally parted molds, the upper mold half is referred to as the cope, The important parameters of molding sand are compressiveand the lower, the drag. strength and permeability. Tests for each are routinely performedFig. 3.3 Typical die casting gating. Source: Ref 3
24 / Aluminum Alloy Castings: Properties, Processes, and Applicationsfor quality assurance. The mold must have sufficient strength to If the casting contains internal passages or undercuts, dry sandmaintain its shape through the casting process and sufficient per- cores may be used. In these cases, the mold includes locating pointsmeability to permit the air, and gases formed during pouring, to and additional impressions or prints for precisely positioning theevacuate the mold cavity as the metal enters. Compressive strength cores after pattern removal and before ﬁnal mold assembly. In rareand permeability in green sand are functions of sand particle size cases, aluminum chaplets may be used to support the core position.and shape, moisture and binder contents, and the degree of com- Molten metal is poured into the mold, and after it has solidiﬁed,paction applied in forming the mold. the mold is physically removed from the casting. Removal is by The advantages of typical sand casting are versatility in a wide physical means including vibration.variety of alloys, shapes, and sizes. Alloys considered hot short Casting quality is determined to a large extent by foundry tech-because of cracking tendencies during solidiﬁcation are more eas- nique. Proper molten metal processing, metal-handling and gatingily cast in green sand since molds offer reduced resistance to di- design and practices including the selective use of chills are nec-mensional contraction during solidiﬁcation. Lower mold strength essary for obtaining sound castings. Complex castings with varyingis also advantageous for parts with widely varying section thick- section thicknesses will be sound only if proper techniques arenesses and intricate designs. These advantages are diminished in used.chemically bonded molds, which display greater rigidity than green While the principles of sand casting are relatively simple, a largesand molds. number of process variations are in use that typically involve ex- There are only practical limitations in the size of the parts that pendable pattern materials and molding methods.can be cast. Minimum wall thickness is normally 0.15 in. (4 mm),but thicknesses as little as 0.090 in. (2 mm) can be achieved. 3.4.2 Evaporative (Lost-Foam) Pattern Casting (EPC) Among disadvantages are relatively low dimensional accuracy Lost foam is a sand casting process that uses an unbonded sandand poor surface ﬁnish; basic linear tolerances of Ϯ0.03 in./in. mold with an expendable polystyrene pattern. This process is some-(Ϯ30 mm/m) with a minimum tolerance of 0.020 in./in. (20 mm/ what similar to investment casting in that an expendable pattern ism), and surface ﬁnishes of 250 to 500 μin. (6 to 13 μm) root mean used to create the mold cavity. Unlike investment casting, thesquare (rms). Chemically bonded sands offer improved surface pattern vaporizes during the pouring of molten metal rather thanﬁnish and dimensional accuracy, and relatively unlimited shelf life, before pouring.depending on the type of binder used. Achievable dimensional The EPC process employs a foamed polystyrene pattern packedtolerances can be substantially improved using precision methods in unbonded sand. The polystyrene model is coated with a thin layerin the forming and assembly of dry sand mold components. Surface of ceramic or refractory wash that seals the pattern surface. Thequality can be improved by using a ﬁner grade of facing sand in pattern is sequentially decomposed by the heat of the molten metal,the molding process. thus replacing the foam pattern and duplicating the features of the Strength is typically lower as a result of slow solidiﬁcation rates. pattern in the solidiﬁed casting. Use of the process has increasedMechanical properties are improved by using sands such as zircon rapidly, especially in large-volume automotive foundries, and manyand olivine with higher heat capacity than silica and by the use of casting facilities are now dedicated to the production of castingscopper, iron, or steel chills at strategic locations in the mold. by this method (Fig. 3.4). Sand casting involves minimum tooling and equipment cost when The major difference between sand castings and castings madesmaller numbers of castings are to be produced. by the EPC process is the extent of subsequent machining and Sand Molding. In both green and dry sand processes, the mold cleaning operations required. Evaporative pattern castings are con-is formed by compacting the preconditioned sand over the pattern.In ﬂoor or hand molding, the sand is compacted using manual orpneumatic rams; for pattern plates (match plates), machines usejolt/squeeze mechanisms to ensure mold integrity. Automatic mold-ing machines provide a high degree of uniformity and very highmold production rates. Patterns may consist of wood, composite, or metal plates con-taining the casting impression or may consist of loose pieces as-sembled in the form to be cast. After compaction of the moldingsand, the pattern is carefully removed, leaving a cavity in the shapeof the casting to be made. A dusting of calcium carbonate or otherparting compound on the pattern surface is helpful in facilitatingthe separation of the pattern from the mold. A small amount ofvibration through transducers attached to the match plate also fa-cilitates pattern removal. The runners and in-gates are usually integral to the pattern, butmay also be manually cut into the sand by the molder. A patternof the sprue is separately placed on the pattern before sand is Fig. 3.4 Typical castings produced by the evaporative pattern casting (EPC)introduced. process
Chapter 3: Aluminum Casting Processes / 25sistently poured at closer tolerances with less stock for grinding, and dimensional accuracy and cool at slightly higher rates; how-machining, and ﬁnishing. Dimensional variability associated with ever, equipment and production costs are higher, and the size andcore setting and the mating of cope and drag are eliminated. The complexity of castings that can be produced are limited.use of untreated, unbonded sand simpliﬁes sand processing, han-dling, and reclamation. Casting cleaning is also greatly reduced andcan often be eliminated because of the absence of ﬂash, sand 3.4.4 Plaster Castingadherence, and resin stains. Further beneﬁts of the EPC process In this method, either a permeable (aerated) or impermeableresult from the freedom in part design offered by the process. plaster is used for the mold. The plaster in slurry form is pouredAssembled patterns can be used to make castings that cannot be around a pattern. When the plaster has set, the pattern is removedproduced by any other high-production process. and the plaster mold is baked to remove free water and reduce waters of hydration. The high insulating value of the plaster allows castings with thin walls to be poured. Minimum wall thickness of3.4.3 Shell Mold Casting aluminum plaster casting is typically 0.060 in. (1.5 mm). Plaster In shell mold casting, molten metal is poured into a shell of molds have high reproducibility, permitting castings to be maderesin-bonded sand only 0.4 to 0.8 in. (10 to 20 mm) thick. The mold with ﬁne details and close tolerances; basic linear tolerances ofis formed by introducing the chemically coated sand to a heated Ϯ0.005 in./in. (Ϯ5 mm/m) are typical. The surface ﬁnish of plasterpattern that thermally cures the bond. By controlling the core mold castings is excellent; aluminum castings attain ﬁnishes of 50 to 125temperature and cycle, the depth of cure can be controlled to the μin. (1.3 to 3.2 μm) rms.desired thickness. Cured mold sections are removed and assembled For complex shapes, such as some precision impellers and elec-for pouring, usually backed by unbonded or green sand (Fig. 3.5). tronic parts, mold patterns made of rubber are used because theirShell mold castings surpass ordinary sand castings in surface ﬁnish ﬂexibility makes them easier to withdraw from the molds than rigid patterns. Intricate plaster castings may also be produced using polystyrene or other expendable pattern materials such as those used in investment casting. Mechanical properties and casting quality depend on alloy com- position and foundry technique. Slow cooling due to the highly insulating nature of plaster molds magniﬁes solidiﬁcation-related problems such as hydrogen pore formation and shrinkage voids and reduces strength and ductility. For many plaster cast parts, there are only limited capabilities for improving internal soundness and properties through traditional gating and risering approaches. The conﬁguration of impellers and other rotating parts subject to strict dimensional requirements as well as strengths compatible with high rotational stresses permits the use of extensive chilling of the shaft and base for purposes of improving internal soundness and mechanical property perfor- mance. These techniques are further enhanced when combined with nonturbulent mold ﬁlling by low-pressure or other counter- gravity methods. Figure 3.6 shows plaster cast alloy 224.0 impel- lers that were produced through a low-pressure method. 3.4.5 Investment Casting Investment casting of aluminum most commonly employs ce- ramic molds and expendable patterns of wax, plastic, or other low-temperature melting materials. In the ceramic shell method, assembled patterns are invested in a ceramic slurry by repetitive immersion and air drying until the desired shell thickness has been formed. In the solid mold investment method, the assembled pat- tern is immersed in a container of sufficient size for ceramic slurry to encase and set around the pattern. In either case, the mold is placed in an autoclave to remove the pattern and then ﬁred at high temperature to remove all free water and organic materials and to cure the binding system being used. Molds are typically preheated and poured under partial vacuum. Christmas-tree gating systemsFig. 3.5 Shell molds assembled before pouring. Source: Ref 1 are employed to produce small multiple parts in one mold.
26 / Aluminum Alloy Castings: Properties, Processes, and Applications Aluminum investment castings can have walls as thin as 0.015 strength range can be achieved with molten metal treatments, gating,to 0.030 in. (0.40 to 0.75 mm), basic linear tolerances of Ϯ5 mils/in. and solidiﬁcation conditions that are not typical for conventional(Ϯ5 mm/m) and surface ﬁnishes of 60 to 90 μin. (1.5 to 2.3 μm). investment castings. Because of porosity and slow solidiﬁcation, the mechanical prop- Investment casting applications include: instrument parts, im-erties of many aluminum investment castings are typically lower pellers, compressor vanes, gears, ratchets, pawls, scrolls, speedthan those demonstrated by other casting processes. The interest of brakes, wing tips, and aircraft pylons.the aerospace and other industries in the combination of accuratedimensional control with controlled mechanical properties has re- 3.4.6 Vacuum Mold (V-Mold) Castingsulted in the use of improved technologies to produce premium- A heated plastic ﬁlm is drawn over the pattern by vacuum.quality castings by investment methods. Castings in the premium- Unbonded sand is ﬁlled against the plastic-covered pattern within a vented ﬂask and compacted by vibration. A vacuum is drawn through the ﬂask after an unheated plastic ﬁlm is placed over the back of the mold, creating a mold vacuum package. Pouring takes place with the vacuum retained or reapplied (Fig. 3.7). Advantages are surface ﬁnish, minimum wall thickness, and reduced draft requirements. Disadvantages are tooling costs and size limitations imposed by maximum ﬂask dimensions. 3.5 Nonexpendable (Permanent) Mold Gravity Feed Casting Process and Its Variations 3.5.1 Permanent Mold Casting In principle, permanent mold casting is analogous to expendable mold casting processes. In this case the molds are machined cast, wrought or nodular iron, cast steel, or wrought steel and can be reused repetitively until damage, wear, or the effects of thermal fatigue necessitate repair or replacement (Fig. 3.8). The ability to form internal passages involves metallic or sand cores. Intricate details and undercuts can often be cast using segmented steel cores.Fig. 3.6 Alloy 224.0 impellers produced by low-pressure plaster casting Sand cores become necessary when the design prohibits drawing the core after the casting has solidiﬁed. When sand cores are used, the process is referred to as “semipermanent mold” casting. Permanent mold tooling is typically more expensive than that required for sand casting and other expendable mold processes and is justiﬁed by the volume of production. The volume of production also dictates the extent of process automation. Molds can be manu- ally operated or extensively automated. Production rates of auto- mated multimold operations are high, and parts display consistent dimensional characteristics and properties. While the principles and mechanics of gravity casting are similar, the metallurgical structure of permanent mold castings reﬂects the reﬁnement of higher solidiﬁcation rates. Typical and speciﬁed mini- mum mechanical properties including ductility are higher than those of expendable mold castings. The improved mechanical prop- erties of permanent mold castings provide part of the justiﬁcation for selecting this process over competing gravity casting options. The same terminologies used in expendable mold gating apply. There is a downsprue into which molten metal is introduced from a pouring basin, from which the metal ﬂows into runners, risers, in-feeds, and casting cavity. Directional solidiﬁcation is promoted by selective chilling of mold sectors by air, mist, or water. An insulating coating is used to protect the mold from the molten aluminum and to facilitate removal of the casting from the mold after solidiﬁcation is complete. Typical mold dressings or washesFig. 3.7 Vacuum molding unit. Source: Ref 1 are suspensions of talc, various metal oxides such as zirconia,
Chapter 3: Aluminum Casting Processes / 27chromia, iron oxide and titania, colloidal graphite and calcium 3.5.2 Low-Pressure Die Casting (LP),carbonate in water, and sodium silicate. The thickness and thermal Pressure Riserless Casting (PRC)characteristics of these coatings are used to locally increase or In this process, permanent molds are mounted over a sealeddecrease heat absorption during solidiﬁcation. As a result of wear, furnace. A tube extends from the mold cavity into the molten metalthese coatings must be periodically repaired or replaced to ensure below. By pressurizing the furnace, metal is forced through the tubeconsistent process performance and casting results. Mold surfaces into the mold cavity (Fig. 3.9). When the metal has solidiﬁed, theare periodically blasted with dry ice or mild abrasives to remove pressure is relieved, the mold is opened, and the casting is removedcoatings and scale after which new mold coatings are applied. in preparation for repeating the cycle. The permanent mold process is less alloy tolerant than most Most low-pressure casting has been conﬁned to radially sym-expendable mold processes. The most popular permanent mold metrical designs, but a wide range of nonsymmetrical parts havealloys display superior castability such as those of the Al-Si, Al- also been produced. Nearly all automotive wheels are cast by thisSi-Mg, and Al-Si-Cu (Mg) families. Mold rigidity is a challenge process (Fig. 3.10, 3.11).in the casting of hot-short alloys in which liquidus-solidus range Process parameters include (a) the rate at which pressure isand elevated-temperature strength combine to increase the ten- applied, which regulates mold ﬁlling, (b) pressure, which is rela-dency for cracking during and after solidiﬁcation. Determined ef- tively unimportant once solidiﬁcation begins, and (c) thermal gra-forts to cast even the most difficult foundry alloys such as low-iron dients, which are essential for establishing directional solidiﬁca-aluminum-copper alloys have nevertheless been successful, and tion. As in conventional permanent mold, these gradients arealloys with limited castability are routinely cast in permanent molds. established by the selection and controlled thicknesses of mold Permanent mold castings can be produced in sizes ranging from coatings and by selective chilling of mold sections. Since mostless than a pound to more than several hundred pounds. Surface low-pressure castings are produced using only one metal entryﬁnish typically varies 150 to 400 μin. (3.8 to 10 μm). Basic linear point and since risers normally necessary to avoid internal shrink-tolerances of about Ϯ0.01 in./in. (Ϯ10 mm/m), and minimum wall age voids are not typically used, the gross-to-net weight ratio is lowthicknesses are about 0.100 in. (2.5 mm). and trimming and ﬁnishing operations associated with gating are minimized. The low-pressure casting cycle is dictated by the solidiﬁcation of metal at the junction of the ﬁll-tube and mold cavity. While countergravity metal ﬂow into the mold cavity is quies- cent, the process does present the risk of inclusion contamination. When the mold is opened and the casting is removed, the vacuum seal that existed at the liquid-solid interface is broken and molten metal remaining in the tube falls to the furnace metal level. The cycling of metal ﬂow vertically in the ﬁll tube can result in the buildup of oxides on the inner surfaces of the ﬁll tube whether theFig. 3.8 Permanent mold machined from steel. Source: Ref 1 Fig. 3.9 Low-pressure permanent mold. Source: Ref 1
28 / Aluminum Alloy Castings: Properties, Processes, and Applicationstube is ceramic or coated metal. To minimize this condition, back nating the casting. Filtration may consist of steel screens, ceramicpressure can be maintained in the system so that molten metal is strainers, or fused or foamed porous ceramics.retained at an elevated level in the ﬁll tube at all times. It is alsopossible to replenish metal in the furnace with each cycle by valv- 3.5.3 Vacuum Riserless Casting (VRC)ing rather than periodically reﬁlling when the metal in the furnaceis nearly depleted. Filtration of metal at the point of entry into the The use of vacuum rather than pressure to introduce molten metalmold is routinely used to prevent included matter from contami- into steel dies has signiﬁcant advantages over low-pressure casting. The molten metal bath is open and accessible. Molten metal level can be maintained within a narrow range in close proximity to the mold entry point so that the vertical dimension between the metal surface and the mold cavity can be minimized. Limitations are in the size and cost of molds that can be engi- neered to apply and retain vacuum pressures. A high degree of mold chilling has been used to enhance met- allurgical structures, improve mechanical properties, and shorten cycle times. The VRC process is ideally suited for automation and high production rates to produce castings with exceptional surface quality and metallurgical properties. Examples of VRC products are shown in Fig. 3.12. 3.5.4 Centrifugal Casting Centrifugal force in aluminum casting involves rotating a mold or a number of molds ﬁlled with molten metal about an axis. Cylindrical or tubular shapes may be centrifugally formed in ver- tically or horizontally rotated drums, while conventional castings are produced by the rotation of one or more molds about a vertical axis. Metal may be introduced before or during rotation. Baked sand, plaster, or graphite molds have been used, but iron and steel dies are most common. Centrifugal castings are generally, but not always, denser than conventionally poured castings and offer the advantage of greater detail. Wheels, wheel hubs, motor rotors, and papermaking and printing rolls are examples of aluminum parts produced by centrifugal cast- ing. Aluminum alloys suitable for permanent mold, sand, or plasterFig. 3.10 Alloy A356.0 alloy automotive wheels produced by low-pressure casting can be cast centrifugally. castingFig. 3.11 Variety of parts, including automotive pistons, metallurgically bonded diesel engine pistons, compressor pistons, cylindrical and Fig. 3.12 Examples of castings produced by the vacuum riserless castingjournal bearings, anodes, and cookware, produced by the low-pressure casting (VRC) process include rocker arms, compressor pistons, connect-process ing rods, trowel handles, valve components, and other parts
Chapter 3: Aluminum Casting Processes / 293.5.5 Squeeze Casting A number of alternative approaches to the production of the Although a number of process developments have been referred semisolid raw material have been or are being developed. A processto as squeeze casting, the process by which molten metal solidiﬁes in which particle ingots are continuously fed and mechanicallyunder pressure within closed dies positioned between the plates of stirred to provide the required semisolid state and microstructurea hydraulic press is the only version of current commercial interest. has been developed and used in magnesium alloy casting produc-The applied pressure and retained contact of the metal with the die tion. The incompatibility of materials of containment with suffi-surface improves heat transfer and inhibits hydrogen precipitation cient strength for this process in molten aluminum remains to beand shrinkage void formation. The result is a denser, ﬁne-grained overcome. Attempts to eliminate expensive thin-cast billet throughcasting with excellent mechanical properties. slurry approaches in mold ﬁlling have also been undertaken. Squeeze casting has been successfully used for a variety of Semisolid forming is more costly than conventional casting, butferrous and nonferrous alloys in traditionally cast and wrought offers unique properties and consistently excellent quality. In ad-compositions. Applications of squeeze-cast aluminum alloys in- dition, the viscous nature of semisolid alloys provides a naturalclude reciprocating engine pistons, brake rotors, automotive and environment for the incorporation of third-phase particles in thetruck wheels, and structural automotive frame components (Fig. preparation of reinforced metal-matrix composites.3.13). Squeeze casting is simple and economical, is efficient in its Specialized billets are commercially available, and semisolid-use of raw material, and has excellent potential for automated formed applications are broadening in the aerospace, automotive,operation at high rates of production. military, and industrial sectors. The process represents an alterna- tive to conventional forgings, permanent mold, investment and die castings, impact extrusions, machined extrusion proﬁles, and screw3.5.6 Semisolid Forming machine products. Applications include automotive wheels, master Semisolid forming incorporates elements of casting, forging, and brake cylinders, antilock brake valves, disk brake calipers, powerextrusion. It involves the near-net-shape forming of metal parts steering pump housings, power steering pinion valve housings,from a semisolid raw material that incorporates a uniquely non- compressor housings, steering column parts, airbag containmentdendritic microstructure. housings, power brake proportioning valves, electrical connectors, Mechanical or electromagnetic force is employed during billet and various covers and housings that require pressure tightness.solidiﬁcation to fragment the solidifying structure. The result is aspherulitic structure that behaves thixotropically in the liquidus-solidus range. The billet retains its shape at closely controlled 3.6 Pressure Die Casting and Its Variationstemperatures above the melting point at which the shear strengthis low, even at relatively high percent fraction solid. When the billet The production of aluminum alloy castings by the die castinghas been reheated, it is forced into dies under pressure to form a process exceeds that of all other processes. It is ideally suited forcasting that retains the characteristics of the starting billet micro- high production rate and volume production of dimensionally ac-structure. Just as important, the mold cavity is ﬁlled without the curate parts with excellent surface ﬁnish. One of the importantturbulence associated with gravity pouring or the injection of mol-ten metal, and internal porosity formation is minimized by reducingthe volume of liquid metal that solidiﬁes from the semisolid con-dition (Fig. 3.14).Fig. 3.13 Automotive parts produced by the squeeze casting process. Cour- tesy of UBE Industries Fig. 3.14 Semisolid formed alloy A357.0 landing gear component
30 / Aluminum Alloy Castings: Properties, Processes, and Applicationsreasons for the success of die castings has been the development Rapid ﬁlling of the mold (20 to 100 μs) and rapid solidiﬁcationof high-speed precision equipment. Another is the extension of die under pressure combine to produce a consistently dense, ﬁne-casting technologies to larger castings with heavier wall thick- grained and highly reﬁned surface structure with excellent prop-nesses. erties including fatigue strength. Internal unsoundness affects bulk In pressure die casting, molten metal is injected under pressure properties, the acceptability of machined surfaces, and pressureinto water-cooled dies. Pressure is maintained until the part has tightness. Impregnation is routine for die castings that must containsolidiﬁed. Molten metal usually enters the mold by the action of gases or liquids under substantial pressure. Internal unsoundnessa hydraulic ram in a containment chamber (shot chamber), result- generally prevents full heat treatment and welding because of theing in rapid ﬁlling of the mold cavity. While lubrication is required risk of blister formation when die castings are exposed to elevatedto facilitate the separation of the casting from the die surface, the temperatures. Lower-temperature thermal treatments for stabiliza-dies are otherwise uninsulated. Dies are usually machined from tion or hardening are routinely used. In special cases and in re-high-quality tool steels. stricted casting areas, limited welding can also be performed. The die casting process has undergone signiﬁcant changes The die casting process is least alloy tolerant of important com-through the evolution of machine design and instrumentation as mercial casting processes. Solidiﬁcation conditions require alloyswell as process development and controls. The demand for larger, of superior castability and that display good resistance to crackingmore complex castings with improved quality and lower cost has at elevated temperatures. The highly castable alloys of the alumi-led to the development and promotion of specialized die casting num-silicon family are the most common. Of these, alloy 380.0 andmachines capable of higher rates of production and improved per- its variations comprise about 85% of total die casting production.formance. These compositions provide attractive combinations of cost, Die casting machines vary in type, size, and capacity. strength, hardness, and corrosion resistance in the as-cast state, There are two basic concepts, hot and cold chamber operation. with excellent ﬂuidity and resistance to hot cracking. Aluminum-In the hot chamber process, the shot chamber and piston are im- silicon alloys lower in copper, such as 360.0, 364.0, 413.0, andmersed in molten metal. Metals such as magnesium and zinc that 443.0, offer improved corrosion resistance and excellent castabil-do not aggressively attack the materials of construction can be ity.efficiently cast by this method with production rate advantages. Hypereutectic aluminum-silicon alloys including 390.0 have be-Despite intensive efforts to develop hot chamber process designs come more important in wear-resistant applications.and materials that could be used in aluminum casting, none have Magnesium content is usually controlled at low levels to mini-been commercially successful. Except in rare cases, all aluminum mize oxidation and the generation of oxides in the casting process.die casting is performed in cold chamber equipment in which the Most commonly used die casting alloys specify restrictive mag-shot chamber is ﬁlled with each cycle, and the chamber and piston nesium limits. Nevertheless, aluminum-magnesium alloys can beassembly are not continuously in contact with molten aluminum. die cast. Alloy 518.0, for example, is speciﬁed when the highest Die casting machine designs are also differentiated by parting corrosion resistance and the brightest, most reﬂective ﬁnish areplane orientation. In practice, the dies are mounted on platens that required.can operate in either vertical or horizontal directions. Early die Iron contents of 0.7% or greater are preferred to maximize el-casting was typically performed with vertical die movement. To- evated-temperature strength, to facilitate ejection, and to minimizeday, with exceptions, vertical die casting is restricted to rotor pro- soldering to the die face. Iron content is usually 1 Ϯ 0.3%, butduction. greater concentrations are also used. Improved ductility through Locking pressure deﬁnes the capacity of the machine to contain reduced iron content has been an incentive resulting in widespreadthe pressure generated during the injection cycle. The larger the efforts to develop a tolerance for iron as low as approximatelyplan area of the casting and the greater the hydraulic pressure 0.25%. These efforts focus on process reﬁnements, design modi-applied, the greater the required locking pressure. Die casting ma- ﬁcations, and improved die lubrication. At higher iron concentra-chines are designed with locking pressures from as little as 25 tions, there is a risk of exceeding solubility limits of coarse Al-tonnes to more than 4500 tonnes corresponding to injection pres- Fe-Cr-Mn segregate at molten metal temperatures. Sludging orsures of up to 40 ksi (280 MPa). precipitation of segregate is prevented by chemistry controls re- The principles of directional solidiﬁcation and gravity-based lated to metal temperature. A common rule is:gating and risering are essentially inapplicable to die casting. Gatesand runners are used to convey metal from the shot chamber to the Fe ϩ 2(Mn) ϩ 3(Cr) Յ 1.7die cavity. Geometrical considerations are observed to minimizeturbulence, air entrapment, and fragmentation of the metal stream,but no effort other than the use of sustained pressure is used to where element values are expressed in weight percent.promote internal soundness. Techniques are used to intensify pres- Die casting is especially suited to production of large quantitiessure during the solidiﬁcation phase to decrease the volume fraction of relatively small parts. Typical aluminum die castings weigh fromof internal porosity. With metal velocities exceeding 100 ft/s (30 a few ounces to more than 100 lb (50 kg).m/s) and solidiﬁcation rates exceeding 1800 ºF/s (1000 ºC/s), the Close tolerances and excellent surface ﬁnishes are characteristic.greatest quality concern is entrapped gases including combustion Aluminum alloys can be die cast to tolerances of Ϯ4 mils/in.or volatilization components of the lubricant and turbulence- (Ϯ0.004 in./in.) and commonly have ﬁnishes as ﬁne as 50 μin. (1.3related inclusions. μm). Parts are cast with walls as thin as 0.040 in. (1.0 mm). Cores,
Chapter 3: Aluminum Casting Processes / 31which are made of metal, are restricted to simple shapes that permit duce the tendency for microshrinkage and cracking during solidi-drawing or removal after solidiﬁcation is complete. ﬁcation. Because unalloyed aluminum can be purchased at lower cost3.6.1 Acurad Die Casting Process than rotor alloys, there has been a trend for their substitution in An acronym for accurate, rapid, and dense, the Acurad process rotor production. For example, P1020 unalloyed smelter ingot hasclaimed a degree of directional solidiﬁcation from thermal analy- the same purity as 170.2 but without impurity ratio controls andsis, die cooling and gating design, modulated lower metal injection with uncontrolled titanium and vanadium content. Ignoring thesevelocities, and intensiﬁed injection pressures during solidiﬁcation differences results in variable electrical performance and poor cast-through the use of a secondary plunger. In effect, Acurad represents ings.a compromise between die casting and permanent mold principles. Minimum and typical conductivities for each grade are:3.6.2 High-Integrity Pressure Die Casting Conductivity, %IACS Alloy Minimum Typical The combination of optimal die casting practices marries met- 100.1 54 56allurgical and mechanical capabilities to provide quality levels 150.1 57 59exceeding those of conventional die casting. Solid-state lubricants 170.1 59 60are used in place of volatile die lubricants. Dies, lubricants, andejector systems are designed to facilitate casting removal at re- Rotor alloy 100.0 with larger concentrations of iron and otherduced iron levels. The die cavity is evacuated before injection. impurities displays superior die casting characteristics. With higherMolten metal processing to reduce dissolved hydrogen and en- iron content, crack resistance is improved and there is a lowertrained nonmetallics approximates that used for gravity casting. tendency for internal shrinkage. This alloy is recommended whenMolten metal handling and the transfer of molten metal to the shot the maximum dimension of the part is greater than 5 in. (125 mm).chamber are nonturbulent, and the injection sequence is adjusted For the same reasons, alloy 150.0 offers castability advantagesto promote nonturbulent die ﬁlling. Large, thin-wall automotive over alloy 170.0.structures and other high-quality die castings are being produced For rotors requiring high resistivity for higher starting torque,that display strength, ductility, and toughness that cannot be conventional die casting or other highly alloyed compositions areachieved in other die casting processes. With improved internal used. The most common are 443.2 and A380.2. By choosing alloysquality, high-integrity die castings can be welded and heat treated, such as these, conductivities from 25 to 35% IACS can be obtained.although some limitations still apply. Experimental rotor alloys have been developed with conductivities as low as 18% IACS.3.6.3 Pore-Free Pressure Die Casting Although gross casting defects may adversely affect electrical In the “pore-free” process, the die cavity is purged with oxygen performance, the conductivity of alloys employed in rotor manu-before metal injection. The oxygen reacts with molten aluminum facture is almost exclusively controlled by composition. Simpleto form oxides that inﬂuence ﬂuid ﬂow and by being chemically calculation using these values accurately predicts total resistivityconsumed reduces the tendency for entrapment as gas pores. The and its reciprocal, conductivity, for any composition. An easy-to-oxides are concentrated in the casting surface after solidiﬁcation so use formula for conductivity that offers sufficient accuracy for mostthat inclusion effects on properties are minimized. purposes is:3.6.4 Vacuum Die Casting Conductivity, %IACS ϭ 63.50 – 6.9(Fe ϩ Si) – 83(Ti ϩ V ϩ Mn ϩ Cr) The application of a partial vacuum to the die cavity evacuatesair and volatilized lubricant from the mold before and during metal where element values are expressed in weight percent.injection. Vacuum die casting reduces the tendency for air entrap- More accurate calculations may be made from the elementalment resulting from rapid and turbulent die ﬁlling. The improve- resistivities given in Table 8.4, in Chapter 8.ment in soundness results in degrees of acceptability for weldingand heat treatment. 3.7 Premium Engineered Castings3.6.5 Rotor Casting Most cast aluminum motor rotors are produced in specialized A premium engineered casting is one that provides higher levelscompositions by smaller vertical die casting machines. The ob- of quality and reliability than found in conventionally producedjective is consistent electrical performance. Alloys 100.0, 150.0, castings. Premium engineering includes intimately detailed designand 170.0 (99.0, 99.5, and 99.7% Al, respectively) specify impurity and control of each step in the manufacturing sequence. The resultslimits and ratios for the formation of intermetallics least harmful are minimally variable premium strength, ductility, soundness, di-to castability and limit the concentrations of peritectic elements mensional control, and ﬁnish. Castings of this classiﬁcation aremost detrimental to electrical conductivity. Titanium and vanadium notable primarily for mechanical property performance that reﬂectsare precipitated or complexed by boron additions. Iron and silicon extreme soundness, ﬁne dendrite-arm spacing, and well-reﬁnedcontents are controlled with the objective of promoting ␣Al-Fe-Si grain structure.formation that is less detrimental to castability. These impurity Premium engineered casting objectives require the use of chemi-controls improve and minimize variations in conductivity and re- cal compositions competent to display superior properties. Alloys
32 / Aluminum Alloy Castings: Properties, Processes, and Applicationsconsidered to be premium-strength compositions are listed in speci- procurement and nondestructive evaluation speciﬁcations and stan-ﬁcation AMS-A-21180, which is extensively used in the United dards.States for premium casting procurement. They include A201.0, Trial and error in alloy development gradually gave way to moreA206.0, 224.0, 249.0, 354.0, C355.0, A356.0, A357.0, D357.0, systematic construction based on experience and the predictable358.0, and 359.0. interrelationship of elements in soluble and insoluble phase for- Premium engineered aluminum castings represent the culmina- mation under differing solidiﬁcation conditions.tion of decades of research and development involving molten The principles of directional solidiﬁcation are easily grasped, butmetal treatment, methods for the removal of included matter, mea- their translation to practice for complex cast parts remains prob-surement or assessment of dissolved hydrogen, gating develop- lematic. There are nevertheless excellent simulation models andment, microstructural modiﬁcation and reﬁnement, casting pro- programs for predicting static and dynamic solidiﬁcation patternscesses, mold materials, and the development of high-strength, for speciﬁc part designs.ductile alloys. Each of these developments was necessary to ad-vance casting capabilities to meet an increasingly challenging range 3.7.4 Solidiﬁcation Rateof application requirements. The marriage of superior technologies The relationship of properties and dendrite arm spacing has sig-in all phases of casting design and production was essential for niﬁcantly inﬂuenced the premium engineered casting effort. So-meeting the most difficult of these challenges. The incentive was lidiﬁcation rate not only improves tensile properties, but also dra-the cost-effective replacement of more expensive wrought product matically improves ductility. Exploiting this relationship withassemblies by competent monolithic cast structures. appropriate alloys moved engineered aluminum castings away from the image of brittleness and damage intolerance that historically3.7.1 Melt Processing characterized design engineers’ perceptions. The principles of sparging for the removal of dissolved hydrogen 3.7.5 Mold Materialshad been developed in the late 1920s and 1930s. The use of activegases such as chlorine and the physicochemical separation of en- Investment casting produced small parts in which dimensionaltrained oxides and other nonmetallics by ﬂuxing became known in accuracy and surface ﬁnish were important criteria. Plaster moldsthe 1930s. The use of diffusers for more efficient gas ﬂuxing was were used in the production of dimensionally accurate cast partsdeveloped later. such as impellers and tire molds. There were corollary pattern, By 1950, particulate ﬁltration and countercurrent ﬂuxing using mold material, and mold processing developments. Differences innitrogen, argon, chlorine, and combinations of these gases became the molding and heat extraction characteristics of differing sandscommon for wrought alloy production, and variations of these were measured, and at the same time supplier developments in dryprocesses were being used in gravity casting foundries. sand binders were studied and evaluated. The later development of rotary degasing systems was quickly In permanent mold, variations in mold wash chemistry and ap-adapted to foundry use. plication were used with air, mist, and water cooling to control solidiﬁcation. On occasion, copper and ceramic inserts were de-3.7.2 Melt Quality Assessment signed into the mold to promote solidiﬁcation directionality. The use of steel chills, contoured sections, and mold plates was normal To a large extent, melt quality has been assessed by variations in sand casting.of the Straube-Pfeiffer test in which the relationship of hydrogen The use of all available mold components from most insulatingsolubility and pressure was qualitatively measured. The absence of (foamed plaster) to most rapid heat extraction (water-cooled cop-entrained oxides was assessed by their inﬂuence on hydrogen pre- per) could be incorporated in mold designs to reproducibly altercipitation under reduced pressure. A semiquantitative approach solidiﬁcation in order to promote the highest possible degree ofusing sample densities was developed and used extensively as a internal soundness. Computer simulations of mold ﬁlling dynamicsprocess control tool (Ref 4). For greater sensitivity, controlled and solidiﬁcation that incorporate differences in heat extractionvibration during sample solidiﬁcation at absolute pressures of 0.04 through ﬁnite-element analysis are gradually supplanting art andto 0.10 psi (2 to 5 mm Hg) was employed. Real-time measurement instinct in process designs.of dissolved hydrogen by partial pressure diffusion in molten metal The result is a composite mold design of signiﬁcant complexitysupplemented vacuum test results. Validation of hydrogen assess- using dry sand and at least several other mold materials for eachments was provided by solid-state extraction techniques. conﬁguration.3.7.3 Solidiﬁcation 3.7.6 Alloys Academicians were largely responsible for improved mathemat- All alloys employed in premium casting engineering work areics-based understanding of solidiﬁcation behavior. The parameters characterized by optimal concentrations of hardening elements andof metallurgical structure that were controlled in the solidiﬁcation restrictively controlled impurities. Although any alloy can be pro-process were extensively studied. The relationships of dendrite arm duced in cast form with properties and soundness conforming tospacing and grain size and type on physical and mechanical prop- a general description of premium values relative to correspondingerties were established, and the inﬂuence of variations in soundness commercial limits, only those alloys demonstrating yield strength,caused by hydrogen porosity, shrinkage, and inclusions on strength tensile strength, and especially elongation in a premium rangeand ductility were broadly used in the development of new general belong in this grouping. They fall into two categories: high-strength
Chapter 3: Aluminum Casting Processes / 33aluminum-silicon alloys containing magnesium or magnesium and The extremely high strength and toughness capabilities of vari-copper, and alloys of the 2xx.0 series, which by restricting impurity ous typically 4.5% Cu alloys including 201.0, 204.0, 206.0, 224.0,element concentrations provide outstanding ductility, toughness, and 249.0 have their roots in 295.0 alloy, which dates from 1921and tensile properties with notably poorer castability. and in earlier European compositions. Most were introduced or The minimum properties of premium-strength alloys might be appeared in reﬁned versions during the period from 1968 to 1974.considered 40 ksi (275 MPa) tensile strength, 30 ksi (205 MPa)yield strength, and 3.0% elongation. Much higher minima are rou-tinely speciﬁed. In all premium casting alloys, impurities are strictly limited forthe purposes of improving ductility. In aluminum-silicon alloys,iron is controlled at or below 0.010% with measurable advantagesin the range of 0.03 to 0.05%. Beryllium is present in A357.0 and358.0 alloys, not to inhibit oxidation although that is a corollarybeneﬁt, but to alter the form of the insoluble phase to a morenodular form less detrimental to ductility. Most of the compositions designated as premium engineeredalloys had their origins in the 1950s and early 1960s. Alloy A356.0,registered in 1955, and B356.0 in 1956 were derivatives of 356.0alloy which was originally developed in 1930. Similarly, alloyC355.0 dates from 1955, while the parent 355.0 was ﬁrst used in1930. Alloys 359.0 and 354.0 were developed in 1961. Alloy A357.0(1962) had its origins in Tens-50 alloy that was also ﬁrst registeredin 1961. Examples of premium engineering castings in alloysA357.0 or D357.0 are shown in Fig. 3.15 to 3.19. Fig. 3.16 Premium engineered casting helicopter rotor hub Fig. 3.17 Premium engineered casting aircraft pylonsFig. 3.15 One-piece alloy D357.0 main landing gear door uplock support for the 767 airplane. The casting replaced a sheet metal assembly;the conversion eliminated 27 separate parts and reduced assembly time by65%. Source: Ref 5 Fig. 3.18 Premium engineered casting aircraft wing ﬂap
34 / Aluminum Alloy Castings: Properties, Processes, and Applications3.7.7 Aluminum-Silicon Eutectic ladles, sprue/gate/runner ratios, runner overruns, dross traps, pour- Modiﬁcation and Grain Reﬁnement ing cup designs, strainers and screens, and nonvortexing cross- sectional geometry of downsprues and runners. The use of optimal The use of chemical modiﬁers in hypoeutectic aluminum-silicon gating designs and rigorously controlled practices are integral com-alloys has been the subject of ongoing research. Beneﬁcial effects ponents of premium casting technology.on solidiﬁcation, feeding, and properties are well established. Re- Several developments have altered mold-ﬁlling options; thesesearch has included the effects of a large number of elements and developments are described in the following paragraphs.element combinations on eutectic and phase structures. The most First, the low-pressure casting process achieved commercial im-potent modiﬁer, sodium, has been extensively used in all gravity portance in the United States in the 1950s. A number of challengescasting operations. The advantageous interaction of sodium and that were unaddressed by commercial low-pressure systems werestrontium was also recognized and became the basis for the use of successfully met. A cam-controlled back-pressure method based onboth elements in modiﬁcation additions. gross casting weight was used to retain residual metal levels at the For premium engineered castings, the artifacts of modiﬁer ad- top of the feed tube. This feature prevented the inclusion spawningditions—notably increased hydrogen solubility and the introduc- characteristic of normal low-pressure cycles. In-gate ﬁltration andtion of large amounts of hydrogen by alloying methods—made screening methods were also devised.eutectic modiﬁcation counterproductive for most premium engi- The range of part designs and alloys that were cast would beneered castings. Casting results for rapidly solidiﬁed unmodiﬁed considered unusual today when the low-pressure process has be-castings proved superior to those of chemically modiﬁed, less- come principally known for automotive wheel production. Instead,sound castings produced under the same conditions. the low-pressure method was considered a means of nonturbulent At one time, essentially uncontrolled titanium additions were mold ﬁlling with a number of additional advantages that includedroutinely made for grain reﬁnement. Extensive studies of the ratios reduced gross/net weight and lower pouring temperature. Someof titanium and boron and their intermetallic forms most effective examples were diesel engine and compressor pistons, air-for grain reﬁning resulted in rapid advances in foundry practice. conditioner compressor bodies, bearings, furniture parts, and mis-Later studies would provide new insights that continuously rede- sile ﬁns. Geometric symmetry, which is normally a criterion forﬁned the advanced standards and procedures for grain structure low-pressure production was not considered a prerequisite, andcontrol in premium engineered casting production. many of the castings that were produced used conventional risering3.7.8 Mold Filling rather than exclusively relying on the in-feed for shrinkage com- pensation. The inevitable degradation of melt quality that occurs in drawing These developments were adapted to premium engineered plas-and pouring through conventional methods was recognized as a ter and dry sand parts. High-speed rotors and impellers were ex-signiﬁcant barrier to achieving premium engineered quality levels cellent examples, but many other premium engineered casting con-and properties. Very signiﬁcant efforts had been made to evaluate ﬁgurations were made by low-pressure mold ﬁlling.different pouring and gating approaches. These included siphon Second, countergravity mold-ﬁlling methods were developed involving the use of mechanical or induction pumps. Third, various techniques have been developed and are in use for ﬁlling molds quiescently by displacement of molten metal. Fourth, solidiﬁcation time was not a signiﬁcant factor in ex- pendable mold production when extensive chilling was used, but it was always a factor in permanent mold. For this reason, and to overcome other low-pressure process limitations, vacuum riserless casting (VRC) was developed in the early 1960s. Rather than pressurize a contained molten reservoir, the application of a vacuum on the mold cavity drew metal from the bath through a short ﬁll tube. The metal source was exposed for periodic treatment, the distance from subsurface metal entry to the casting cavity was minimal, dies were extensively chilled, and the process could be highly automated. While only relatively small and simple shapes were produced by the VRC method, productivity and mechanical properties were exceptional. More than 20 million air-conditioner pistons and millions of rocker arms were produced by this process. Fifth, the level pour process for premium engineered castings was developed. This process had its origins in the direct chill process that was developed for fabricating ingot. It was natural that the shared concerns for metal distribution and solidiﬁcation prin- ciples would result in the synthesis of process concepts. Aluminum-tin alloy bearings, which were typically hollow orFig. 3.19 Premium engineered casting aircraft canopy solid cylinders, could be produced by the direct chill process, but
Chapter 3: Aluminum Casting Processes / 35segregation and safety concerns led to a variation in which metal From the applications standpoint, strength, ductility, and otherwas introduced to the bottom of a permanent mold through a mechanical attributes are only equal in importance to reliability.moving pouring cup that traversed the length of the mold. Qui- Variability in soundness and performance remains the greatest con-escent ﬂow and the continuous layering of molten metal provided cern in engineered structural applications for which castings com-improved internal quality. Excellent soundness was obtained with- pete. The processes and controls for narrowing material variationsout the use of the extensive risering normally required for these in premium engineered castings form part of the basis for aggres-long solidiﬁcation range alloys, pouring temperature was reduced, sive cooperative materials development programs in automotiveand the solidiﬁed structure was more chemically homogeneous and aerospace applications that emphasize process capabilitiesthan in conventionally cast parts. rather than reliance on nondestructive evaluation. No premium With determined engineering, the same approach was success- engineered castings foundry could survive the inspection losses iffully used for more complex conﬁgurations with more challenging the process was not capable of consistently meeting speciﬁed re-metallurgical requirements. The cost of doing so in permanent quirements. No commercial foundry can expect to remain com-mold was not typically justiﬁed. However, aircraft and aerospace petitive if the casting process cannot deliver consistent quality withparts in the limited quantities normally associated with sand casting minimum internal and external losses without reliance on expen-offered exciting opportunities for level pour technology, and a large sive and time-consuming nondestructive testing.number of prototype and production parts were produced by this The goal of reducing product variability and the consistentmethod. In its ﬁnal form, the assembled mold was lowered on a achievement of speciﬁed product characteristics through the se-hydraulic platform through a trough arrangement that provided lected use of processes and controls developed for premium en-nonturbulent ﬂow of metal through entry points that paralleled the gineered castings is within the range of capability for all aluminumvertical traverse of the mold. Metal ﬂow was controlled by the foundries and for the fullest range of casting types and speciﬁca-dimensions of the entries and the lowering rate, which could be tions.modulated for cross-sectional variations as a function of moldtravel. Characteristic of the direct chill process on which it wasbased, the level pour process features quiescent molten metal ﬂow, 3.8 Other Process Technologiesminimized feeding distances, and reduced pouring temperatures.3.7.9 Quality Assurance Other process technologies of importance for aluminum alloy castings that affect properties and performance are: The production of premium engineered castings involves ex-tensive nondestructive evaluation and certiﬁcation. Acceptance usu- • Metallurgical bondingally requires radiographic examination, ﬂuorescent penetrant in- • Metal-matrix composites (MMCs)spection, and dimensional veriﬁcation. Mechanical properties are • Hot isostatic pressureoften determined in destructive tests, usually involving machinedsubsize specimens taken from designated areas of randomly se-lected castings. 3.8.1 Metallurgical Bonding Practices developed for ﬁrst article qualiﬁcation must be me- It is possible to mechanically or metallurgically bond dissimilarticulously deﬁned, and speciﬁcation restrictions and requaliﬁcation metals in aluminum casting.procedures are imposed on changes or modiﬁcations. In some The Al-Fin Process results in a continuous metallurgical struc-cases, the practices must be disclosed and in others may remain ture from the insert through an intermetallic boundary to the baseproprietary. Conﬁrmation that practices have been observed may alloy of the casting. While inserts can be simply placed in the moldtake the form of furnace and heat treatment records, for example, before pouring to form a mechanical union between the two ma-by government and/or customer on-site inspectors. Another pos- terials, the union is dependent only on the intimacy of contact andsibility is that these records may become part of the certiﬁcation the force exerted by differences in thermal contraction character-process in which inspection records, mechanical property test re- istics. Copper, ferrous, and other alloy components such as cast-insults, and radiographic ﬁlm are submitted with the castings. cooling coils and piston wrist pin struts become integral to the cast The objective of premium engineered casting is the ultimate structure.development of material properties, consistency, and performance. By preimmersing inserts in molten aluminum so that an inter-The pioneering developments of these efforts have been continu- metallic layer is developed by chemical attack, the insert rapidlyously reﬁned, and today a number of foundries demonstrate the placed in the mold can be metallurgically rather than mechanicallyunique capabilities for meeting the exacting standards that are bonded to the cast aluminum structure.required. Compression ring groove inserts in diesel engine pistons and the bearing surfaces of rotating parts are often metallurgically bonded3.7.10 Relevance of Premium Casting Engineering to ensure structural integrity, strength, and heat transfer. Various Just as technologies developed in the space program have found iron grades, steel, and stainless steel elements have been success-applications in industry, premium engineered casting develop- fully and routinely bonded to aluminum casting structures. Highments have important implications for all aluminum foundries. The nickel iron and steel offer advantages in the similarity of expansionprinciples and processes of premium casting can be cost effectively coefficients so that stresses through operating temperature rangesapplied to conventional aluminum casting production. are reduced.
36 / Aluminum Alloy Castings: Properties, Processes, and Applications Preimmersion baths of aluminum-silicon alloys provide uniform can be successfully used. Production parts have been cast in sand,thin intermetallic layers with minimal residual retention of bath permanent mold, pressure die, and investment processes.when inserts are transferred to the mold. Since iron is continuously Metal-matrix composites are also cast by impregnation of ﬁberdissolved, the bath must be periodically discarded or diluted to cake in gravity and squeeze casting processes. Impregnated castprevent the deposition of iron containing insoluble phases on the composites begin with a permeable ceramic cake formed to com-insert surface. prise a section of the casting to be reinforced. The cake is intruded Because the insert must be positioned, the mold closed and to obtain the composite structure.poured before the aluminum residual to the insert surface solidiﬁes, Recent alternative developments involving matrix reinforcementbonding is typically performed in permanent molds. concepts include the investigation of postsolidiﬁcation surface treat- ments including ﬂame and plasma spray deposition, and high-3.8.2 Cast Aluminum-Matrix Composites intensity infrared and plasma heating of ceramic overlays. Typically, MMC scrap cannot be recovered except by separation Incorporating particles or ﬁbers of dissimilar materials in cast of the composite component.aluminum structures substantially alters material properties. Ce- Existing or emerging applications for cast aluminum compositesramics, graphite, alumina, silicon carbide, other carbides, and ni- are:trides wet by molten aluminum form a reinforced structure typi-cally displaying substantially increased modulus of elasticity, higher • Brake rotors (Fig. 3.20)strength, and improved wear resistance. While tensile strengths in • Cylinder liners (Fig. 3.21)excess of 100 ksi (700 MPa) can be achieved, the characteristic • Power-steering pulleysductility of composite structures is limited. • Connecting rods Powder metallurgy composites are commercially important, andthere is a growing technical capability and market for cast alumi-num metal-matrix composite parts. Cast composites offer cost-advantaged near-net-shape capabilities in sizes and conﬁgurationsnot achievable in powder metallurgy or by other forming methodswith the same advantages in exceptional speciﬁc stiffness (elasticmodulus-to-weight ratio), strength, wear resistance, and the optionof selectively reinforcing or altering local material properties. Most cast MMC parts are produced from prealloyed/mixed alloyin conventional casting processes. Mechanical or other forms ofagitation are employed to maintain the homogeneous suspensionof particulate after melting. The segregation of density-differen-tiated particles in aluminum is strongly inﬂuenced by particle sizeand time. If the dispersion can be maintained through melting,holding, and mold ﬁlling, more rapid solidiﬁcation characterized Fig. 3.20 Alloy 359/SiC/20p metal-matrix composite brake rotor. Source:by permanent mold and die casting promotes the more uniform Ref 6distribution of particles in the solidiﬁed structure. Recent developments concern increasingly ﬁne particle sizes tonanodimensions and shapes such as ﬁbrules and microspheres,which will result in a reduced tendency for density segregationbefore and during solidiﬁcation. Finer particulate distribution hasalso shown improvements in ductile behavior while preservingadvantages in stiffness and strength. Another notable developmentinvolves the use of low-cost particulate such as represented byindustrial waste materials such as ﬂy ash to produce low-density,property-enhanced parts with reduced material costs. The most important castable aluminum-base MMC composi-tions originate in conventional alloys to which from 10 to 20 vol%particulate silicon carbide (SiC), alumina, or other ceramic materialhas been added. Particle wetting and distribution are functions ofingot production or of procedures used during melting and blend-ing. Composite ingots are remelted, uniform dispersion of par-ticulate is mechanically or inductively ensured, and casting is ac-complished using conventional foundry practices and equipment.The ﬂuidity and ﬂow characteristics of composite alloys are notsigniﬁcantly different from those of conventional unreinforced al- Fig. 3.21 Metal-matrix composite (MMC) cylinder liners. The MMC offers an alternative to cast iron or hypereutectic aluminum-silicon alloyloys so that mold designs and gating systems of routine production for this application.
Chapter 3: Aluminum Casting Processes / 37• Bicycle frames • G. Bouse and M. Behrendt, Metallurgical and Mechanical Prop-• Scraper blades and shoes erty Characterization of Premium Quality Vacuum Investment• Sporting equipment Cast 200 and 300 Series Aluminum Alloys, Adv. Cast. Technol.,• Golf club heads Nov 1986• Aerospace optical systems • Computer Gating Program, SDCE • Core and Mold Process Control, American Foundrymen’s So-• Electronic/avionic thermal management components ciety, 1977• Pressure vessels • A.K. Dahle, S.M. Nabulski, and D.H. St. John, Thermome-• Brackets chanical Basis for Understanding Hot Tearing During Solidi-• Wave guides ﬁcation, AFS Trans., Vol 106, 1998 • Fundamental Molding Sand Technology, American Foundry-3.8.3 Hot Isostatic Pressing (HIP) men’s Society, 1973 The application of hot isostatic pressing (HIP) to aluminum • J.C. Hebeisen, HIP Casting Densiﬁcation, ASME, 1999alloys following casting is a key technology for improving prop- • E.A. Herman, Die Casting Handbook, Society of Die Casting Engineers, 1982erties by reducing or eliminating the effects of porosity and in- • W. Hunt, Jr., Metal Matrix Composites, Chapter 6.05, Com-clusions. This technology is sufficiently important that it is covered prehensive Composite Materials, Pergamon Press, July 2000in a separate chapter (Chapter 6), following the discussion of the • W.H. Hunt and D.R. Herling, Applications of Aluminum Metalnature and cause of such imperfections. Matrix Composites: Past, Present, and Future, Proc. Interna- tional Symposium of Aluminum Applications: Thrusts and Chal-REFERENCES lenges, Present and Future, Oct 2003 (Pittsburgh, PA), ASM International1. Principles of Purchasing Castings, American Foundry Society, • H. Koch and A.J. Franke, Ductile Pressure Die Castings for 2002 Automotive Applications, Automotive Alloys, TMS, 19972. Gating and Feeding for Light Metal Castings, American Found- • S.J. Mashl et al., “Hot Isostatic Pressing of A356 and 380/383 rymen’s Society, 1946 Aluminum Alloys: An Evaluation of Porosity, Fatigue Prop- erties and Processing Costs,” SAE, 20003. Aluminum Casting Technology, American Foundrymen’s So- • Plaster Mold Handbook, American Foundrymen’s Society, ciety, 1993 19844. E.L. Rooy, Hydrogen in Aluminum, AFS Trans., 1993 • H. Pokorny and P. Thukkaram, Gating Die Casting Dies, So-5. Aluminum Now, The Aluminum Association Inc. ciety of Die Casting Engineers, 19846. Engineered Casting Solutions, American Foundry Society • E. Rooy, Improved Casting Properties and Integrity with Hot Isostatic Processing, Mod. Cast., Dec 1983SELECTED REFERENCES • E.L. Rooy, Origins and Evolution of Premium Engineered Alu- minum Castings, MPI Symposium on Premium Engineered• Basic Principles of Gating, American Foundrymen’s Society, Castings, May 2002 1967 • A.C. Street, The Die Casting Book, Portcullis Press Ltd., 1977• Basic Principles of Risering, American Foundrymen’s Society, • M. Tiryakioglu et al., Review of Reliable Processes for Alu- ˘ 1968 minum Aerospace Castings, AFS Trans., Vol 104, 1996
40 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsThe larger the dendrite arm spacing, the coarser the microcon- compositions are by comparison detrimental to mechanical prop-stituents and the more pronounced their effects on properties. Finer erties. The type and size of grains formed are functions of alloydendrite arm spacing is desirable for improved mechanical prop- composition, solidiﬁcation rate, and the concentration of effectiveerty performance (Fig. 4.2, 4.3) (Ref 2). grain nucleation sites. Cooling rates directly control dendrite arm spacing, which in- Increased solidiﬁcation rate reduces grain size (Ref 4), but so-ﬂuences property development and substantially improves ductil- lidiﬁcation rates in complex cast structures typically vary and theity: degree of grain reﬁnement practically achievable in commercial gravity casting processes is lower than that obtained by effective Cooling rate Dendrite arm spacing heterogeneous nucleation through grain-reﬁner additions beforeCasting processes °F/s °C/s mils μm casting (Fig. 4.4).Plaster, investment 1.80 1 3.94–39.4 100–1000Green sand, shell 18.0 10 1.97–19.7 50–500 All aluminum alloys can be made to solidify with a fully equi-Permanent mold 180.0 100 1.18–2.76 30–70 axed, ﬁne-grain structure through the use of suitable grain-reﬁningDie 1800 1000 0.20–0.59 5–15 additions (Ref 5, 6). The most widely used are master alloys of titanium or of titanium and boron. Aluminum-titanium reﬁners generally contain from 3 to 10% Ti. The same range of titanium4.3 Grain Reﬁnement concentrations is used in Al-Ti-B reﬁners with boron contents from 0.2 to 1% and titanium-to-boron ratios ranging from 5 to 50. Se- Fine, equiaxed grains are desired for the best combination of lected carbides also serve grain-reﬁning purposes in aluminumstrength and ductility by maximizing grain-boundary surface area alloys (Ref 7).and more ﬁnely distributing grain-boundary constituents (Ref 3). Although grain reﬁners of these types can be considered con-Coarse grain structure and columnar and feather or twin-columnar ventional hardeners or master alloys, they differ from true mastergrains that form with high thermal gradients in low-alloy-content alloys added to the melt exclusively for alloying purposes. To be effective, grain reﬁners must introduce controlled, predictable, and operative quantities of aluminides and borides or carbides in the correct form, size, and distribution for grain nucleation. Reﬁners in rod form, developed for the continuous treatment of aluminum in primary operations and displaying clean, ﬁne, unagglomerated microstructures, are available in sheared lengths for foundry use. In addition to grain-reﬁning master alloys in waffle or rolled rod form, salts, usually in compacted form that react with molten alu- minum to form combinations of TiAl3 and TiB2, are also available. Transduced ultrasonic energy has been shown to provide degrees of grain reﬁnement under laboratory conditions (Ref 8, 9). No commercial use of this technology has been demonstrated. The application of this method to engineered castings is problematic. 4.4 Aluminum-Silicon Eutectic Modiﬁcation The properties of hypoeutectic aluminum-silicon alloys can be affected by modifying the form of the eutectic. A ﬁner, more ﬁbrous eutectic structure can be obtained by increased solidiﬁcation rate and by the addition of chemical modiﬁers. Calcium, sodium, stron- tium, and antimony are known to inﬂuence the degree of eutectic modiﬁcation that can be achieved during solidiﬁcation. Figure 4.5 illustrates variations in degree of modiﬁcation achieved by modi- ﬁer additions. Sodium is arguably the most potent modiﬁer, but its effects are transient because of oxidation and vapor pressure losses. Strontium is less transient but may be less effective for modiﬁcation under slow solidiﬁcation rates (Fig. 4.6). The combination of sodium and strontium offers advantages in initial effectiveness. Calcium is a weak modiﬁer with little com- mercial value. Antimony provides a sustained effect, although the result is a ﬁner lamellar rather than ﬁbrous eutectic. The effects ofFig. 4.2 Dendrite cell size effects on the strength and elongation of several sodium, strontium, and Na ϩ Sr on modiﬁcation are shown in Fig. aluminum casting alloys. Source: Ref 1 4.6 and 4.7.
Chapter 4: The Effects of Microstructure on Properties / 41 The addition of metallic sodium to molten aluminum creates with minimum melt degradation, strontium is associated with anturbulence that can result in increased hydrogen and entrained increased tendency for hydrogen porosity, either through increas-oxide levels. The use of hygroscopic salts including NaCl and NaF ing hydrogen solubility or decreased surface tension.for modiﬁcation also risks oxide formation and increased dissolved The greatest beneﬁts of eutectic aluminum-silicon modiﬁcationhydrogen content. Postaddition ﬂuxing to restore melt quality in- are achieved in alloys containing from 5% Si to the eutectic con-creases the rate of sodium losses. The excessive use of sodium centration. The addition of modifying elements to these alloys(>0.01 wt%) increases misrun tendencies through increases in sur- results in a ﬁner lamellar or ﬁbrous eutectic structure. The modi-face tension and diminished ﬂuidity. fying additions either suppress the growth of silicon crystals within Strontium additions are usually made through master alloys con- the eutectic or equilibrate silicon-matrix growth rates, providingtaining up to 10% of the modiﬁer. While these additions are made ﬁner lamellae.Fig. 4.3 Correlation between dendrite cell size and tensile properties of specimens machined from production castings in alloy A356.0-T62. The different data points indicate specimens from different heats. Source: Ref 1Fig. 4.4 As-cast Al-7Si ingots showing the effects of grain reﬁnement. (a) No grain reﬁner. (b) Grain reﬁned. Both etched using Poulton’s etch; both 2ϫ. Courtesy of W.G. Lidman, KB Alloys Inc.
42 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsFig. 4.5 Variations in degrees and types of aluminum-silicon eutectic modiﬁcation. (a) Class 1, fully unmodiﬁed structure. 200ϫ. (b) Same as (a) but at 800ϫ. (c) Class 2, lamellar structure. 200ϫ. (d) Same as (c) but at 800ϫ. (e) Class 3, partial modiﬁcation. 200ϫ. (f) Same as (e) but at 800ϫ. (g) Class 4,absence of lamellar structure. 200ϫ. (h) Same as (g) but at 800ϫ. (i) Class 5, ﬁbrous silicon eutectic. 200ϫ. (j) Same as (i) but at 800ϫ. (k) Class 6, very ﬁnestructure. 200ϫ. (l) Same as (k) but at 800ϫ. Source: Ref 10
Chapter 4: The Effects of Microstructure on Properties / 43Fig. 4.5 (continued) (g) Class 4, absence of lamellar structure. 200ϫ. (h) Same as (g) but at 800ϫ. (i) Class 5, ﬁbrous silicon eutectic. 200ϫ. (j) Same as (i) but at 800ϫ. (k) Class 6, very ﬁne structure. 200ϫ. (l) Same as (k) but at 800ϫ. Source: Ref 10
44 / Aluminum Alloy Castings: Properties, Processes, and Applications Phosphorus interferes with the modiﬁcation mechanism. It reacts Thermal analysis is useful in assessing the degree of modiﬁcationto form phosphides that nullify the effectiveness of modiﬁer ad- that can be displayed by the melt (Ref 11). A sample of metalditions. It is therefore desirable to use low-phosphorus metal whenmodiﬁcation is a process objective and to make larger modiﬁeradditions to compensate for phosphorus-related losses. Typically, modiﬁed structures display higher tensile propertiesand appreciably improved ductility when compared to unmodiﬁedstructures (Table 4.1). Property improvement is dependent on thedegree to which porosity associated with the addition of modiﬁersis suppressed. Improved casting results include improved feedingand superior resistance to elevated-temperature cracking. Fig. 4.7 Varying degrees of aluminum-silicon eutectic modiﬁcation rangingFig. 4.6 Effectiveness of sodium and strontium modiﬁers as a function of from unmodiﬁed (A) to well modiﬁed (F). See Fig. 4.6 for the ef- time. See Fig. 4.7 for degrees of modiﬁcation fectiveness of various modiﬁersTable 4.1 Typical mechanical properties of modiﬁed and unmodiﬁed cast aluminum alloys Tensile yield Ultimate tensileAlloy and Modiﬁcation strength strength Elongation,temper Product treatment ksi MPa ksi MPa %13% Si Sand cast test bars None ... ... 18.0 124 2.0 Na-modiﬁed ... ... 28.0 193 13.0 Permanent mold test bars None ... ... 28.0 193 3.6 Na-modiﬁed ... ... 32.0 221 8.0359.0 Permanent mold test bars None ... ... 26.1 180 5.5 0.07% Sr ... ... 30.5 210 12.0356.0-T6 Sand cast test bars None 30.1 208 41.9 289 2.0 0.07% Sr 34.5 238 42.5 293 3.0 Bars cut from chilled sand casting None 30.9 213 41.2 284 4.4 0.07% Sr 31.6 218 42.2 291 7.2A356.0-T6 Sand cast test bars None 26.0 179 40.0 226 4.8 0.01% Sr 30.0 207 43.0 297 8.0A444.0-T4 Permanent mold test bars None ... ... 21.9 151 24.0 0.07% Sr ... ... 21.6 149 30.0A413.2 Sand cast test bars None 16.3 112 19.8 137 1.8 0.005–0.05% Sr 15.6 108 23.0 159 8.4 Permanent mold test bars None 18.1 125 24.4 168 6.0 0.005–0.08% Sr 18.1 125 27.7 191 12.0 Test bar cut from auto wheel 0.05% Sr 17.5 121 28.0 193 10.6 0.06% Sr 18.2 126 28.0 193 12.8Source: Ref 4
Chapter 4: The Effects of Microstructure on Properties / 45is cooled slowly, permitting time and temperature to be plotted Practices recommended for melt reﬁnement are:(Fig. 4.8). The effectiveness of modiﬁcation treatment is deﬁned bythe degree and duration of undercooling at the solidus. Test results • Melting and holding temperature should be minimum.must be correlated with the degree of modiﬁcation established • Calcium and sodium contents should be controlled to low con-metallographically for the castings since cooling rate for the sample centration levels.will differ. • Brief nitrogen or argon ﬂuxing after the addition of phosphorus is recommended to remove the hydrogen introduced during the addition and to distribute the aluminum phosphide nuclei uni-4.5 Reﬁnement of Hypereutectic formly in the melt. Aluminum-Silicon Alloys The elimination of large, coarse primary silicon crystals that areharmful in the casting and machining of hypereutectic silicon alloycompositions is a function of primary silicon reﬁnement (Ref 13).Phosphorus added to molten alloys containing more than the eu-tectic concentration of silicon, made in the form of metallic phos-phorus or phosphorus-containing compounds such as phosphor-copper and phosphorus pentachloride, has a marked effect on thedistribution and form of the primary silicon phase (Fig. 4.9). Re-tained concentrations of phosphorus as low as 0.0015% are ef-fective in achieving reﬁnement of the primary phase. Reﬁnement resulting from phosphorus additions can be expectedto be less transient than the effects of eutectic modiﬁcation inhypoeutectic alloys. Phosphorus-treated melts can be solidiﬁed andremelted without loss of reﬁnement. Primary silicon particle sizeincreases gradually with time as phosphorus concentration de-creases. Gas ﬂuxing accelerates phosphorus loss when chlorine orother reactive gases are used. Brief inert gas ﬂuxing is frequentlyemployed to reactivate aluminum phosphide nuclei, presumably byresuspension.Fig. 4.8 Cooling curve of the eutectic region of an unmodiﬁed and modiﬁed aluminum-silicon casting alloy. Tmin, temperature at the minimumbefore the eutectic plateau; Tg, eutectic growth temperature; tmin, time at theminimum of the curve; tE, time corresponding to the beginning of the eutectic Fig. 4.9 Effect of phosphorus reﬁnement on the microstructure of a hyper-plateau; tﬁnish, time corresponding to the end of the eutectic plateau. Source: eutectic Al-22Si-1Ni-1Cu alloy. (a) Unreﬁned. (b) Phosphorus re-Ref 12 ﬁned. (c) Reﬁned and ﬂuxed. All 100ϫ
46 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsREFERENCES • J. Burke, M. Flemings, and A. Gorum, Solidiﬁcation Technol- ogy, Brook Hill Publishing, 1974 1. R. Spear and G. Gardner, Mod. Cast., May 1963 • J.C. Claudet and H.J. Huber, Effect of Solidiﬁcation Conditions 2. R. Spear and G. Gardner, Dendrite Cell Size, AFS Trans., 1963 on Tensile Properties and Microstructure of Hypoeutectic Al-Si 3. S. Avner, Introduction to Physical Metallurgy, McGraw-Hill, Casting Alloys, Giessereiforschung, Vol 38, 1986 1964 • P.B. Crosley and L.F. Mondolfo, The Modiﬁcation of Alumi- 4. Aluminum Casting Technology, 2nd ed., American Foundry- num-Silicon Alloys, Mod. Cast., March 1966 men’s Society, 1993 • A.K. Dahle, S.M. Nabulski, and D.H. St. John, A Thermome- chanical Basis for Understanding and Predicting Hot Tearing 5. L. Backerud and Y. Shao, Grain Reﬁning Mechanisms in Alu- During Solidiﬁcation, AFS Trans., Vol 106, 1998 minum as a Result of Additions of Titanium and Boron, Part • M.C. Flemings, Behavior of Metal in the Semisolid State, Met- I, Aluminium, Vol 67 (No. 7–8), July-Aug 1991, p 780–785 all. Trans. B, Vol 22B, 1991 6. L. Backerud, M. Johnsson, and P. Gustafson, Grain Reﬁning • J.E. Gruzleski et al., Hydrogen Measurement by Telegas in Mechanisms in Aluminium as a Result of Additions of Tita- Strontium Treated A356 Melts, AFS Casting Congress, Ameri- nium and Boron, Part II, Aluminium, Vol 67 (No. 9), Sept 1991, can Foundrymen’s Society, 1986 p 910–915 • M. Guzowski and G. Sigworth, Grain Reﬁning of Hypoeutectic 7. A. Banerji and W. Reif, Development of Al-Ti-C Grain Re- Al-Si Alloys, AFS Trans., 1985 ﬁners Containing TiC, Metall. Trans. A, Vol 17A (No. 12), Dec • M. Guzowski, G. Sigworth, and D. Sentner, The Role of Boron 1986, p 2127–2137 in the Grain Reﬁnement of Aluminum with Titanium, Metall. 8. G.I. Eskin, Ultrasonic Treatment of Molten Aluminum, Met- Trans. A, Vol 10A (No. 4), April 1987, p 603–619 • N. Handiak, J. Gruzleski, and D. Argo, Sodium, Strontium and allurgiya, 1988 Antimony Interactions During the Modiﬁcation of ASG03 9. G.I. Eskin, Inﬂuence of Cavitation Treatment of Melts on (A356) Alloys, AFS Trans., 1987 the Processes of Nucleation and Growth of Crystals during • E. Herman, Heat Flow in the Die Casting Process, Society of Solidiﬁcation of Ingots and Castings from Light Alloys, Die Casting Engineers, 1985 Ultrasonics Sonochemistry, Vol 1 (No. 1), March 1994, p • W. Kurz and E. Fisher, Fundamentals of Solidiﬁcation, Trans S59–S63 Tech Publications, 198610. “Modiﬁcation Rating System for Structure of Hypoeutectic • L.F. Mondolfo, Aluminum Alloys: Structures of Metals and Aluminum Silicon Casting Alloys,” KBI Aluminum Master Alloys, Butterworths, 1976 Alloys product literature, Cabot Corporation • K. Oswalt and M. Misra, Dendrite Arm Spacing, AFS Trans.,11. J. Charbonnier et al., Application of Thermal Analysis in the 1980 Foundry for Aluminum Alloys, Hommes Fonderie, Nov 1975, • K. Radhakrishna, S. Seshan, and M. Seshadri, Dendrite Arm Spacing and Mechanical Properties of Aluminum Alloy Cast- p 29–36 ings, Aluminum, Vol 38, 197912. N. Tenekedjiev and J.E. Gruzleski, Thermal Analysis of Stron- • G. Scott, D. Granger, and B. Cheney, Fracture Toughness and tium Treated Hypoeutectic and Eutectic Aluminum-Silicon Tensile Properties of Directionally Solidiﬁed Aluminum Casting Alloys, AFS Trans., 1991 Foundry Alloys, AFS Trans., 198713. E.L. Rooy, Summary of Technical Information on Hypereu- • M. Shamsuzzoha and L. Hogan, The Crystal Morphology of tectic Al-Si Alloys, AFS Trans., 1972 Fibrous Silicon in Strontium Modiﬁed Al-Si Eutectic, Philos. Mag., Vol 54, 1986SELECTED REFERENCES • G. Sigworth, Observations on the Reﬁnement of Hypereutectic Silicon Alloys, AFS Trans., 1982• A.C. Arruda and M. Prates, Solidiﬁcation Technology in the • Solidiﬁcation, American Society for Metals, 1971 Foundry and Cast House, The Metals Society, 1983 • Solidiﬁcation Characteristics of Aluminum Alloys, Skan Alu-• O. Atasoy, F. Yilmazaned, and R. Elliot, Growth Structures in minum, 1986 Aluminum Silicon Alloys, J. Cryst. Growth, Jan–Feb 1984 • N. Tenekedjiev, D. Argo, and J.E. Gruzleski, Sodium, Stron-• L. Backerud, G.Chai, and J. Tamminen, Solidiﬁcation Char- tium and Phosphorus Effects in Hypereutectic Al-Si Alloys, acteristics of Aluminum Alloys, American Foundrymen’s So- AFS Trans., 1989 ciety, 1990 • O. Vorrent, J. Evensen, and T. Pedersen, Microstructure and• S. Bercovici, Solidiﬁcation, Structure and Properties of Alu- Mechanical Properties of Al-Si (Mg) Casting Alloys, AFS minum Silicon Alloys, Giesserei, Vol 67, 1980 Trans., 1984• J.M. Boileau, J.W. Zindel, and J.E. Allison, The Effect of So- • C. Zheng, L. Yao, and Q. Zhang, Effects of Cooling Rate and lidiﬁcation Time on the Mechanical Properties in a Cast A356- Modiﬁer Concentrations on Modiﬁcation of Al-Si Eutectic Al- T6 Alloy, SAE, 1997 loys, Acta Metall., Vol 18, Dec 1982
48 / Aluminum Alloy Castings: Properties, Processes, and Applicationsis generally more harmful to casting properties. In isolated cases, cause of its relevance when negative relative pressures associatedhydrogen may be intentionally introduced and controlled in spe- with shrinkage develop in the solidifying structure.ciﬁc concentrations compatible with the application requirements Just as in the case of crystal formation, hydrogen precipitationof the casting in order to promote superﬁcial soundness. may occur as a result of heterogeneous or homogeneous nucleation. The following rules describe the tendency for hydrogen pore The most powerful nucleants for hydrogen precipitation are oxides,formation (Fig.5.2 to 5.5) (Ref 1): especially oxides that through turbulence in gating, pouring, melt handling, and treatment entrain air or gaseous phases. In the pres-• There is a critical or threshold hydrogen value for any com- position that must be exceeded for hydrogen porosity to occur.• Residual pore volume fraction for each alloy corresponds to hydrogen content above the threshold value.• Pore volume fraction and pore size decrease with decreased hydrogen content above the threshold value.• Hydrogen pore volume fraction and pore size decrease with increased cooling rate. The critical or threshold value of hydrogen concentration is alsodependent on pressure and on the number (n) and tortuosity (t) ofliquid paths that exist in a solidifying dendritic network. The higherthe product of these factors (nt), the higher the hydrogen threshold. The foundry industry has long used various forms of vacuumtesting of molten metal samples to determine acceptability of theprocessed melt for any casting application. The basis for this testis the relationship between hydrogen solubility and pressure. Sincehydrogen solubility is related directly to the square root of pressure,decreased pressure reduces hydrogen solubility, increasing the ten-dency for bubble formation in the sample. The results of the re-duced pressure test can then predict in relative terms the tendency Fig. 5.3 Relationship of hydrogen content to cooling rate in A356.0 forfor formation of hydrogen voids in the cast part at ambient pressure. different porosity fractions. fp, porosity fractionThe pressure/solubility relationship recurs in this discussion be- Fig. 5.4 Relationship of pore volume to cooling rate for different hydrogen contents in Al-4.7Mg alloy (similar to alloy 514.0). Hydrogen con- tent (cm3/100 g): 1, 0.31 (no grain reﬁner); 2, 0.31 (grain reﬁned); 3, 0.22 (grainFig. 5.2 Hydrogen content, pore size, and cooling rate relationships in Al-4Mg alloy reﬁned); 4, 0.18 (grain reﬁned); 5, 0.10 (grain reﬁned)
Chapter 5: The Inﬂuence and Control of Porosity and Inclusions in Aluminum Castings / 49ence of such nuclei, hydrogen precipitates readily at even relatively is absorbed and coincidentally is responsible for degradation of thelow dissolved hydrogen levels. In the absence of nucleating phases liquid melt after effective treatment for hydrogen removal. At anysuch as oxides and gaseous species, surface tension forces are time the protective oxide surface of the melt is disturbed, an in-generally strong enough that precipitation is suppressed at even crease in hydrogen content can be expected.relatively high dissolved hydrogen levels. When properly per- In magnesium-containing alloys, an amorphous magnesium ox-formed, the vacuum solidiﬁcation test discriminates between bubble ide forms that is more permeable or less protective to the diffusionformation by heterogeneous and homogeneous nucleation. The of hydrogen from the atmosphere to the melt. It follows that periodsdetermination is made by observing the sample as it cools and of high humidity increase the problems faced in dealing with hy-solidiﬁes: drogen contamination and its removal and that magnesium- containing alloys are more susceptible to hydrogen absorption than• Immediate bubble formation when vacuum is applied indicates others. that the melt is contaminated by oxides and contains an inde- Incompletely dried or cured furnace refractories and refractories terminate amount of hydrogen. used to line troughing results in hydrogen absorption.• Gas evolution appearing in the solidifying sample only during Dissolved hydrogen is present in some amount in alloyed remelt the last stages of solidiﬁcation indicates that oxides are not ingot and master alloys. present and that hydrogen is present at a relatively high con- Moisture contamination of ﬂuxes and hydrogen in gas ﬂuxes centration. increase hydrogen levels and, in the latter case, affects the efficiency• If no evolution of gas occurs, it may be assumed that the melt of hydrogen removal. is free of oxides and that hydrogen contained in liquid solution Moisture in any form: contamination on tools, ﬂux tubes, ingot, is below the threshold value for precipitation. scrap, metallurgical metals, grain reﬁners, and master alloys that may be added to the heat additively affect dissolved hydrogenSources of hydrogen contamination include: content up to the applicable solubility limit. Degassing by the use of inert or active gases reduces hydrogen• Atmosphere concentrations by diffusion into bubbles of the ﬂuxing gas corre-• Incompletely dried refractories sponding to the partial pressure of hydrogen in the ﬂuxing gas.• Remelt ingot, master alloys, metallurgical metals, and other Spinning-rotor techniques have been developed that provide more charge components intimate mixing, efficient gas-metal reactions, and shorter reaction• Fluxes times to achieve low hydrogen levels. The use of active ﬂuxing• Tools, ﬂux tubes, and ladles gases and ﬁltration removes oxides, permitting acceptable quality• Products of combustion (POCs) in gas-ﬁred furnaces castings to be produced from metal with higher hydrogen contents. Hydrogen can be introduced through the disassociation of mois-ture in the atmosphere and products of combustion in furnace 5.2 Shrinkage Porosityatmospheres allowing atomic hydrogen diffusion into the melt.Turbulence, whether in melt treatment or in pouring can rapidly For most metals, the transformation from the liquid to the solidaccelerate the rate at which hydrogen from atmospheric moisture state is accompanied by a decrease in volume. In aluminum alloys, the volumetric shrinkage that occurs during solidiﬁcation ranges from 3.5 to 8.5%. The tendency for the formation of shrinkage porosity is related to both the liquid/solid volume fraction at the time of ﬁnal solidiﬁcation and the solidiﬁcation temperature range of the alloy. Shrinkage occurs during solidiﬁcation as a result of volumetric differences between liquid and solid states. It is important to make a distinction between the differences in liquid and solid volume that are of greatest concern to foundry personnel and the contraction that takes place after solidiﬁcation as a result of solid-state con- traction that most concerns die design and patternmaking. A sphere of molten metal solidifying without risering is an easily understood example of the diverse ways in which shrinkage forms. Once the shell of the sphere has solidiﬁed and assumes sufficient strength to resist collapse, the continued process of cooling and solidiﬁcation results in substantial tensile stresses in the liquid pool since the shell is contracting at the low rate dictated by the solid-Fig. 5.5 Relationship of pore size to cooling rate for different hydrogen state coefficient of thermal contraction, and the volume occupied contents in alloy A356.0. Hydrogen content (cm3/100 g): 1, 0.25 by the liquid that is cooling and experiencing volume change as(no grain reﬁner); 2, 0.31 (grain reﬁned); 3, 0.25 (grain reﬁned); 4, 0.11 (grain additional solid is formed is contracting at a far greater rate. Whilereﬁned); 5, 0.31 (grain reﬁned and modiﬁed) the liquid struggles to maintain coherency, tensile forces ultimately
50 / Aluminum Alloy Castings: Properties, Processes, and Applicationsexceed surface tension forces associated with the liquid-solid in- In Al-Si-Cu alloys, rapid cooling leads to the distribution of voidsterface and a void will form (Fig. 5.6a). Alloying elements that in the grain boundaries, while slow cooling results in interden-contribute to elevated-temperature strength such as iron, copper, dritically distributed shrinkage. Shrinkage is much more likely toand nickel increase resistance to surface collapse, leading to con- be localized in a eutectic composition such as 443.0 or A444.0. Intained shrinkage voids. There are variations in which the solidiﬁed any case, voids ﬁrst begin to form at liquidus-solidus temperaturesshell lacks the integrity to resist the negative pressures developed corresponding to 65 to 75% solid.within the sphere. If the shell is coherent, but weak, localized In short solidiﬁcation range compositions such as 356.0 andcollapse of the shell occurs to compensate for the volumetric change 413.0, there is an improved opportunity for establishing directional(Fig. 5.6b). Alloys with short solidiﬁcation ranges often display this solidiﬁcation. Defects may take the form of extensive piping asform of shrinkage. If localized failure of the shell occurs, inter- opposed to distributed shrinkage porosity. These alloys may bedendritic liquid will drain gravimetrically into the liquid pool that characterized by a higher proportion of mass feeding relative toremains (Fig. 5.6c). The result is a “wormhole” or “sponge” shrink- interdendritic feeding and are therefore less susceptible, under rea-age defect visible from the casting surface. These void concen- sonable efforts to establish directional solidiﬁcation, to the forma-trations are often associated with cracks that form during and after tion of widely distributed shrinkage voids.solidiﬁcation. Alloys with wide solidiﬁcation ranges are prone to When good foundry practices are used in long solidiﬁcationthis form of shrinkage. range compositions such as some aluminum-copper and aluminum- In the case of a risered casting, the intention is to prevent shrink- magnesium alloys, solidiﬁcation distance loses its importance to aage formation by maintaining a path for ﬂuid ﬂow from the higher more general tendency for interdendritic shrinkage. These alloysheat mass and pressure of the riser to the encased liquid pool. are susceptible to extensive microporosity that results from the Shrinkage displacement takes place in three modes: higher proportion of feeding that takes place interdendritically. The severity of shrinkage is increased by geometrical complexity, vary-• Mass feeding ing section thickness, solidiﬁcation rate, alloy feeding character-• Interdendritic feeding istics, and by limitations in effective gating and risering practice• Solid feeding that fail to provide the gradients required for directional solidiﬁ- cation. Mass feeding is liquid displacement occurring in the absence of Shrinkage void fraction varies in proportion to the fourth root ofsubstantial resistance. In these cases, pressure at the solidiﬁcation the pressure, leading to the conclusion that increasing pressure hasinterface and pressure in the riser system are essentially equivalent. little effect on shrinkage unless extremely high pressures can bePressure drop develops as obstructions to the feeding path form. employed. The progressive development of a dendritic network and local- Improved modiﬁcation and reﬁnement of aluminum-silicon al-ized solidiﬁcation results in increased resistance to ﬂuid ﬂow until loys, improved grain reﬁnement, and reduced oxide contents allthe pressure at the solidiﬁcation front is reduced to zero, at which improve feedability and therefore reduce shrinkage severity.time a shrinkage void will form. Interdendritic feeding takes placein the interval between mass feeding and the point at which suf-ﬁcient resistance develops that liquid ﬂow through the solidifying 5.3 Inclusionsdendrite network no longer occurs. Solid feeding occurs when the incipient shrinkage void is ﬁlled Nonmetallic inclusions are a particular concern in cast alumi-by the collapse of surrounding solidiﬁed metal. num. Because of its reactivity, aluminum oxidizes readily in liquid Shrinkage may assume many forms. Distributed voids or mi- and solid states. Oxidation rate is greater at molten metal tem-croshrinkage are found between dendrite arms as a result of failure peratures and increases with temperature and time of exposure.during the last stages of interdendritic feeding. Centerline or piping Magnesium in aluminum alloys oxidizes and with time and tem-voids result from gross directional effects, when, for example, large perature reacts with oxygen and aluminum oxide to form spinel.fully contained liquid pools are isolated within the casting during Table 5.1 categorizes inclusion types typically encountered.solidiﬁcation. Many oxide forms display densities similar to that of molten aluminum and sizes that reduce the effectiveness of gravimetric separation. Also, most oxides are wet by molten aluminum, re- ducing the effectiveness of mechanical separation methods. Aluminum is also chemically aggressive and can react with com- pounds in refractory formulations or with the coatings used to protect crucibles, ladles, and tools resulting in the entrainment of exogenous nonmetallics. While the oxide that initially forms on the surface of molten aluminum is highly protective and self-limiting, any agitation or turbulence in the treatment and handling of molten aluminum in-Fig. 5.6 How shrinkage voids form in aluminum castings. (a) Initial void creases the risk of oxide entrainment and the immediate reforma- formation. (b) Collapse of shell increases void size. (c) “Wormhole” tion of additional oxides. Oxide concentration can increase whenformation with additional shrinkage alloying additions are stirred into the melt, when reactive elements
Chapter 5: The Inﬂuence and Control of Porosity and Inclusions in Aluminum Castings / 51and compounds are immersed, when metal is drawn for pouring, hard nodules or large complex shapes. Aluminum carbide andand when metal is poured and conducted by the gating system into aluminum nitride can be found in smelted aluminum, but are usu-the mold cavity. Induction melting is highly energy efficient and ally of size and concentration of no signiﬁcance in aluminumeffective for melting ﬁnes and poor-quality scrap, but electromag- castings. Refractory and other exogenous inclusions may be iden-netically induced eddy currents result in high levels of entrained tiﬁed by their appearance and composition.oxides. Inclusions, such as shrinkage and hydrogen porosity, reduce The prevention of inclusions is the product of equipment and properties by detracting from the effective cross-sectional areapractices that minimize oxidation, avoid entrainment, and effec- when stress is applied and by the concentration of stresses at thetively remove particulate by ﬂuxing reactions or ﬁltration. inclusion interface (Fig. 5.7). Degassing with inert (argon) or quasi-inert (nitrogen) gases areonly partially effective in the removal of included matter. Rotarydegassing improves inclusion-removal efficiency, but the use of 5.4 Combined Effects of Hydrogen,active ﬂuxing gases such as chlorine or other halogens is necessary Shrinkage, and Inclusionsto dewet included oxides, facilitating their separation by the sweep-ing action of the ﬂuxing gas. The use of appropriate solid ﬂuxes Hydrogen precipitation and shrinkage porosity formation arehas the same effect. usually considered separate and independent phenomena. There are Molten aluminum can be ﬁltered by various means with varying interactive mechanisms that affect both.effectiveness. Strainers, screens, steel wool, porous foam, and fused Small amounts of dissolved hydrogen signiﬁcantly increase poreceramics can be used in the gating system as long as the combi- size when shrinkage voids form. In this respect, the effects of gasnation of pore size, level of inclusion contamination, and surface and shrinkage on pore volume fraction can be considered additive.area does not excessively restrict metal ﬂow. Cake-mode ceramic Since shrinkage voids must by deﬁnition result in areas of re-and deep-bed ﬁlters are used in furnaces and crucibles. duced pressure relative to atmospheric, hydrogen solubility is re- The removal of oxides can be seen to suppress hydrogen pore duced in the surrounding liquid facilitating the precipitation offormation as shown in Table 5.2. hydrogen into the forming void. The important measures of these Inclusions occur as varying types with differing sizes and shapes. pores—morphology, pore density, pore size, and volume fractionAluminum oxides are of different crystallographic or amorphous of pores—are affected by hydrogen.forms as ﬁlms, ﬂakes, and agglomerated particles. Magnesium The conventional wisdom is that hydrogen voids are alwaysoxide is typically present as ﬁne particulate. Spinels can be small rounded, smooth surface defects, while shrinkage voids invariablyTable 5.1 Inclusion sources and types in aluminum alloy castingsClassiﬁcation Types observed Potential source(s)Nonmetallic exogenous Various refractory particles, Al4C3, etc. Refractory degradation, remelt ingot, refractory/metal reactionsNonmetallic in situ MgO, Al2O3 ﬁlms, clusters, and disperoids; Melting, alloying: metal transfer turbulence MgAl2O4 ﬁlms and clustersHomogeneous halide salts MgCl2-NaCl-CaCl2, etc. Poor separation of ﬂuxing reaction productsParticle/salt MgCl2-NaCl-CaCl2/MgO, etc. Salt generated during chlorine ﬂuxing of magnesium-containing alloys, ﬁlter and metal-handling system releasesTable 5.2 Effect of ﬁltration on vacuum density test results and hydrogen content 50 mm Hg vacuum gas test 5 mm Hg vacuum gas test Dissolved hydrogen content, density, g/cm3 density, g/cm3 mL/100 gTest No. Before ﬁltering After ﬁltering Before ﬁltering After ﬁltering Before ﬁltering After ﬁltering1 2.05 2.67 2.28 2.64 0.76 0.702 2.14 2.69 2.45 2.69 0.61 0.693 2.16 2.72 2.48 2.70 0.51 0.534 2.25 2.78 1.99 2.76 0.38 0.435 2.29 2.74 2.07 2.60 0.39 0.386 2.24 2.74 1.97 2.71 0.36 0.417 2.30 2.73 1.94 2.66 0.31 0.368 2.48 2.74 2.27 2.76 0.33 0.319 2.34 2.73 2.06 2.61 0.30 0.3510 2.37 2.73 1.99 2.74 0.30 0.3111 2.59 2.78 2.29 2.77 0.29 0.2712 2.58 2.76 2.47 2.76 0.28 0.2813 2.25 2.74 2.26 2.76 0.27 0.3114 2.50 2.76 2.13 2.77 0.27 0.2815 2.62 2.76 2.35 2.78 0.23 0.2616 2.53 2.73 2.34 2.73 0.28 0.2817 2.56 2.72 2.32 2.68 0.27 0.3218 2.19 2.76 2.16 2.76 0.19 0.19
52 / Aluminum Alloy Castings: Properties, Processes, and Applicationshave the characteristic crystalline, jagged appearance that charac- portant to consider the interaction rather than to attempt to correlateterizes the dendrite structure. However, hydrogen porosity can absolute hydrogen content with defect formation.conform to dendrite-arm regions, which give bubble formation the Layered feeding in castings can be exploited to improve castingcharacteristic appearance of a shrinkage void. Shrinkage occurring results. The ﬁrst metal that establishes stable contact with the moldunder extremely low gradients may assume a smooth-walled con- wall begins solidifying and is fed not by the risering system but byﬁguration. The precipitation of hydrogen into a forming shrinkage immediately adjacent molten metal layers. In sand castings (lowvoid likewise inﬂuences the surface morphology. It is impossible gradient), the last liquid to freeze may not be localized along theto completely separate the effects of shrinkage and dissolved gas centerline. When the gradient is low and the freezing range large,in the formation of microporosity. liquid-solid mushy zones may exist throughout the casting in vari- Hydrogen may be intentionally added to counteract the more ous stages of solidiﬁcation, and changes in fraction solid fromharmful effects of shrinkage on casting acceptability. For parts surface to center may be small. Nevertheless, localized gradientsrequiring only cosmetic as-cast appearance, there would appear to and the availability of thermally differentiated liquid at or near thebe no compelling reason not to add hydrogen by any number of solidiﬁcation interface during and after mold ﬁlling result in un-means to improve superﬁcial quality. However, for parts requiring expected soundness in areas in which shrinkage voids might oth-structural integrity, machining, leak resistance, or other speciﬁc erwise be expected to occur. This principal is routinely applied inmechanical or physical characteristic, the intentional addition of the casting of wrought alloy ingot by continuous and discontinuoushydrogen is unacceptable. direct chill casting processes. In these processes, the solidifying The precipitation of hydrogen during solidiﬁcation offsets the interface is constantly fed by newly introduced thermally differ-negative relative pressures that develop when shrinkage voids form. entiated molten alloy, and a degree of heat-ﬂow equilibrium isThe equalization of internal and external pressures brought about established to provide solidiﬁcation conditions that ensure mini-by hydrogen precipitation into internal shrinkage voids minimizes mum solidiﬁcation zone growth accompanied by unlimited liquidthe tendency for surface collapse and wormhole shrinkage in the feed and an adequate thermal gradient for the promotion of struc-examples used earlier and alters the size and distribution of voids tural soundness. These principles are reﬂected in gating designsin a manner generally beneﬁting external appearance at the expense that approximate layering effects without resorting to more costlyof internal quality and integrity. methods of promoting internal quality. The formation of hydrogen voids and the effects of hydrogen on Finite-element modeling aimed at predicting mold and metalinternal shrinkage are inﬂuenced by entrained inclusions that nucle- temperature distributions during and after mold ﬁlling, solidiﬁca-ate precipitation. Because inclusions strongly facilitate bubble for- tion patterns, and the required position, size, and conﬁguration ofmation even at very low levels of dissolved hydrogen, it is im- risers has achieved valuable progress. Porosity in castings, whether hydrogen voids, shrinkage, or the more usual defects that can be associated with both conditions, can be understood and prevented by: • Melt treatment must be performed for effective removal of oxides and other entrained nonmetallics and the reduction in dissolved hydrogen concentration. • Metal handling, pouring, and the design of the gating system must preserve minimum required molten metal quality. • The gating and risering system with variable heat extraction techniques and application of the principles of directional so- lidiﬁcation must be capable of minimizing or preventing shrink- age porosity. It is important that void appearance and distribution be consid- ered in deﬁning the nature of porosity defects. The interactive effects of hydrogen, inclusions, and shrinkage should be considered in the development of appropriate corrective actions when unac- ceptable levels of porosity are experienced. Typically, hydrogen porosity appears as evenly distributed voids while shrinkage is more localized or concentrated. The distinctions are facilitated through radiographic analysis. The presence of internal voids diminishes property capability (Fig. 5.8). The void fraction reduces the effective cross-sectionalFig. 5.7 Effect of inclusions on tensile strength of Al-12Si sand cast test bars. area under stress and void topography concentrates applied stresses Inclusions decrease the tensile strength about twice as much as to substantially lower tensile and yield strengths and elongation.would be predicted on the basis of the decrease in cross section. Tensile The effect of void content on the tensile strengths of selected alloysstrength at 0% inclusions ϭ 27 ksi (186 MPa). is shown in Fig. 5.9.
Chapter 5: The Inﬂuence and Control of Porosity and Inclusions in Aluminum Castings / 535.5 Radiographic Inspection • Conﬁrm that speciﬁed internal quality standards have been met • Inspect weldments and weld repairs Radiography and ﬂuoroscopy are extensively used by the alu-minum foundry industry to reveal internal discontinuities. Other ASTM E 155, “Reference Radiographs for the Examination ofmeans of assessing internal quality such as sectioning castings, Aluminum and Magnesium Castings,” is the recommended refer-metallography, and microradiography are destructive and offer onlyplane surfaces for examination. Radiographic methods permit non-destructive whole casting evaluation and the discrimination ofshrinkage, hydrogen porosity, and more and less dense inclusionswithin limits of resolution. X-ray testing is performed as a process-control tool and as acompliance test of casting acceptability. Ultrasonic and other acous-tic techniques have not been proven for engineered aluminumcastings. Radiography is used to:• Facilitate the optimization of gating design, processes, and prac- tices in pilot stages through rapid comprehensive correlations with casting quality• Inspect castings during production, as speciﬁed by the customer or foundry quality-control standards Fig. 5.9 Effect of void content on the tensile strengths of selected aluminum casting alloys. Large decreases in tensile strength are associatedFig. 5.8 Effect of hydrogen porosity on the tensile and yield strengths of alloy with relatively small increases in the amount of voids. (a) Alloy 355.0-T61. (b) 356.0-T6 sand castings Alloy 443.0-F. (c) Alloy 520.0-T4
54 / Aluminum Alloy Castings: Properties, Processes, and Applicationsence for the interpretation of discontinuities as revealed by radio- • T.S. Piwonka and M.C. Flemings, Pore Formation in Solidi-graphic inspection. This ASTM standard and the Aluminum As- ﬁcation, Metall. Trans., Vol 236, 1966sociation standards for aluminum sand and permanent mold casting • D.R. Poirier, K. Yeum, and A.L. Maples, A Thermodynamicare the recommended references for those needing more detailed Prediction for Microporosity Formation in Aluminum-Rich Al-information on radiographic inspection. Cu Alloys, Metall. Trans., Vol 18A (No. 11), Nov 1987, p 1979–1987 • E.L. Rooy, Hydrogen in Aluminum, AFS Trans., 1993REFERENCE • E.L. Rooy, Mechanisms of Porosity Formation in Aluminum,1. D.A. Granger, Q.T. Fang, and P.N. Anyalebechi, Effects of Mod. Cast., Sept and Oct l992 Solidiﬁcation Conditions on Hydrogen Porosity in Aluminum • E. Rooy, The Use of Molten Metal Filters to Eliminate Air Pollution and Improve Melt Quality, AFS Trans., 1968 Alloy Castings, AFS Trans, 1989 • G. Sigworth and C. Wang, Evolution of Porosity During So- lidiﬁcation, AFS Trans., 1992SELECTED REFERENCES • D. Talbot, Effects of Hydrogen in Aluminum, Magnesium and Copper and Their Alloys, Int. Met. Rev., Vol 20, 1975• J.M. Boleau and J.E. Allison, The Effect of Porosity Size on the Fatigue Properties in a Cast 319 Aluminum Alloy, SAE Inter- • D. Talbot and D. Granger, Secondary Hydrogen Porosity in national, 2001 Aluminum, J. Inst. Met., Vol 92, 1963• K. Brondyke and P. Hess, Filtering and Fluxing Processes for • W. Thiele, The Oxidation of Melts of Aluminum and Aluminum Aluminum Alloys, AIME, 1964 Alloys, Aluminum, Vol 38, 1962• J. Campbell, On the Origin of Porosity in Long Freezing-Range • P. Thomas and J. Gruzleski, Threshold Hydrogen for Pore For- Alloys, Brit. Foundryman, Vol 62, 1969 mation During the Solidiﬁcation of Aluminum Alloys, Metall.• G.A. Edwards et al., Microporosity Formation in Al-Si-Cu-Mg Trans. B, March 1978 Casting Alloys, AFS Trans., Vol 105, 1997 • K.T. Tyneleius, “A Parametric Study of the Evolution of Mi-• Q.T. Fang and D.A. Granger, Porosity Formation in Modiﬁed croporosity in Al-Si Foundry Alloys,” Thesis, Drexel Univer- and Unmodiﬁed A356 Alloy Castings, AFS Trans., 1989 sity, 1992• J.E. Gruzleski et al., An Experimental Study of the Distribution • Q.G. Wang, D. Apelian, and D.A. Lados, Fatigue Behavior of of Microporosity in Cast Aluminum Base Alloys, Brit. Found- A356-T6 Aluminum Cast Alloys. Effect of Casting Defects, J. ryman, Vol 71, 1978 Light Met., 2001• C. Leroy and G. Pignault, The Use of Rotating Impeller Gas • M.J. Young, Correlation of Tensile Properties to the Amounts Injection in Aluminum Processing, J. Met., Sept 1991 of Porosity in Permanent Mold Test Bars, AFS Trans., 1981
56 / Aluminum Alloy Castings: Properties, Processes, and Applications6.2 The Effect of HIP on Tensile Properties Table 6.3 and Fig. 6.3 through 6.5 illustrate the effect of the Densal II HIP process on fatigue life. Densiﬁcation (HIP) to various extents generally enhances tensile The data in Table 6.3 illustrate that fatigue life was improved forand yield strengths and improves ductility, most markedly in com- D357.0-T6 castings with both acceptable and unacceptable levelspositions more susceptible to internal porosity under normal cast- of porosity based on radiographic examination, and that the effecting conditions. was signiﬁcantly greater for the casting with the greater porosity A comparison of tensile test results for cast plates with and as indicated by the x-rays.without densiﬁcation treatment is shown in Table 6.1; both the In a Weibull analysis for an A356.0-T6 casting (Fig. 6.3), Boi-Alcoa A359 process (Ref 2) and the Densal II Process (Bodycote leau, Zindel, and Allison (Ref 6) show a rather consistent order ofInternational) (Ref 3) are represented. magnitude increase in fatigue life for the HIPped sample. As il- For the castings given the Alcoa A359 treatment, the internal lustrated in Fig. 6.4, such consistent increases were not found forquality of 332.0, A356.0, and A357.0 permanent mold castings had VRC/PRC and sand castings, and in fact only small increasesbeen intentionally degraded by a high level of hydrogen in the melt favoring the HIPped samples are apparent; perhaps this reﬂects thebefore the A359 process was applied. The Densal II treatment was higher quality of the VRC/PRC casting in the ﬁrst place. Data fromapplied to a commercially produced A356.0-T62 vacuum riserless Bodycote (Fig. 6.5) seem to support the signiﬁcant advantage ofcasting/pressure riserless casting (VRC/PRC). their Densal process at all stress levels for 359.0-T6, with an ap- The data show that tensile and yield strength were improved by parent improvement in endurance limit of almost 50%.densiﬁcation in every case of the degraded castings, and elongation Based on the data available, it is reasonable to anticipate that HIPwas improved in most cases. For the Densal-treated castings, will likely improve fatigue properties, and that the magnitude ofstrength was not consistently affected signiﬁcantly, but elongation the improvement may be greatest in cases where signiﬁcant po-was greatly enhanced. rosity is present, especially near the surfaces. Some of the Alcoa test plates given the hydrogen-degradingtreatment beforehand exhibited progressively decreasing tensileproperties from the bottom to the top of the casting; the data in 6.4 Radiographic Inspection of HIPped CastingsTable 6.1 are presented in sequence of position in the castings andreﬂect this gradation. The A359 process treatment of these plates Radiographs of laboratory-prepared permanent mold cast platesresulted in much more uniform properties. indicated that most but not all porosity was eliminated or reduced Large numbers of additional tests by Alcoa, Bodycote, and oth- beyond x-ray resolution (Fig. 6.6 and 6.7). Voids that communi-ers, and involving experimental and production castings have now cated to the surface including shrinkage porosity extending into thebeen performed to conﬁrm that HIP generally increases tensile and casting from the riser were not affected. Some voids in close prox-yield strengths and elongation. Experience also conﬁrms that the imity to the surface, but lacking communication, collapsed, re-treatment provides greater uniformity of tensile properties within sulting in indentations.most parts. Comparison radiographs of whole production castings also re- ﬂected the dramatic improvement in radiographic quality through HIP. In many instances, improvements in radiographic quality were6.3 The Effect of HIP on Fatigue Performance consistent with the most challenging speciﬁcation requirements. The HIP cycle could be used in solution heat treatment. Pro- It was the signiﬁcant positive effect of mechanical densiﬁcation cessing costs and the incompatibility of cycles in which solutionon fatigue properties that encouraged the commercial development heat treatment requires up to six times that required for densiﬁ-of the HIP processes, and that beneﬁcial effect is well illustrated cation makes that impractical, but parts could be partially solutionby data for both the A359 and Densal II processes. heat treated and then transferred at temperature to the autoclave for Table 6.2 summarizes the results of fatigue tests of six castings completion of HIP and solution treatments.representing four different alloys given the Alcoa A359 process; all Casting methods can be used to minimize the presence of un-tests were run at 20 ksi (138 MPa). The Alcoa A359 HIP treatment densiﬁable porosity on casting surfaces, leading to the wider ap-resulted in an average increase of about 200%, with the range being plicability of HIP to cast parts. Surface treatments may also be used35 to 360%. to enhance the densiﬁcation of surface related porosity. Complete fatigue curves were developed for only one alloy, Process success is a consequence of the combined effect of332.0-F, and that is shown in Fig. 6.2. The advantage for HIPped external pressure and temperature that causes the collapse of in-casting is apparent at all stress levels, and the endurance limit for ternal voids through plastic deformation. Hydrogen solubility isthe HIPped casting is almost 20% above that of the untreated directly related to the square root of the pressure and calculationscasting. indicate that at 930 °F (500 °C), hydrogen solubility increases 32 From Table 6.2, it is clear that in cases where tests were run of times at an external pressure of 15 ksi (105 MPa). Since the solu-untreated and treated samples at the same stress level of 20 ksi (140 bility of hydrogen in aluminum at 930 °F (500 °C) is approximatelyMPa), the Alcoa A359 HIP treatment resulted in an average in- 0.003 mL per 100 g, the amount of hydrogen that can be dissolvedcrease of about 200%. For 332.0-F, where the entire fatigue curve through HIP treatment approximates 0.10 mL per 100 g. At rea-was determined (Fig. 6.2), the advantage for HIPped material was sonable hydrogen levels, void compression and the redistributionapparent at all stress levels, and the endurance limit for the HIPped or repartition of precipitated hydrogen through HIP results in es-material was almost 20% above that of the untreated casting. sentially closed porosity. Extensive reheat treatment at ambient
58 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsTable 6.2 Effect of HIP by Alcoa Process on fatigue life of representative aluminum alloy castingsHot isostatic pressing (HIP) by Alcoa 359 process Fatigue stress, ksi Fatigue life Smooth Untreated HIPped(b) ImprovementAlloy Temper Type of casting(a) Lot ID ksi MPa cycles cycles HIPped/UnHIPped(b)242.0 F PM pistons 317843,4 20.0 138 0.6 ϫ 106 1.55 ϫ 106 1.0 ϫ 106 1.75 ϫ 106 1.45 ϫ 106 1.9 ϫ 106 2.35 ϫ 106 2.1 ϫ 106 Average 1.35 ϫ 106 1.82 ϫ 106 35%332.0 F PM casting 317439,437 20.0 138 6 ϫ 104 2.05 ϫ 105 20.0 138 ... 1.6 ϫ 105 Average 6 ϫ 104 1.82 ϫ 105 203%354.0 T61 Sand cast part 317433,2 20.0 138 2.1 ϫ 105 7.6 ϫ 105 1.6 ϫ 105 7.1 ϫ 105 0.94 ϫ 105 6.2 ϫ 105 ... 4.8 ϫ 105 Average 1.55 ϫ 105 6.39 ϫ 105 312%354.0 T61 PM cast part 317429,428 20.0 138 7.2 ϫ 105 3.05 ϫ 106 6.3 ϫ 105 2.8 ϫ 106 4.5 ϫ 105 2.3 ϫ 106 2.1 ϫ 105 1.5 ϫ 106 Average 5.24 ϫ 105 2.41 ϫ 106 360%A356.0 T61 Sand cast part 317435,434 20.0 138 1.35 ϫ 105 4.3 ϫ 105 0.97 ϫ 105 3.1 ϫ 105 0.92 ϫ 105 2.05 ϫ 105 0.85 ϫ 105 1.6 ϫ 105 Average 1.02 ϫ 105 2.79 ϫ 105 174%A356.0 T61 PM cast part 317431,430 20.0 138 1.95 ϫ 105 4.4 ϫ 105 1.4 ϫ 105 3.3 ϫ 105 1.3 ϫ 105 2.9 ϫ 105 1.15 ϫ 105 2.1 ϫ 105 Average 1.45 ϫ 105 3.33 ϫ 105 130% Average increase in fatigue life at 20 ksi (138 MPa) 202%(a) Casting process and part shape if known; PM, permanent mold. (b) Percent improvement by HIP in fatigue strength or endurance limit as compared to unHIPped material from same lot.Source: Ref 5pressure can, in the worst cases, result in the reformation of internal Proc. International Symposium of Aluminum Applications:porosity. In the case of castings with high hydrogen contents, this Thrusts and Challenges, Present and Future, ASM Materialseffect is seen following the heat treatment of HIPped parts. Solutions Conference (Pittsburgh, PA), Oct 2003 The extent of outgassing occurring through diffusion in the HIP 4. J.C. Hebeisen, B.M. Cox, and B. Rampulla, Improving thetreatment cycle is insigniﬁcant. Quality of Commercial Aluminum Alloy Castings for Airframe Hot isostatic pressing is capable of upgrading mechanical prop- and Automotive Applications using the Densal II Process, 13–erties and internal soundness and dramatically improving fatigue 15 Oct 2003, ASM Internationalperformance in a wide range of sand and permanent mold cast 5. Alcoa Laboratories; from previously unpublished R.R. Mooreparts. The process can result in the salvage of unsatisfactory quality rotating beam fatigue curvescastings, an upgrading of mechanical properties for purposes of 6. J.M. Boileau, J.W. Zindel, and J.E. Allison, “The Effects ofspeciﬁcation compliance, and substantial improvement in radio- Solidiﬁcation Time on the Mechanical Properties in a Castgraphic inspection capability. A356-T6 Aluminum Alloy,” Technical Paper Series 970019, Applications of Aluminum in Vehicle Design, SAE Interna- tional, 1997REFERENCES1. Aluminum Now, The Aluminum Association SELECTED REFERENCE2. E.L. Rooy, Improving Casting Properties and Integrity with • M.M. Diem and S.J. Mashi, Simultaneous Densiﬁcation and Hot Isostatic Processing, Mod. Met., Dec 1963 Solution Heat Treatment of Aluminum Castings, Proc. Inter-3. J.C. Hebeisen, B.M. Cox, and B. Rampulla, Improving the national Symposium of Aluminum Applications: Thrusts and Quality of Commercial Aluminum Alloy Castings for Airframe Challenges, Present and Future, ASM Materials Solutions Con- and Automotive Applications Using the Densal II Process, ference (Pittsburgh, PA), Oct 2003
Chapter 6: Hot Isostatic Processing / 59Fig. 6.2 Effect of Alcoa A359 HIP process on the rotating beam fatigue life of a 332.0-F casting (specimen per Fig. A3.2 in Appendix 3)Table 6.3 Effect of HIP by Densal II on fatigue life of representative aluminum alloy castings Fatigue life Fatigue stress, smooth Untreated HIPped Alloy Temper Type of casting ksi MPa cycles cycles Improvement(a)D357.0 T6 Investment 26.4 182 19,337 177,169 (acceptable 63,515 174,555 x-rays) 69,824 161,533 94,191 130,645 60,986 84,000 80,524 199,535 39,271 121,004 31,126 164,405 34,240 125,950 29,200 144,569 ... 163,364 Average 52,221 149,703 187%D357.0 T6 Investment 26.4 182 15,509 136,361 (unacceptable 19,718 133,401 x-rays) 16,501 49,067 13,447 63,190 13,795 130,114 5,121 143,122 19,210 142,519 10,147 154,453 10,763 160,191 2,444 178,372 60,707 63,357 ... 146,253 ... 152,991 ... 172,748 ... 119,570 ... 69,473 ... 22,604 ... 125,499 Average 17,033 120,183 606%(a) Percent improvement by HIP in fatigue strength or endurance limit as compared to unHIPped material from same lot. Source: Ref 4
60 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsFig. 6.3 Weibull analysis of fatigue data for A357.0-T6 aluminum alloy castings with and without Densal II HIP. Source: Ref 6 Fig. 6.4 Fatigue S-N curves for VCR/PCR and sand cast A356.0-T6 alumi- num alloy castings with and without Densal II HIPFig. 6.5 Rotating bending fatigue S-N curves (R ϭ –1.0) for gravity die cast 359.0-T64 aluminum alloy casting with and without Densal II HIPFig. 6.6 Radiographs showing an untreated A356 alloy cast section with heavy porosity (right) and after hot isostatic pressing (left) Fig. 6.7 Thin-section radiographs taken from A356 plate casting sections at one-inch intervals: A–D after HIP treatment, E–H as cast
62 / Aluminum Alloy Castings: Properties, Processes, and Applicationstice types and maintains a registry of standard heat treatment prac- practice with a large margin of safety to avoid the delays and coststices and designations for industry use: of reheat treatment when property limits are not met. Because of the changing slope of the characteristic solvus as• F, as-cast temperature approaches the eutectic melting point, solution heat• O, annealed treatment temperature is critical in determining the degree of so-• T2, annealed (obsolete designation; use O instead) lution that can be attained. There is, furthermore, the effect of• T4, solution heat treated and quenched temperature on diffusion rates, which directly inﬂuences degree of• T5, artiﬁcially aged from the as-cast condition solution as a function of time at temperature.• T6, solution heat treated, quenched, and artiﬁcially aged Within temperature ranges deﬁned for solution heat treatment• T7, solution heat treated, quenched, and overaged by applicable speciﬁcation lies a signiﬁcant corresponding range of solution potentials. The knowledgeable heat treatment facility orFor tempers T4 through T7, additional digits such as T5x, T5xx, foundry seeking to obtain superior properties will bias solution heatT6x, etc. may be used to deﬁne practice variations. The T101 treatment temperature within speciﬁcation limits to obtain the high-temper has been assigned to a compressively cold-worked condi- est practical degree of solution. Superior properties can be achievedtion applicable only to alloy x850.0. with furnaces, thermocouples, and furnace controls that are capable Speciﬁc criteria for heat treatment and the practices that will be of operating within close temperature ranges near the eutectic melt-used are often separately negotiated between buyer and seller. ing region, recognizing the resistance of cast structures to melting The heat treatment of aluminum alloys is based on the varying based on diffusion considerations. While temperatures just belowsolubilities of metallurgical phases in a crystallographically mono- the eutectic melting point are desirable for optimal property de-tropic system. Since solubility of the eutectic phase increases with velopment, it is critically important that eutectic melting resultingincreasing temperature to the solidus, the formation and distribu- in brittle intergranular eutectic networks be avoided.tion of precipitated phases can be manipulated to inﬂuence material Insoluble phases including those containing impurity elementsproperties. are normally thought to be unaffected by solution heat treatment. In addition to phase and morphology changes associated with However, limited changes do occur. The surfaces of primary andsoluble elements and compounds, other (sometimes desirable) ef- eutectic silicon particles are characteristically rounded during so-fects accompany elevated-temperature treatment. Microsegrega- lution heat treatment. The solution heat treatment of alloy A444.0,tion in all solidiﬁed structures is minimized or eliminated. Residual which contains no soluble phase, is justiﬁed solely by this phe-stresses caused by solidiﬁcation or by prior quenching are reduced, nomenon and its effect on ductility. Limited solubility also resultsinsoluble phases may be physically altered, and susceptibility to in similar physical boundary changes in other insoluble interme-corrosion may be affected. tallics.7.1 Solution Heat Treatment 7.2 Quenching Exposure to temperatures corresponding to maximum safe limits The objective of quenching is retention of the highest possiblerelative to the lowest melting temperature for a speciﬁc heat treat- degree of solution with the lowest level of induced residual stressesable composition results in dissolution of soluble phases that formed and the least warpage or distortion consistent with commercial orduring and after solidiﬁcation. The rate of heating to solution tem- speciﬁed requirements. Quenching is a distinct step in thermalperature is technically unimportant. When more than one soluble practice leading to the metastable, supersaturated solution heatphase is present such as in Al-Si-Cu-Mg and Al-Zn-Cu-Mg sys- treated condition, T4. Speciﬁc parameters may be associated withtems, stepped heat treatment may be required to avoid melting of the heating of parts to achieve solution, and separate parameterslower-melting-temperature phases. apply to the steps required to achieve the highest postquench degree The most complete degree of solution that can be practically and of retained solution. Rapid cooling from solution temperature toeconomically achieved is desirable for optimal properties. Differ- room temperature is critical, difficult, and often the least-controlledent casting processes and foundry practices result in microstruc- step in thermal processing.tural differences with relevance to heat treatment practice. Coarser Speciﬁcations often deﬁne or recommend quench delay limits.microstructures associated with slow-solidiﬁcation-rate processes In practice, the shortest possible delay is desirable. Specializedrequire longer exposure at solution heat treatment temperature for equipment such as bottom-drop and continuous furnaces offer thesesolution to be achieved. The time required at temperature is typi- advantages. Excessive delays result in temperature drop and thecally progressively shorter for investment, sand, and permanent rapid formation of coarse precipitates in a temperature range atmold castings, but thin-walled sand castings produced with ex- which the effects of precipitation are ineffective for hardeningtensive use of chills can also often display ﬁner microstructures. purposes. The slope of the temperature-time relationship duringFor these reasons, solution heat treatment practices may be opti- quenching from solution temperature should be sufficiently steepmized for any speciﬁc part to achieve solution with the shortest that limits of precipitate solubility are not intersected (Fig. 7.2).reasonable cycle once a production practice is ﬁnalized. Most Even though castings are characteristically more tolerant of quenchfoundries and heat treaters will select a solution heat treatment delay than wrought products because of coarser structures and
Chapter 7: Heat Treatment of Aluminum Castings / 63longer diffusion times, excessive quench delays nevertheless result geometry inﬂuence the results. As section thicknesses increase, thein less-than-optimal strengthening potential. metallurgical advantage of quench rates obtained by water tem- Water is the quench medium of choice for aluminum alloys, and peratures less than 150 °F (65 °C) diminish, but the cooling rateits temperature has a major effect on results. Most commercial advantage of 150 °F (65 °C) versus 212 °F (100 °C) water quenchquenching is accomplished in water entered near the boiling point, temperature is retained independent of section thickness.but room temperature, 150 °F (65 °C), and 180 °F (80 °C) are In addition to developing racking and loading methods thatcommon standardized alternatives. Effects of thickness and quen- space and orient parts for most uniform quenching, quenchantchant temperature on average cooling rates at midplane are shown additions are often made to:in Fig. 7.3. Figure 7.4 shows differences in mechanical propertiesthat result from quenching in water at different temperatures. • Promote stable vapor ﬁlm boiling by the deposition of com- Since higher potential strength is associated with the most rapid pounds on the surface of parts as they are submerged in thequenching and, in general, corrosion and stress-corrosion perfor- quench solutionmance are enhanced by rapid quenching, it would appear that • Suppress variations in heat ﬂux by increasing vapor ﬁlm boilingroom-temperature water should routinely be employed. More se- stability through chemically decreased surface tensionvere quenching offers diminishing beneﬁts in property potentials • Moderate quench rate for a given water temperatureand signiﬁcant increases in residual stresses and distortion. Quen-chant temperature is the dominant factor in these considerations. Quenching rates are also affected by surface condition of the parts. The key to the compromise between goals involving property More rapid quenching occurs with oxidized, stained, and roughdevelopment and the physical consequences of quenching is heat- surfaces while bright, freshly machined, and etched surfaces quenchextraction uniformity, which is in turn a complex function of the more slowly.operable heat-extraction mechanism. Nucleant, vapor ﬁlm, and The common use of water as a quenching medium is largelyconvective boiling occur with dramatically different heat- based on its superiority in heat extraction relative to other mate-extraction rates at different temperature intervals, section thick- rials. Nevertheless, quenching has been accomplished in oil, saltness, and surface conditions. Load density, positioning, and casting baths, and in organic solutions. For many compositions, fan or mistFig. 7.2 Time-temperature-precipitation chart for aluminum alloys containing 7% Al and varying amounts of magnesium
64 / Aluminum Alloy Castings: Properties, Processes, and Applicationsquench is feasible as a means of obtaining dramatic reductions in Most aluminum alloys age harden to some extent naturally afterresidual stress levels at considerable sacriﬁce in hardening poten- quenching; that is, properties change as a function of time at roomtial. temperature solely as a result of Guinier-Preston (GP) zone for- In general, parts that have been solution heat treated and quenched mation within the lattice structure. The extent of change is highlydisplay tensile properties and elongation superior to those of the alloy dependent. For example, room-temperature aging in alloysas-cast, F, condition. It is unique in improving strength, hardness, such as A356.0 and C355.0 occurs within 48 h with insigniﬁcantand ductility. Typical thermal treatments sacriﬁce strength and changes thereafter. Alloy 520.0, normally used in the T4 condition,hardness for elongation or develop strength and hardness at the age hardens over a period of years, and a number of Al-Zn-Mgexpense of ductility. The T4 condition is, however, rarely em- alloys that are employed without heat treatment exhibit rapidployed. Instead, the advantages of aging or precipitation hardening changes in properties over three or four weeks and harden at pro-are obtained by additional thermal treatment following quenching. gressively reduced rates thereafter.Among these advantages are increased strength and hardness with The process of hardening is accelerated by artiﬁcially aging ata corresponding sacriﬁce in ductility, improved machinability, the temperatures ranging from approximately 200 to 500 °F (90 to 260development of more stable mechanical properties, and reduced °C), depending on the alloy and the properties desired. In naturalresidual stresses. and artiﬁcial aging, supersaturation, which characterizes the room- temperature solution condition, is relieved by the precipitation of solute that proceeds in stages with speciﬁc structural effects. At7.3 Precipitation Heat Treating/Aging room or low aging temperatures or during transition at higher temperatures, the principal change is the diffusion of solute atoms Natural or artiﬁcial precipitation hardening following solution to high-energy sites such as dislocations, dislocation tangles, andheat treatment and quench most powerfully differentiates the prop- vacancies within the crystal lattice producing distortion of latticeerties of cast aluminum products. Hardening is deﬁned as changes planes and forming concentrations of subcritical crystal nuclei.in metallurgical structure resulting in increased resistance to de- With continued exposure at aging temperature, these sites reach,formation. or fail to reach, critical nucleation size, a stage leading to theFig. 7.3 Midplane cooling rates for varying water quench temperatures and aluminum alloy casting thicknesses
Chapter 7: Heat Treatment of Aluminum Castings / 65formation of discrete particles displaying the identiﬁable crystal- siﬁes room-temperature aging, and the progression is from GPlographic character of the precipitated phase. With additional treat- zones to the transition and stable equilibrium phases:ment, these transitional phase particles grow with an increase incoherency strains until with sufficient time and temperature, in- S ϭ Al2CuMgterfacial bond strength is exceeded. Coherency is lost, and with it,the strengthening effects associated with precipitate formation andgrowth. Continued growth of the now equilibrium phase occurs SS → GP → SЈ → Swith the loss of hardness and strength corresponding to the over-aged condition. 7.3.3 Aluminum-Silicon-Magnesium Magnesium silicide is the soluble phase in important alloys such7.3.1 Aluminum-Copper as 356.0, A356.0, and A357.0 alloys. Unlike the hardening that The soluble phase in aluminum-copper alloys is copper alu- accompanies the development of coherent lattice strains, this phaseminide (CuAl2). At temperatures above 212 °F (100 °C), GP zones acts to increase the energy required for deformation of the crystalthat form by diffusion of copper atoms in the supersaturated solid lattice. Spherical zones convert to needle-shaped particles at pointssolution (SS) are replaced by Љ, sometimes referred to as GP, corresponding to peak hardening. Further aging produces rod-with an ordered three-dimensional atomic arrangement. Continued shaped particles. The transition from ␤Ј to equilibrium Mg2Si oc-diffusion and growth lead to the formation of the transition phase curs without further diffusion:Ј, which has the same composition and structure as the stable phase and maintains coherency with the crystal lattice. Finally, as ␤ ϭ Mg2Sidiscrete transition phase regions continue to grow, Ј transforms tostable, noncoherent equilibrium : SS → GP → ␤Ј → ␤ ϭ CuAl2 7.3.4 Aluminum-Zinc-Magnesium SS → GP → Љ → Ј → Several hardening phases may be formed in Al-Zn-Mg alloys. Most alloys of this type room-temperature age for extended pe-7.3.2 Aluminum-Copper-Magnesium riods. The presence of M and T in precipitation-hardened alloys A similar sequence occurs in the artiﬁcial age hardening of Al- such as 712.0, 713.0, and 771.0 is largely dictated by composition,Cu-Mg alloys. The addition of magnesium accelerates and inten- but both may be present. MЈ is less effective in strength develop- ment, and transition to the stable forms occurs rapidly at conven- tional aging temperatures: M ϭ MgZn2 T ϭ Mg3Zn3Al2 SS R GP R MЈ R M ↓ TЈ → T The practice to be employed in artiﬁcial aging is entirely de- pendent on the desired level of property/strength development. Aging curves facilitate process selection. The heat treater may reasonably predict the results of aging by reference to these curves (see Data Set 1). It should be noted that longer times at lower aging temperature generally result in higher peak strengths. The aging response, or rate of property change as a function of time at peak strength, is also of interest. The ﬂatter curves associated with lower aging temperatures allow greater tolerance in the effects of time/ temperature variations. Unlike solution heat treatment, the time required to reach aging temperature may be signiﬁcant, but is seldom included in age-cycleFig. 7.4 Tensile properties of end-chilled A356-T6 at different quench tem- control. The energy imparted during heating to precipitation- peratures. 0.75 in. (19 mm) thick test slab, aged 310 °F (155 °C) hardening temperature may be integrated into the control sequencefor 5 h to more accurately control results and minimize cycle time.
66 / Aluminum Alloy Castings: Properties, Processes, and Applications The overaged T7 condition is less common than is the T6 temper, and more rapid temperature change results in large differences inbut there are good reasons for its use in many applications. Pre- the cooling rates of surface and internal regions of the castingcipitation hardening as practiced for the T6 condition results in structure. When the part is cooled from elevated temperature, thereductions of 10 to 35% in residual stresses imposed by quenching. normal distribution of residual stresses when the part has reachedWhile overaging, by deﬁnition, is carrying the aging cycle to a room temperature is compression at the surface and counterbal-point beyond peak hardness, it is also most often conducted at a ancing tension in core regions (Fig. 7.5). Increasing thickness andhigher temperature than employed for the fully hardened condition. alloy strength increases the magnitude of residual stresses.A substantial further decrease in residual stresses is associated with Stresses induced by quenching from solution heat treatment tem-the higher-temperature aging treatment. Furthermore, parts be- perature are many times more important than casting stresses orcome more dimensionally stable as a result of more complete stresses imposed in any other conventional process. Decreasing thedegrowthing, and increased stability in performance is ensured severity of quench from solution heat treatment results in a lowerwhen service involves exposure at elevated temperatures. level of residual stresses but with correspondingly decreased ma- terial strength. Air quenching may provide a useful compromise in applications requiring unusual dimensional stability.7.4 Annealing Residual stresses may only be relaxed by exposure to elevated temperature followed by slow cooling or by plastic deformation. Annealing, originally assigned the designation T2, now the O Plastic deformation, routinely practiced for stress relief in wroughttemper, is rarely employed but serves a useful purpose in providing products, has little application in the complex designs of engi-parts with extreme dimensional and physical stability and the low- neered products such as castings, so that stress relief becomes moreest level of residual stresses. The annealed condition is also char- exclusively a function of thermal treatment. Overaging results inacterized by low strength levels, softness, and correspondingly signiﬁcant reductions in residual stresses, and annealing providespoor machinability. Typical annealing practices are for relatively a practical minimum in residual stress levels. The residual stressesshort (2 to 4 h) exposures at a minimum temperature of 650 °F (340 retained after annealing or aging is limited by the yield strength of°C). Higher-temperature practices are employed for more complete the material at treatment temperature.relaxation of residual stresses. The cooling rate from annealingtemperature must be controlled in such a way that residual stressesare not reinduced and that resolution effects are avoided. Typical 7.7 Troubleshooting Heat Treatment Problemspractice is to cool from annealing temperature in the furnace or instill air. 7.7.1 Acceptance Criteria Mechanical properties that include ultimate tensile strength, yield strength, and elongation are the usual criteria by which material7.5 Stability acceptability is determined after heat treatment. Mechanical prop- erty limits statistically deﬁne normalcy for a given composition Stability is deﬁned as the condition of unchanging structural and cast by a speciﬁc process or a composition cast by a speciﬁc processphysical characteristics as a function of time under service con- that has been heat treated to a speciﬁed temper.ditions. The metastable T4 condition is subject to hardening, ex- Separately cast tensile specimens, poured from the melt fromtensive in some alloys and limited in others, at room and higher which the casting lot is poured, are typically used for all castingtemperatures. With exposure to elevated temperatures, signiﬁcant processes. When castings are heat treated, these specimens ac-additional physical and mechanical property changes are to be company the castings they represent through all phases of thermalexpected. They include dimensional change or growth and changes operations. Speciﬁcations may also require or rely exclusively onin susceptibility to corrosion and stress corrosion that can be as- the testing of specimens excised and machined from the casting.sociated with transitional states in some alloys. The most stable conditions obtainable are annealed, overaged,aged, and as-cast, in that order. Underaged and solution heat treatedparts are least stable.7.6 Residual Stresses Thermal treatment not only affects mechanical properties, butalso directly inﬂuences residual stress levels. Residual stresses are caused by differences in postsolidiﬁcationcooling between surface and interior regions. They are induced bycooling from solidiﬁcation temperature, quenching from solutionheat treatment temperature, and by changes in temperature at anyintermediate step. Residual stresses are functions of differential Fig. 7.5 Characteristic residual stress distribution after solution heat treat-cooling rates, section thickness, and material strength. More severe ment and quench. t, thickness
Chapter 7: Heat Treatment of Aluminum Castings / 67 Minimum mechanical property limits are usually deﬁned by the tion limits and no other practice discrepancies are determined, alloyterms of general procurement speciﬁcations, such as those devel- content should be carefully examined.oped by government agencies and technical societies. These docu- The role of trace elements in mechanical property developmentments specify testing frequency, tensile specimen type, casting lot is important since these are often not separately deﬁned in alloydeﬁnitions, testing procedures, and test limits. These requirements speciﬁcations except as “others each” and “others total.” Sodiummay also be separately negotiated. and calcium are embrittling in 5xx.0 alloys. Low-temperature- Brinell hardness (10 mm ball, 500 kg load, 30 s) is only ap- melting elements, such as lead, tin, and bismuth may, under someproximately related to yield strength, and while it is used routinely conditions, form embrittling intergranular networks with similaras an easily measurable nondestructive indicator of material con- effects. Insoluble impurity elements are generally responsible fordition, it is not normally guaranteed. decreases in elongation. Electrical conductivity only approximates the relationship of Low concentrations of soluble elements in heat treatable com-chemistry, structure, and thermal treatment in cast or cast and heat positions naturally result in the more frequent distribution of me-treated aluminum structures. Electrical conductivity is used in ro- chanical property values in the lower speciﬁcation range. Elementtors and anodes as an acceptance criterion. It may also be used to relationships such as Cu-Mg, Si-Mg, Fe-Si, Fe-Mn, and Zn-Cu-Mgestimate susceptibility to stress-corrosion cracking. are also important considerations in deﬁning the causes of abnor- mal mechanical property response to thermal treatment. Mechani- cal property failure may be caused by structural unsoundness and7.7.2 Diagnosis not by inadequate heat treatment. It is not appropriate to believe When speciﬁed mechanical property limits are not met after heat that unsound castings and tensile specimens will consistently meettreatment, analytical procedures and judgments are applied to es- speciﬁed mechanical property limits. All defects adversely affecttablish a corrective course of action based on evidence or assump- strength and elongation. Shrinkage, hydrogen porosity, cracks, in-tions concerning the cause of failure. Variations in chemical com- clusions, and other casting-related defects inﬂuence mechanicalposition, even within speciﬁed limits, can have measurable effects. properties adversely, and their effects should be considered beforeMetallurgical considerations such as chemical segregation, phase addressing the possibility of heat treatment problems.size and distribution, grain and dendrite cell sizes, and the modi- The quality of solution heat treatment may be assessed in severalﬁcation or degree of reﬁnement of eutectic and hypereutectic struc- ways. There is, of course, the rounding effect on “insoluble phases”tures alter properties. For heat treated and aged tempers, variables that can be observed metallographically and serves as evidence ofinclude solution time and temperature, temperature of quenching elevated-temperature exposure. The elimination of microsegrega-medium, quench delay, and aging cycle. Annealing times and tem- tion or coring in many alloys is another indication of elevated-peratures and postanneal cooling conditions are important for O temperature treatment. The effective solution of soluble phases cantemper material. be determined microscopically. Undissolved solute can be distin- It is important to establish that the tensile specimens involved guished from the appearance of precipitate that forms at high tem-were representative and that test procedures conformed to the re- peratures and that result from quench delay or an inadequate orquirements of applicable test method standards: incomplete quench by particle size and distribution. There is also a tendency for precipitate that forms as a result of quench delay or• The stress-strain diagram should be used to conﬁrm that test inadequate quench to concentrate at grain boundaries as opposed procedures including strain rate were appropriate. to more normal distribution through the microstructure for properly• Failure should not be associated with surface damage such as solution heat treated and aged material. nicks and scratches or machining errors. While the overaged condition is microscopically apparent, under-• Specimens may contain nonrepresentative defects. aging is difficult to assess because of the submicroscopic nature of• The fracture surface should be examined to determine that no transitional precipitates. Evidence of acceptable aging practice is anomalous condition contributed to failure. best obtained from aging furnace records that might indicate errors• The entire fracture must be contained within the center half of in the age cycle. While underaging may be corrected by additional the gage length. aging, for all other heat treatment aberrations, except those associ-• Replacement and retest provisions are deﬁned by speciﬁcation ated with objectionable conditions such as high-temperature oxida- and standards. tion or eutectic melting, resolution heat treatment is an acceptable corrective action. Eutectic melting occurs when the eutectic meltingFurnace records and time-temperature charts should be consulted temperature is exceeded in solution heat treatment, resulting in char-to conﬁrm that speciﬁed practices were observed. acteristic rosettes of resolidiﬁed eutectic. The chemical composition of alloys of aluminum is determined High-temperature oxidation is a misnamed condition of hydro-by light emission spectroscopy. Quantometers simplify and stan- gen diffusion affecting surface layers during solution heat treat-dardize chemical element concentrations. In some cases, wet chem- ment. It results from excessive moisture in the furnace atmosphere,istry or alternative techniques such as atomic absorption are em- sometimes aggravated by oil, grease, sulfur, or other furnace orployed. Less accurate methods including x-ray ﬂuorescence are casting surface contamination.used to discriminate composition ranges. There are no technical reasons for discouraging even repeated Chemical composition is a major variable in mechanical property reheat treatment to obtain acceptable mechanical properties. In thedevelopment. When mechanical properties have failed speciﬁca- case of aluminum-copper alloys, it is essential that resolution heat
68 / Aluminum Alloy Castings: Properties, Processes, and Applicationstreatment be conducted at a temperature equivalent to or higher • NADCA Product Speciﬁcation Standards for Die Casting, 5ththan the original practice to ensure effective resolution; however, ed., North American Die Casting Association (NADCA), 2003it should be apparent that when the results of repeated reheat • E.L. Rooy, Heat Treatment of Aluminum Cast Products, Metaltreatment prove to be equally unsatisfactory that other conditions Processing Institute, WPI, 1999are responsible for mechanical property failure. • E.L. Rooy, Practical Aspects of Heat Treatment, TMS, 1988 • S. Shivkumar et al., Heat Treatment of Al-Si-Mg Alloys, ACRL, Drexel University, 1989SELECTED REFERENCES • Standards for Aluminum Sand and Permanent Mold Casting, The Aluminum Association, Inc., Dec 1992• Alloy and Temper Registrations Records, The Aluminum As- • K.R. Van Horn, Ed., Aluminum, Vol 1, American Society for sociation, Inc. Metals, 1967• J.E. Hatch, Aluminum: Properties and Physical Metallurgy, • D. Zalenas, Ed., Aluminum Casting Technology, 2nd ed., Ameri- American Society for Metals, 1984 can Foundrymen’s Society, 1993
Chapter 8: Properties and Performance of Aluminum Castings / 718.3 Typical and Minimum Mechanical It is important to note that there are no published industry sta- Properties of Aluminum Alloy Castings tistically reliable minimum values for die castings of any alloy. This reﬂects the fact that the properties of individual cast parts may vary The typical and minimum (design) mechanical properties of rather widely depending on their conﬁguration and the speciﬁcaluminum casting alloys are presented and discussed in the fol- casting process. It is recommended that users of aluminum dielowing sections: castings plan to carry out a statistical analysis of the properties of the speciﬁc cast part they intend to use as part of the design pro-• 8.3.1 Published typical mechanical properties gram.• 8.3.2 Published minimum (design) mechanical properties As with typical properties, it is important to keep in mind that,• 8.3.3 Effects of subzero and elevated temperatures on mechani- except where explicitly stated, the speciﬁcation minimum prop- cal properties erties are based on tests of separately cast test bars (i.e., cast at the• 8.3.4 Inﬂuence of premium practices and emerging casting same time as the speciﬁc cast parts). Thus it is to be expected that technologies on mechanical properties in many if not all locations in speciﬁc cast parts, the properties may be lower than those determined from the separately cast test bars.8.3.1 Published Typical Mechanical Properties The industry practice is to consider that the properties of actual The published aluminum industry typical mechanical properties conventional castings may be as low as 75% of the cast test barof aluminum casting alloys are presented in Table 8.6 in English speciﬁcation values.units and in Table 8.7 in metric units (Ref 3–7). Also, as with the typical properties of aluminum castings, the In using the values from Table 8.6 and 8.7, one should bear in metric minimum values have been created by converting directlymind that the published typical values are normally based on the from the English values by multiplying by the appropriate con-analysis of the results of separately cast test bars (Appendix 3, Fig. version factors and rounding to the nearest megapascal (MPa). ItA3.1), not of specimens taken from actual cast components. The may be noted that this situation is different than for wrought alu-casting practices for separately cast test bars are typically more minum alloy products, for which hard metric minimum values (i.e.,uniform and controlled than for the broad array of cast parts, and calculated from the original metric test data and rounded) haveso the published typical values may be higher than can be realis- been determined.tically expected from individual cast parts. The industry guidelineis that the strengths of actual cast parts may be as low as 75% of 8.3.3 Effects of Subzero and Elevated Temperaturesthe values for separately cast test bars. on Mechanical Properties In these tables, the typical properties are deﬁned as the averageof the range for all compositions of the respective alloy and temper.In most cases, the metric values are converted directly from the The published typical tensile properties of several aluminumEnglish values by multiplying by the appropriate conversion fac- casting alloys at temperatures as high as 700 °F (370 °C) fortors and rounding to the nearest megapascal (MPa). holding times as long as 10,000 h are presented in Data Set 4 (Ref Published typical stress-strain curves for a variety of aluminum 14). For some alloys, data are also included for room temperaturealloys are presented in Data Set 3 (Ref 12). after the alloys have been exposed to extended heating at tem- peratures up to 500 °F (260 °C). Also included where available are8.3.2 Published Minimum and Design Mechanical data at subzero temperatures as low as –452 °F (–270 °C), near Properties absolute zero. Creep properties are presented in Data Set 5 (also The published aluminum industry speciﬁcation minimum me- from Ref 14).chanical properties of aluminum casting alloys in both English and Like most other aluminum alloys, the casting alloys have notmetric units are presented in Table 8.8 (Ref 3–7). only higher strengths but also higher elongations at subzero tem- These properties are consistent with the speciﬁed minimum ten- peratures than at room temperature. While data are available forsile requirements cited in the several ASTM standards as published only one alloy (A356.0-T6) at temperatures below –320 °F (–196in the Annual Book of ASTM Standards, Volume 02.02, namely: °C), it is clear that this trend continues at lower temperatures, essentially to absolute zero. Aluminum casting alloys may be usedASTM under arctic conditions and for cryogenic applications without anydesignation Title fear of low-ductility or brittle fracture.B 26/B 26M Standard Speciﬁcation for Aluminum Alloy Sand CastingsB 85 Standard Speciﬁcation for Aluminum Alloy Die Castings The effects of temperatures above room temperature also parallelB 108 Standard Speciﬁcation for Aluminum Alloy Permanent Mold expectations from other aluminum alloys. Typically, as temperature CastingsB 618 Standard Speciﬁcation for Aluminum Alloy Investment Castings increases above about 212 °F (100 °C), strengths decrease at anB 686 Standard Speciﬁcation for Aluminum Alloy Castings, High- increasing rate until they level out around 500 to 600 °F (260 to Strength 315 °C). Strengths also decrease with increasing time at tempera-
80 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsTable 8.3 Alloy constants for calculation of coefﬁcients of thermal expansion for some aluminum casting alloys overvarious temperature rangesAlloy Alloy constant C Alloy Alloy constant C Alloy Alloy constant C208.0 0.950 356.0 0.910 511.0 1.005240.0 0.990 A356.0 0.910 513.0 1.020242.0 0.955 357.0 0.920 514.0 1.020295.0 0.970 A357.0 0.920 518.0 1.015308.0 0.910 359.0 0.900 520.0 1.040319.0 0.905 360.0 0.890 710.0 1.020332.0 0.875 A360.0 0.900 711.0 1.000333.0 0.880 380.0 0.885 712.0 1.010336.0 0.845 A380 0.895 850.0 0.990354.0 0.895 413.0 0.860 851.0 0.965355.0 0.950 C443.0 0.945 852.0 0.985C355.0 0.950 A444.0 0.920 ... ...Equations of linear thermal expansion:1. Lt (0 to −320 °F) = L0[1 ϩ C (11.74t − 0.00125t 2 − 0.0000248t 3) 10 −6]2. Lt (0 to 1000 °F) = L0[1 ϩ C (12.19t ϩ 0.003115t 2) 10 −6]3. Lt (−76 to 212 °F) = L0[1 ϩ C (12.08t ϩ 0.003765t 2) 10 −6] L0 = Length at 0 °F Lt = Length at temperature, t °F, within the range indicated C = Alloy constantConstants established from determinations made on alloys in the annealed (O temper) condition. With heat treatable alloys, the application of the above equations and alloy constants is lim-ited to temperatures below 600 °F (315 °C); for such alloys, the alloy constants are approximately 0.015 higher in the heat treated condition and should be applied to temperatures that donot exceed those used in the ﬁnal aging treatments. For 7xx.x and 8xx.x casting alloys, application is restricted to 400 °F (200 °C). Source: Ref 10Table 8.4 Effect of elements in and out of solution ture, especially in the intermediate temperature range. Elongationson resistivity increase with increasing time and/or temperature. Of the alloys for which data are presented, 201.0-T7 clearly has Average increase in resistivity per wt%(a), μ⍀/cm the superior strengths at elevated temperatures. In fact all of the Maximum solubilityElement in aluminum, % In solution Out of solution(b) 2xx.0 alloys hold up rather well at temperatures up to about 400Chromium 0.77 4 0.18 °F (205 °C) compared to alloys of the other series. It is theCopper 5.65 0.344 0.03 inﬂuence of the copper content providing the high-temperatureIron 0.052 2.56 0.058Lithium 4 3.31 0.68 resistance of the 2xx.0 series.Magnesium 14.9 0.54(c) 0.22(c)Manganese 1.82 2.94 0.34Nickel 0.05 0.81 0.061Silicon 1.65 1.02 0.088Titanium 1 2.88 0.12Vanadium 0.5 3.58 0.28Zinc 82.8 0.094(d) 0.023(d)Zirconium 0.28 1.74 0.044(a) Add increase to the base resistivity for high-purity aluminum: 2.65 μ⍀-cm at 20 °C (68°F) or 2.71 μ⍀-cm at 25 °C (77 °F). (b) Limited to about twice the concentration given forthe maximum solid solubility, except as noted. (c) Limited to approximately 10%. (d) Lim-ited to approximately 20%Table 8.5 Densities and elastic moduli of aluminum andaluminum alloying elements Density Elastic modulusAlloying element lb/in.2 g/cm3 106 psi GPaAluminum 0.0971 2.699 10.0 69Chromium 0.260 7.19 36.0 248Copper 0.324 8.96 16.0 128Iron 0.284 7.87 28.5 208Magnesium 0.0628 1.74 6.5(a) 44(a)Manganese 0.268 7.43 23.0 159Nickel 0.322 8.90 30.0 207Silicon 0.084 2.33 16.0 110Tin 0.264 7.30 6.0 44Titanium 0.164 4.54 16.8 120Zinc 0.258 7.13 10(b) 69(b)Zirconium 0.23 6.5 11.0 49(a) Effect of magnesium is equivalent to approximately 11.0 ϫ 106 psi or 75 GPa. (b) The Fig. 8.1 Damping characteristics of 319.0 and 356.0 casting alloys com-modulus of zinc is not well deﬁned; these values are lower limit estimates. pared with those of wrought alloys, including clad 2024. Source: Ref 11
84 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsTable 8.6 (continued) Tension Shear Fatigue Modulus Ultimate Yield Elongation ultimate ultimate of strength, strength(a), in 2 in. or 4D, Hardness(b), strength, limit(c), elasticity(d),Alloy Temper ksi ksi % HB ksi ksi 10 6 psiPermanent mold casting (continued)705.0 T5 37 17 10 55–75 ... ... ...707.0 T7 45 35 3 80–110 ... ... ...711.0 T1 28 18 7 55–85 ... ... ...713.0 T5 32 22 4 60–90850.0 T5 23 11 12 45 15 9 10.3851.0 T5 20 11 5 45 14 9 10.3 T6 18 ... 8 ... ... ... 10.3852.0 T5 32 23 5 70 21 11 10.3Die casting360.0 F 44 25 3 75 28 20 10.3A360.0 F 46 24 4 75 26 18 10.3380.0 F 46 23 3 80 28 20 10.3A380.0 F 47 23 4 80 27 20 10.3383.0 F 45 22 4 75 ... 21 10.3384.0 F 48 24 3 85 29 20 ...390.0 F 40.5 35 <1 ... ... ... ...B390.0 F 46 36 <1 120 ... 20 11.8392.0 F 42 39 <1 ... ... ... ...413.0 F 43 21 3 80 25 19 10.3A413.0 F 42 19 4 80 25 19 ...C443.0 F 33 14 9 65 29 17 10.3518.0 F 45 28 5 80 29 20 ...(a) For tensile yield strengths, offset ϭ 0.2%. (b) 500 kg load, 10 mm ball. (c) Based on 500,000,000 cycles of completely reversed stress using R.R. Moore type of machines and speci-mens. (d) Average of tension and compression moduli; compressive modulus is nominally about 2% greater than the tension modulus. Source: Ref 3–58.3.4 Inﬂuence of Premium Practices and Emerging Both aluminum industry sources and MMPDS/MIL-HDBK-5 Casting Technologies on Mechanical deﬁne the minimum and/or design properties as the values which Properties the properties of 99% of the lots of a given alloy and temper would equal or exceed, with 95% conﬁdence. Speciﬁcation AMS-A-21180 deﬁnes the requirements for high- Premium Engineered Castings. As noted in Chapter 3, it has strength aluminum alloy castings. Mechanical properties based onbeen recognized for many years that special care in the application the results of excised or prolongation specimens representing theof metal ﬂow and chill practices can lead to superior properties for actual casting rather than separately cast specimens that representaluminum casting alloys, and the consistent use of such practices conformance to expected chemistry and heat treatment responses.has led to a classiﬁcation of aluminum castings known as “premium In most cases, this and other speciﬁcations and standards serve onlyquality” or “premium engineered” castings. as the guide to separately negotiated requirements. With the pas- The typical and minimum properties of the more widely used sage of time property requirements for premium engineered cast-casting alloys developed using this technology are summarized ings increasingly exceeded those deﬁned by this speciﬁcation.in Tables 8.9 and 8.10, respectively (Ref 8, 15). The minimum Plaster cast low-pressure impellers and rotors that were heavilyproperties shown are the design mechanical properties published and directionally chilled routinely exceeded even negotiated prop-in MMPDS (previously known as MIL-HDBK-5) and from erty limits. For level and conventionally poured premium engi-AMS-A-21180 (previously MIL-A-21180). Note the several lev- neered castings, consistently meeting mechanical testing require-els of control on location and quality of casting, which some- ments was more tenuous when guarantees for tensile propertiestimes greatly inﬂuences the published design property. were 15 to 25% and ductility 60 to 100% higher than the limits
88 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsTable 8.7 (continued) Tension Shear Fatigue Modulus Ultimate Yield Elongation Hardness(b), ultimate endurance of strength, strength(a), in 5D, HB strength, limit(b), elasticity(c),Alloy Temper MPa MPa % 500 kg/10 mm MPa MPa GPaPermanent mold casting (continued)851.0 T5 140 75 5 45 95 60 71 T6 125 ... 8 ... ... ... 71852.0 T5 220 160 5 70 145 75 71Die casting360.0 F 305 170 3 75 195 140 71A360.0 F 315 165 4 75 180 124 71380.0 F 315 160 3 80 195 140 71A380.0 F 325 160 4 80 185 140 71383.0 F 310 150 4 75 ... 145 71384.0 F 330 165 3 85 200 140 ...390.0 F 280 240 <1 ... ... ... ...B390.0 F 315 250 <1 120 ... 140 81392.0 F 290 270 <1 ... ... ... ...413.0 F 295 145 3 80 170 130 71A413.0 F 290 130 4 80 170 130 ...C443.0 F 230 95 9 65 200 115 71518.0 F 310 193 5 80 200 140 ...(a) For tensile yield strengths, offset ϭ 0.2%. (b) Based on 500,000,000 cycles of completely reversed stress using R.R. Moore type of machines and specimens. (c) Average of tension andcompression moduli; compressive modulus is nominally about 2% greater than the tension modulus. Source: Ref 3–5deﬁned by statistical analysis, and every technique permitted by and 3 to 4% in elongation are sometimes seen. Such differences arepracticality and speciﬁcation was used to improve conformance. particularly signiﬁcant when it is noted that the values for theAlloying impurities were reduced, soluble phase components were premium quality castings are based on tests of specimens cut fromadjusted, heat treatment practices stretched to permissible limits, the castings, whereas the published typical and minimum values forand there was unusual concentration on the metallurgical structure standard alloys are based on tests of separately cast tensile speci-of critical casting areas corresponding to test specimen locations. mens. Aluminum rocker arm requirements include strength at modestly Squeeze Casting. In recent years, broader use has been madeelevated temperatures, hardness, and cost.Alloy 333.0, developed at of techniques for applying pressure to the metal while it is solidi-the same time as 319.0 as the preferred secondary general-purpose fying during the manufacture of castings. The most common andpermanent mold composition, was selected for this application. Over commercially most widely implemented technique is squeeze cast-several years, randomly selected parts were destructively tested to ing (see Chapter 3, Section 3.5.5).ensure that casting quality and properties were maintained. The The properties of representative castings produced by squeezepower of casting process and solidiﬁcation conditions was evident. casting technology are presented in Table 8.11, as published in RefTypical mechanical properties for 333.0-T6 are 42 ksi (290 MPa) 8 and 16, compared with the published typical properties of alu-tensile strength, 30 ksi (210 MPa) yield strength, and 2% elongation. minum castings of the same alloys.What was consistently demonstrated was 60 ksi (420 MPa) tensile The strengths range from about the same as to about 5 ksi (35strength, 50 ksi (350 MPa) yield strength, and 5% elongation, easily MPa) above the typical properties for comparable sand and per-exceeding speciﬁcation requirements for all conventional high- manent mold castings, very signiﬁcant considering that the valuesstrength alloys in use at that time and matching many wrought com- for the squeeze castings are based on tests of specimens cut frompositions in plate and forged form with the advantage of near-net- the castings themselves, whereas the typical values used in com-shape and anisotropic properties. The application of premium parison are based on separately cast test bars. In addition, theengineered casting practices even to conventional casting alloys pro- elongations of the squeeze castings are, with only one exception,vides signiﬁcant rewards. signiﬁcantly higher than the published typical values. The magnitude of the improvement achievable utilizing pre- In general, it appears that consistently better properties may bemium quality practices may be seen by comparing the values in obtained by squeeze casting than by conventional casting tech-Tables 8.9 and 8.10 with those in Tables 8.6 to 8.8, where differ- nologies, in the absence of the application of premium castingences of 5 to 15 ksi (35 to 105 MPa) or more in tensile yield strength technologies.
Chapter 8: Properties and Performance of Aluminum Castings / 91Table 8.8 (continued) Tension Compression Shear Ultimate Yield yield ultimate Elongation strength strength(a) strength(a) strength in 2 in. or 4D,Alloy Temper ksi MPa ksi MPa % ksi MPa ksi MPa RefPermanent mold casting (continued)D357.0 T6 46.0 315 39.0 270 3.0 39.0 270 29.0 200 13(b)359.0 T6 45.0 310 35.0 240 4 35.0 240 28.0 195 13(b) T61 45.0 310 34.0 235 4.0 ... ... ... ... 6 T62 47.0 325 38.0 260 3.0 ... ... ... ... 6443.0 F 21.0 145 7.0 50 2.0 ... ... ... ... 6B443.0 F 21.0 145 6.0 40 2.5 ... ... ... ... 6A444.0 T4 20.0 140 ... ... 20.0 ... ... ... ... 6513.0 F 22.0 150 12.0 85 2.5 ... ... ... ... 6535.0 F 35.0 240 18.0 125 8.0 ... ... ... ... 6705.0 T5 37.0 255 17.0 120 10.0 ... ... ... ... 6707.0 T7 45.0 310 35.0 240 3.0 ... ... ... ... 6711.0 T1 28.0 195 18.0 125 7.0 ... ... ... ... 6713.0 T5 32.0 220 22.0 150 4.0 ... ... ... ... 6850.0 T5 18.0 125 ... ... 8.0 ... ... ... ... 6851.0 T5 17.0 115 ... ... 3.0 ... ... ... ... 6 T6 18.0 125 ... ... 8.0 ... ... ... ... 6852.0 T5 27.0 185 ... ... 3.0 ... ... ... ... 6Die casting360.0 FA360.0 F380.0 FA380.0 F383.0 F384.0 F390.0 F Not available for die castingsB390.0 F392.0 F413.0 FA413.0 FC443.0 F518.0 F(a) For tensile compressive yield strengths, offset ϭ 0.2%. (b) Values for class 1 only Semisolid casting also holds promise for providing higher- typical values used in comparison are based on separately cast testquality aluminum alloy castings, though it has as yet been less bars. The elongations of the semisolid castings are superior to thewidely implemented successfully. The properties of some repre- typical values for sand castings and are about the same as those forsentative semisolid casting are presented in Table 8.12, again with permanent mold castings.published typical values for sand and permanent mold castings. It appears that with careful engineering of the process, some As for squeeze castings, the strengths of the semisolid castings gains are possible with semisolid casting if the process can berange from about the same as to about 5 ksi (35 MPa) above the successfully implemented on a broader scale.typical properties for comparable sand and permanent mold cast- High-Integrity Die Casting. The application of vacuum andings. Also, as in the case for squeeze castings, this is signiﬁcant other technologies to die casting has resulted in superior strengthsconsidering that the values for the semisolid castings are based on and substantially higher elongations especially when combinedtests of specimens cut from the castings themselves, whereas the with process features described in Chapter 3, Section 3.6.2. Figure
92 / Aluminum Alloy Castings: Properties, Processes, and Applications Table 8.9 Typical mechanical properties of premium engineered aluminum castings Typical values of premium engineered casting are the same regardless of class or the area from which the specimen is cut; see Table 8.10 for minimum values. Tension Fatigue Ultimate strength Yield strength Elongation endurance limit(a) in 50 mm (2 in.), Alloy Temper ksi MPa ksi MPa % ksi MPa A201.0 T7 72 495 65 448 6 14 97 A206.0 T7 65 445 59 405 6 13 90 224.0 T7 61 420 48 330 4 12.5 86 249.0 T7 68 470 59 407 6 11 75 354.0 T6 55 380 41 283 6 19.5(b) 135(b) C355.0 T6 46 317 34 235 6 14 97 A356.0 T6 41 283 30 207 10 13 90 A357.0 T6 52 360 42 290 8 13 90 (a) Rotating beam reversed bending (R = −1.0) tests; endurance limit at 5 ϫ 108 cycles. (b) Fatigue strength for 106 cycles. Source: Ref 88.2 (Ref 17) illustrates the properties obtained in European appli- erties above the ranges of typical and minimum values for com-cations of this technology; speciﬁc heat treatment conditions were parable sand and permanent mold castings. The principal value ofnot cited but are assumed to comprise lower solution heat treatment the study appears to have been that the published values based ontemperature than that of the true T6 temper. cast test bars are pretty representative of what may be expected in According to Altenpohl (Ref 17), the pressure in the casting closely controlled high-quality commercial production, providedchamber must be less than 50 millibars (5 kPa) to ensure the success consistent casting practices and quality control are exercised; inof the vacuum casting technique, and by its application components such cases, it appears that the use of the reduced strength guidelinepreviously made by other casting processes, forging, and impact (75%) may not be necessary.extrusion have been replaced. USCAR. In the period from 1999 to 2001, a number of auto- 8.4 Fatigue Properties of Aluminum Castingmotive components were produced and evaluated by USCAR Alloys(Ref 18) to determine the statistical levels of strength achievablewith several carefully controlled casting processes, including in Rotating beam reversed-bending fatigue data, at a stress ratio ofsome cases vacuum casting and squeeze casting. In all of the –1.0, have long been a standard in aluminum industry publications,USCAR activity, the test results were based on specimens cut and extensive ﬁles of such data are available for aluminum castingfrom speciﬁc locations in actual full-size castings. A summary of alloys as presented herein. It is appropriate to recognize that suchthe tensile properties of the castings from that study are presented data are simply one of many indices of fatigue strength, and forin Table 8.13. speciﬁc applications, engineers may wish to consult data for other While individual castings developed interesting properties in this stress ratios such as 0.0, ϩ0.1, and/or ϩ0.5.study, none of the practices employed consistently provided prop- The fatigue properties of a rather wide range of sand and per- manent mold castings (specimens per Appendix 3, Fig. A3.2) at room temperature are summarized in Table 8.14 (Ref 15). Actual rotating beam (R ϭ –1.0) fatigue curves for representative lots of castings at room temperature are shown in Data Set 6, in these cases often including both smooth and notched specimens of the types in Appendix 3, Fig. A3.2. In most cases, the specimens were as-cast test bars, tested with the as-cast surface in place; in a few cases, the tests were made with specimens machined from cast parts, such as pistons. A summary of the rotating-beam fatigue strengths from these tests of individual castings (as contrasted to the “typical” values in Table 8.14) is presented in Table 8.15. Most of these individual test results are compatible with the typical values in Table 8.14. The fatigue strengths of a number of these alloys from similar tests at elevated temperatures are presented in Table 8.16. A close review of the data in Tables 8.14 to 8.16 indicates to theFig. 8.2 Average tensile properties of representative aluminum alloy castings authors that these data, though developed in accordance to good produced by vacuum technology. UTS, ultimate tensile strength; engineering laboratory standards, should be used very carefully,TYS, tensile yield strength. Source: Ref 17 and the differences from alloy to alloy or among tempers of a
Chapter 8: Properties and Performance of Aluminum Castings / 97Table 8.14 (continued) Fatigue strength at life of Endurance limit 104 cycles 105 cycles 106 cycles 107 cycles 108 cycles at 5 ϫ 108 cyclesAlloy Temper ksi MPa ksi MPa ksi MPa ksi MPa ksi MPa ksi MPaPermanent mold casting (continued)359.0 T61 43.0 297 34.0 234 27.0 186 21.5 148 17.5 121 16.5 114 T62 ... ... 37.0 255 28.0 193 21.0 145 17.0 117 16.0 110A390.0 T6 ... ... ... ... ... ... ... ... ... ... 17.0 117 T7 ... ... ... ... ... ... ... ... ... ... 15.0 103B443.0 F ... ... ... ... ... ... ... ... ... ... 8.0 55513.0 F ... ... ... ... ... ... ... ... ... ... 10.0 69711.0 F ... ... ... ... ... ... ... ... ... ... 11.0 76713.0 T5 ... ... ... ... ... ... ... ... ... ... 9.0 62850.0 T5 ... ... ... ... ... ... ... ... ... ... 9.0 62851.0 T5 ... ... ... ... ... ... ... ... ... ... 9.0 62852.0 T5 11.0 76Die casting360.0 F ... ... 30.0 207 25.0 172 23.0 159 21.0 145 19.0 131A360.0 F ... ... ... ... ... ... ... ... ... ... 18.0 124364.0 F ... ... ... ... ... ... ... ... ... ... 18.0 124380.0 F ... ... 28.0 193 22.0 152 20.5 141 20.0 138 20.0 138A380.0 F ... ... ... ... ... ... ... ... ... ... 20.0 138384.0 F 39.0 269 32.0 221 26.0 179 23.5 162 22.0 152 21.5 148390.0 F ... ... ... ... ... ... ... ... ... ... 11.0 76B390.0 F ... ... ... ... ... ... ... ... ... ... 20.0 138413.0 F ... ... ... ... ... ... ... ... ... ... 19.0 131A413.0 F ... ... ... ... ... ... ... ... ... ... 19.0 131C443.0 F ... ... ... ... ... ... ... ... ... ... 16.0 110513.0 F ... ... ... ... ... ... ... ... ... ... 18.0 124515.0 F ... ... ... ... ... ... ... ... ... ... 19.0 131518.0 F ... ... ... ... ... ... ... ... ... ... 20.0 138Metric values of strength determined by multiplying strengths originally determined in English units by conversion facator of 6.897.English units measured by nearest 0.5 ksi; metric units rounded to nearest MPa. Source: Aluminum Association and Alcoa publications fatigue strengths include sand cast A206.0-T71 and A240.0-F, per- Other illustrations of such differences are found in Data Set 6, manent mold cast 354.0-T6, 359.0-T6, and A390.0-T6. Among thein which the fatigue results for permanent mold cast 242.0-T571 die cast alloys, there was less overall variability, but 384.0-F ex-and for sand cast 355.0-T7 and -T71, for which tests were made hibited the highest strengths. The role of positive residual stressof both as-cast test bars and of specimens taken from actual cast- patterns in promoting these speciﬁc alloys is unknown, but it mightings. In both cases, as illustrated in the table that follows, the be noted that all of the specimens for the die castings had as-castfatigue endurance limits were signiﬁcantly lower for specimens surfaces, perhaps accounting for their apparently overall highermachined from the castings than for the as-cast test bars: fatigue strengths. Overall, it is fair to say that with a few exceptions there is not a great amount of variability in endurance limits among Endurance limit the alloys, for either smooth or notched specimens.Alloy and temper Fatigue specimens ksi MPa At elevated temperatures, as at room temperature, there are not242.0-T571 As-cast test bars 15.0 103 very great differences among the endurance limits of the various Machined from cast pistons 9.5 66C355.0-T7, -T71 As-cast test bars 10.5 72 alloys. Machined from cast crankcase 5.5 38 It should be emphasized that all of the values in Tables 8.14 and Table 8.16 are based on tests of small specimens machined from In these cases, it should be noted that the as-cast test bars and castings, including in many (regrettably unidentiﬁed) cases, castthe cast parts used for each alloy were totally different lots, and so test bars. These values may not be representative of the perfor-the comparisons are not perfect; however, the differences seem to mance of speciﬁc cast components. More detail on the variationssupport indications that there is a positive inﬂuence on fatigue life that may be observed is illustrated in the following sections.of having cast-to-shape fatigue specimens. This, of course, also may suggest that for cast parts where the 8.4.1 Inﬂuence of Casting Quality on Fatiguesurfaces are in highly stressed regions, the design of the casting Strengthmay favor having the as-cast surface intact, with the resultant Several studies have been reported indicating the inﬂuence ofpositive residual stresses working in favor of improved perfor- casting process and microstructure on fatigue strength.mance. In any such considerations, care should be taken to provide Data from Juvinall (Ref 20), reproduced in Fig. 8.3, illustrate thatfor a smooth, stress-raiser-free ﬁnished surface on the as-cast part. in general the fatigue strengths of aluminum castings are not as high Ignoring such inﬂuences, for the moment, of the alloys and as those of wrought aluminum products (i.e., components madetempers for which data are available, those exhibiting the highest from plate, forgings, or extrusions). Further, indications from this
98 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsTable 8.15 Summary of reversed-bending fatigue curves for representative lots of aluminum alloy castingsStress ratio, R = −1.0 Endurance limit(c), ksi Type of specimens(b) Smooth NotchedAlloy Temper Cast part(a) Lot ID Smooth Notched ksi MPa ksi MPaPlaster mold casting255.0 T62 CTB D1699 X X 15.0 103 7.5 52C355.0 T62 CTB D1701 X X 15.0 103 7.5 52356.0 T6 CTB D223A,B X X 12.0 83 8.0 55 T61 CTB D1702 X X 13.0 90 7.5 52A356.0 T61 CTB D1703 X X 12.0 83 7.0 48 T61 Casting 206548 X X 8.0 55 8.0 55 T61 PEC Casting 206547 X X 11.0 76 7.5 52 T62 Casting 175138 X ... 13.0 90 ... ...Sand casting213.0 F CTB C6611 X X 10.0 69 7.5 52224.0 T62 CTB E8419C X X 12.5 86 7.5 52240.0 F CTB D23,D403 X ... 18.0 124 ... ... CTB D424 X ... 13.0 90 ... ... F CTB D2551 X X 17.0 117 7.5 52242.0 O(T21) CTB C7043F X X 10.0 69 8.0 55 T571 CTB C7043A X X 12.0 83 9.0 62 T75 CTB L2567 X X 9.0 62 5.5 38 T77 CTB C5107 X X 11.5 79 7.5 52 CTB L2579 X ... 9.5 66 ... ... CTB C6765B X X 10.0 69 7.0 48249.0 T63 CTB E8083D,E8115 X X 9.5 66 6.0 41295.0 T6 CTB C3508 X ... 7.0 48 ... ... CTB Unknown X ... 7.5 52 ... ... CTB L1585 X ... 7.0 48 ... ... T62 CTB Unknown X ... 7.0 48 ... ... CTB L1670 ... X ... ... 5.0 34308.0 F CTB 117105 X X 11.5 79 7.0 48319.0 F CTB C6884E X X 12.0 83 9.0 62 T5 CTB C6884T X X 11.0 76 8.0 55 T6 CTB C6884K X X 12.5 86 10.0 69 T71 CTB C6884L X X 10.5 72 8.0 55355.0 T51 CTB C6285M X X 10.0 69 6.0 41 T6 CTB 5 lots X ... 10.0 69 ... ... CTB 5 lots ... X ... ... 9.0 62 T61 CTB C3509-T61 X X 9.5 66 7.5 52 T7 CTB C6285K X X 10.5 72 7.0 48 T71 CTB C6285L X X 11.5 79 7.5 52 T7,T71 CTB Unknown X X 10.5 72 7.0 48 Cast crankcase 175472 X ... 5.5 38 ... ...A355.0 T51 CTB L758 X ... 8.5 59 ... ... T59 CTB L759 X ... 8.5 59 ... ... T6 CTB P255A X ... 7.5 52 ... ...B355.0 T6 CTB L3032 X ... 8.5 59 ... ... CTB L3032 ... X ... ... 8.5 59356.0 T51 CTB C6385D X X 9.0 62 6.5 45 CTB L757 X ... 6.5 45 ... ... CTB L1661 ... X ... ... 6.0 41 T6 CTB L1704 X ... 7.5 52 ... ... CTB C6385K X X 12.0 83 9.0 62 CTB C3510 X ... 8.5 59 ... ... CTB C3510 ... X ... ... 6.0 41 T7,T71 CTB C3510,C6385L X ... 8.0 55 ... ... CTB C3510,C6385L ... X ... ... 7.0 48B443 F CTB 117104 X X 8.5 59 6.0 41712.0 F CTB C8455 X X 9.5 66 7.0 48A712.0 F CTB C8533 X X 10.5 72 7.0 48 CTB C9004H X X 7.5 52 6.0 41852.0 T5 CTB C8454 X X 9.5 66 6.0 41Permanent mold casting213.0 F CTB D665 X X 17.0 117 7.5 52 CTB L1652 X X 9.5 66 7.0 48242.0 T571 CTB C6156 X X 15.0 103 7.5 52 CTB C9609D X X 15.5 107 9.0 62 Pistons 301974 X ... 9.5 66 ... ... VRC pistons 317189 X ... 10.0 69 ... ... T61 CTB C6156 X X 15.0 103 7.5 52 (continued)(a) CTB, cast test bars; casting, undeﬁned cast part other than CTB; speciﬁc part given if stated on data sheet. (b) Specimens shown in Appendix 3, Fig. A3.2(b) for notched specimen,notch-tip radius Յ 0.001 in; Kt Ն 12. (c) Endurance limit at 500 million cycles. Source: Ref 19
Chapter 8: Properties and Performance of Aluminum Castings / 99Table 8.15 (continued) Endurance limit(c), ksi Type of specimens(b) Smooth NotchedAlloy Temper Cast part(a) Lot ID Smooth Notched ksi MPa ksi MPaPermanent mold casting (continued)296.0 T6 CTB C5449 X X 12.0 83 8.5 59 T7 CTB C5449 X X 8.0 55 6.5 45308.0 F CTB C8902 X X 13.0 90 8.0 55332.0 T5 CTB C8281 X X 14.0 97 8.0 55333.0 F CTB C6028 X X 13.0 90 8.0 55 T5 CTB C6028 X X 12.0 83 8.0 55 D278B X X 13.0 90 7.5 52 T6 CTB C6028 X X 15.0 103 10.0 69 T7 CTB C6028 X X 12.0 83 9.0 62 C9176C X X 12.0 83 8.0 55336.0 T551 CTB 105678 X X 13.5 93 7.5 52A344.0 T4 CTB 317644 X X 9.0 62 3.5 24354.0 T61 CTB D3860 X X 19.0 131 12.0 83 E6161 X X 15.0 103 9.0 62355.0 T51 CTB C8067K X X 12.5 86 7.0 48 T6 CTB C5448 X X 10.0 69 8.0 55 C8067K X X 16.0 110 10.5 72 T62 CTB C5448 X X 9.5 66 6.0 41 C8067K X X 15.5 107 7.5 52 T7 CTB C8067K X X 13.0 90 8.5 59 T71 CTB C5448 X X 9.5 66 6.0 41 C8067K X X 12.5 86 8.0 55C355.0 T61 CTB D2245B X X 12.5 86 10.0 69 T61 PEC PE casting 206428 X X 12.0 83 9.0 62356.0 T6 CTB C6235 X X 13.0 90 7.5 52 T7 CTB C6235 X X 10.5 72 5.0 34A356.0 T6 CTB D2543 X X 13.5 93 7.5 52 T61 Casting 206587 X X 8.0 55 7.5 52 PE casting 206588 X X 8.0 55 7.5 52 PE casting 206547 X X ND ... ND ...A357.0 T61 CTB 302022 X X 12.5 86 7.5 52 302023 X X 13.5 93 7.0 48 T62 Casting 302108 X X 11.0est 76est 6.0 41359.0 T61 CTB D4228 X X 16.0 110 11.0 76 T62 CTB E2520A X X 15.0 103 9.0 62B443.0 F CTB 118348 X X 7.0 48 4.0 28C712.0 F CTB C8278 X X 11.0 76 6.5 45850.0 F CTB R8036 X ... 9.0 62 ... ... T101 CTB 270257 X ... 10.0 69 ... ... T5 CTB 270263 X ... 8.5 59 ... ...851.0 T6 CTB C1670 X ... 8.5 59 ... ...852.0 T5 CTB D3278 X X 11.5 79 5.0 34 C8094 X X 10.5 72 5.0 34Die casting360.0 F CTB P1003 X ... 19.0 131 ... ...A360.0 F CTB P1004 X ... 18.0 124 ... ...364.0 F CTB 206520 X ... 15.0 103 ... ...380.0 F CTB P1005 X ... 18.5 128 ... ... CTB-as cast 147979 X ... 21.0 145 ... ... 0.01 in. removed X ... 19.5 134 ... ... 0.025 in. removed X ... 17.5 121 ... ... Notches ... X ... ... 7.0 48A380.0 F CTB P1006 X ... 21.5 148 ... ...383.0 F CTB P1007 X ... 21.0 145 ... ...390.0 F CTB-as cast 317782 X X 19.0 131 10.5 72 CTB machined 317782 X X 19.0 131 10.5 72413.0 F P998 X ... 19.0 131 ... ... 317250 X X 13.0 90 5.5 38B443.0 F CTB P1000 X ... 16.5 114 ... ...518.0 F CTB 158837 X X 15.5 107 6.0 41 P1002 X ... 22.5 155 ... ...(a) CTB, cast test bars; casting, undeﬁned cast part other than CTB; speciﬁc part given if stated on data sheet. (b) Specimens shown in Appendix 3, Fig. A3.2(b) for notched specimen, notch-tip radius Յ 0.001 in; Kt Ն 12. (c) Endurance limit at 500 million cycles. Source: Ref 19
Chapter 8: Properties and Performance of Aluminum Castings / 101Table 8.16 (continued) Test Fatigue strength at life of Endurance limit temperature 104 cycles 105 cycles 106 cycles 107 cycles 108 cycles at 5 ϫ 108 cyclesAlloy Temper °F °C ksi MPa ksi MPa ksi MPa ksi MPa ksi MPa ksi MPaPermanent mold casting (continued)355.0 T71 RT RT ... ... 27.0 186 21.0 145 17.0 117 14.5 100 13.0 90 300 150 ... ... 25.0 172 19.5 134 15.0 103 11.0 76 10.0 69 400 205 ... ... 21.0 145 16.0 110 12.0 83 8.5 59 8.0 55 600 315 ... ... 10.0 69 8.0 55 5.5 38 3.0 21 2.5 17359.0 T61 RT RT 43.0 297 34.0 234 27.0 186 21.5 148 17.5 121 16.5 114 300 150 41.0 283 31.0 214 23.5 162 18.5 128 14.0 97 12.5 86 400 205 34.0 234 26.0 179 18.0 124 11.5 79 6.0 41 4.0 28Die casting380.0 F RT RT ... ... 28.0 193 22.0 152 20.5 141 20.0 138 20.0 138 300 150 ... ... 18.5 128 15.0 103 13.0 90 11.0 76 10.0 69 400 205 ... ... 15.0 103 11.0 76 8.5 59 7.5 52 7.0 48 500 260 ... ... 12.5 86 9.0 62 6.5 45 5.5 38 5.0 34Metric values of strength determined by multiplying strengths originally determined in English units by conversion factor of 6.897. RT, room temperature. Source: Aluminum Associationand Alcoa publicationssummary are that the fatigue properties of permanent mold cast are presented, fatigue strength rather consistently increases as thealuminum alloys may be expected to be superior to those of sand degree of porosity is decreased, that is, as casting quality increases.castings, the lowest band. While there are few data to demonstrate it, it is also therefore Further indication that the fatigue strengths of cast aluminum reasonable to expect that improvements in casting practices thatcomponents may be expected to be inferior to those of wrought lead to better soundness and minimal porosity, such as premiumaluminum products are borne out by ﬂexural fatigue (R ϭ 0.0) tests quality casting, squeeze casting, and semisolid casting, will resultof 220.0-T4 and 356.0-T6 sand cast beams, 218.0-F and 380.0-F in improved fatigue properties. One indication of that is found indie cast beams, and 6061-T6 wrought beams (Ref 21), shown in the work of Williams and Fisher (Ref 23), shown in Fig. 8.6, whoFig. 8.4. The band of data for the cast beams falls consistently found that the axial-stress fatigue strengths of A356.0-T6 squeezebelow the curve for 6061-T6. castings consistently performed better than conventionally chill Such generalized views of the differences in fatigue lives of cast cast A356.0-T6 castings.and wrought aluminum alloys probably overlook the more basic Further evidence of the effect of defects and discontinuities isfact that casting quality itself is the most important factor in de- illustrated by the work on hot isostatic pressing by Boileau andtermining fatigue life (just as it is for strength and toughness). Data Wang discussed in Chapter 6.reported by Promisel (Ref 22), reproduced in Fig. 8.5, demonstratethat the degree of porosity of 295.0 (regrettably not documentedas to temper, but probably T6) has a direct bearing on fatigue 8.4.2 Inﬂuence of Stress Raisers on Fatigue Strengthstrength; for the eight different degrees of porosity for which data of Aluminum Castings As with wrought aluminum alloys, stress raisers such as notches or holes signiﬁcantly reduce the fatigue strengths of aluminum castings. Data were presented in Section 8.3.4, under “Premium Engineered Castings,” to show that fatigue strength decreases with increasing porosity, and notches represent an even more severe stress concentration. The S-N curves in Data Set 6, the results of which are summarized in Table 8.15, provide examples of the effects of severe machined notches (with theoretical stress con- centration factors, Kt > 12) on fatigue strengths of representative casting alloys; in these cases, the notched specimen endurance limits are one-third to one-half those for the smooth specimens. Sharp et al. (Ref 21) (Fig. 8.7) have shown that the sharp notch fatigue strengths of 355.0-T6 aluminum castings are about the same as, perhaps even slightly superior to, those of 6070-T6 and 7005-T53 wrought products. The signiﬁcance of this is that, despiteFig. 8.3 Alternating bending stress fatigue curves for wrought and cast alu- the smooth-specimen superiority of wrought products over cast- minum alloys. Source: Ref 20 ings, when real design discontinuities are present the fatigue prop-
102 / Aluminum Alloy Castings: Properties, Processes, and Applicationserties of the various products may not differ signiﬁcantly, and 8.4.3 Fatigue Strengths of Welded Aluminumimproving fatigue performance may be more a problem of reducing Castingscomponent stress concentrators and in the selection of an alloy or Few data are available to document the fatigue strengths ofproduct form. weldments in aluminum castings, but Sharp et al. (Ref 21) presentFig. 8.4 Flexural fatigue properties (R ϭ 0) of aluminum alloy beams produced from wrought and cast aluminum alloys. Source: Ref 20Fig. 8.5 Fatigue properties of 295.0 aluminum alloy castings with various degrees of porosity. Source: Ref 22
Chapter 8: Properties and Performance of Aluminum Castings / 103the results of axial-stress (R ϭ 0.0) fatigue tests of 355.0-T6 casting 8.5 Fracture Resistance of Aluminum Alloyswelded together with 355.0 as ﬁller metal and also 355.0-T6 weldedto 5456-H321 with 4043 as ﬁller metal, as in Fig. 8.8. There was Notch toughness, tear resistance, and plane-strain fracture tough-no signiﬁcant difference in fatigue strength of the two weld com- ness have been the primary measures used to assess the toughnessbinations, nor was there any signiﬁcant effect of removing the weld of aluminum alloy castings (Ref 24). Because of the difficulty inbead or leaving it intact. getting valid fracture toughness tests from castings, more data are available for notch toughness and tear resistance, but representative8.4.4 Design Fatigue Strengths for Aluminum data for all three are presented and discussed in the sections that Castings follow. MMPDS/MIL-HDBK-5H (Ref 15) includes strain-life fatigue 8.5.1 Notch Toughness and Notch Sensitivitycurves for use in design of aluminum aircraft. For aluminum alloycastings, a curve is shown only for A201.0-T7, and those data are One of the earliest approaches to the evaluation of the fracturereproduced in Fig. 8.9. No other fatigue data for aluminum castings characteristics of aluminum alloys was via tensile tests of speci-are presented. mens containing various types of stress raisers (Ref 24). The results from these tests were analyzed in terms of the theoretical stress- concentration factors. This approach, however, has not always been very useful in design, since the same theoretical stress concentra- tion factors can be obtained with a great variety of different geo- metrical notch and specimen conﬁgurations, each of which has a unique inﬂuence on the numerical results of the tests; if design is the goal, the notched specimen must mirror the stress conditions in the component, including its stress raisers. Therefore, the results of tensile tests of notched specimens have been used primarily to qualitatively merit rate aluminum alloys with respect to their notch toughness, that is, their ability to plas- tically deform locally in the presence of stress raisers and thus redistribute the stress. The notch tensile strength itself is of small value for this rating; the relationship of the notch tensile strength to the tensile properties is much more meaningful. For many years, the criterion most often used from notch tensile test results was the notch-strength ratio, the ratio of the notchFig. 8.6 Fatigue properties of conventionally cast and squeeze cast alumi- tensile strength to the tensile strength of the material. However, this num alloy A356.0-T6. Source: Ref 23 ratio tells little about the relative abilities of alloys to deformFig. 8.7 Rotating beam (R ϭ –1.0) fatigue properties of notched specimens from wrought and cast aluminum alloys. Source: Ref 21
104 / Aluminum Alloy Castings: Properties, Processes, and Applicationsplastically in the presence of stress raisers. In fact, for different strength tells more about the behavior of the material in the pres-notch geometries, it can indicate contradictory ratings (Ref 24). ence of a stress raiser than the ratio of the notch tensile strengthThere are instances, of course, when the notch-strength ratio is to the tensile strength. If the notch tensile strength is appreciablyuseful, for example, when a measure of tensile efficiency of a above the yield strength (regardless of its relation to the tensilespeciﬁc structural member is required, or when the ultimate strength strength), the material has exhibited an ability to deform locally inis the primary data taken for the smooth specimens, as in fatigue the presence of the stress raiser.tests or stress rupture tests. If the notch tensile strength is appreciably below the yield A more meaningful indication of the inherent ability of a material strength, the fracture must have taken place without very muchto plastically deform locally in the presence of a severe stress raiser plastic deformation. For a speciﬁc notch design, this may or mayis provided by the notch-yield ratio—the ratio of the notch tensile not provide much speciﬁc design information, but as a relativestrength to the tensile yield strength (Ref 24). The yield strength, measure of how several alloys behave in that situation, it is quitealthough arbitrarily deﬁned, is a measure of the lowest stress at useful. Further indication of this fact is the experimental result thatwhich appreciable plastic deformation occurs in a tensile test. There- the notch-yield ratio provides rather consistent ratings of manyfore, the relationship of the notch tensile strength to the yield alloys and tempers for a wide variety of notch geometries, and the ratings are consistent with those from fracture parameters, as de- scribed later. While a number of different designs of notch have been used by different investigators, very sharp 60° V-notches provide the great- est discrimination among different alloys. In addition, such notches come close to representing the most severe unintentional stress raiser that is likely to exist in a structure: a crack. ASTM standards for notch tensile testing (Ref 25) call for notch-tip radii equal to or less than 0.0005 in. (0.013 mm), easily maintained in machining aluminum specimens (though quality assurance measurements are recommended). Notch Toughness at Room Temperature. The speciﬁc design of notch for which data for a wide variety of casting alloys are available is shown in Appendix 3, Fig. A3.5. Representative data for various aluminum casting alloys with this design of specimen are given in Table 8.17 (Ref 24). Data for welds in various alu-Fig. 8.8 Axial-stress (R ϭ 0) fatigue properties of welded aluminum alloy minum casting alloys are presented in Table 8.18. In all cases, the castings. Source: Ref 21 data were generated in accordance with ASTM E 602 (Ref 25).Fig. 8.9 Best-ﬁt fatigue curves for aluminum alloy A201-T7 at various strain rates at 75 °F (24 °C). Source: Ref 14
106 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsTable 8.17 (continued) Ultimate tensile Tensile yield Notch tensileAlloy and strength strength(a) Elongation Reduction strengthtemper ksi MPa ksi MPa in 2 in., % of area, % ksi MPa NTS/TS NTS/YSPremium engineered casting (continued)249.0-T7 57.6 397 49.2 339 7.4 11 69.3 478 1.20 1.41354.0-T6 48.0 331 43.0 297 1.2 1 45.4 313 0.95 1.06C355.0-T6 43.6 301 40.8 281 1.0 1 43.4 299 1.00 1.06C355.0-T61 43.6 301 30.3 209 6.4 9 52.6 363 1.21 1.74A356.0-T6 41.6 287 30.2 208 8.8 10 51.4 355 1.23 1.70A357.0-T6 52.0 359 43.2 298 4.5 6 48.4 334 0.93 1.12A357.0-T61 51.2 353 40.0 276 11.4 13 56.2 388 1.10 1.41A357.0-T62 53.9 372 46.4 320 5.3 7 59.4 410 1.10 1.28NTS, notch tensile strength; TS, tensile strength; YS, yield strength. (a) For tensile yield strength, offset = 0.2%. Relative rankings of the casting alloys are presented in the bar Alloys A444.0-F and B535.0-F have among the best combina-graphs in Fig. 8.10, segregated by sand castings (Fig. 8.10a), per- tions of strength and notch toughness, as do the premium-strengthmanent mold castings (Fig. 8.10b), and premium-strength castings castings in the T61, T62, and T7 tempers; they fall in or near lower(Fig 8.10c). edge of the band for wrought alloy data. However, the other sand Alloy A444.0-F permanent mold castings, with the lowest yield and permanent mold cast alloys fall below the wrought alloy band;strength of the entire group, ranks highest. Otherwise, for the re- of the latter groups, the permanent mold castings generally exhibitspective groups, 295.0-T6 and B535.0-F rank highest among sand the best performance.cast alloys; A356.0-T6 and -T71 rank highest among permanent Relative rankings for welds in aluminum alloy castings based onmold castings; and 224.0-T7, A356.0-T6, and C355.0-T61 rank notch-yield ratio (Table 8.18) are shown in Fig. 8.12.highest among the premium-strength castings. Among the higher- Welds in A444.0-F have the highest notch-yield ratios by a con-strength casting alloys, the premium quality castings (that is, sand siderable margin, not surprising with their low strength. Alloyscastings made with special care to provide high metal chill rates 354.0-T62 and C355.0-T6 are within a fairly narrow range, within highly stressed regions) rate well, and A356.0-T6 consistently C355.0-T6 welds being slightly superior.has higher toughness than does 356.0-T6, the positive effect of its Once again, looking at the data on the basis of NYR versushigher purity (i.e., lower content of impurities such as iron). tensile yield strength (TYS) as in Fig. 8.13 reveals additional in- Looking at the relationship between notch-yield ratio (NYR) and formation.tensile yield strength also provides interesting information for cast- For the two higher-strength alloys, 354.0-T62 and C355.0-T6,ings (Fig. 8.11), most notably the relationship of their performance there is also an indication that welds made with 5356 and 5556 ﬁllerto that of wrought alloys. alloys have somewhat better combinations of strength and tough-Table 8.18 Representative notch toughness test results of welds in cast aluminum alloys at room temperatureSpecimens per Appendix 3, Fig. A3.5; each line represents the average of duplicate tests on one lot of material. Joint efﬁciencies based on typical values forparent alloys. No postweld thermal treatment Ultimate tensile Tensile yield Elongation Reduction Joint strength Notch tensileAlloy and temper Filler strength strength(a) in 2 in., of area, efﬁciency, Location strengthcombination alloy ksi MPa ksi MPa % % % of fracture(b) ksi MPa NTS/TS NTS/YSA444.0-F to A444.0-F 4043 23.8 164 9.5 66 12.1 22 100 B 27.5 190 1.15 2.90A444.0-F to 6061-T6 4043 24.0 166 11.4 79 5.7 23 100 B 29.3 202 1.22 2.51A444.0-F to 5456-H321 5556 24.1 166 12.2 84 12.1 27 100 B 29.5 203 1.22 2.42354.0-T62 to 354.0-T6 4043 37.8 261 21.5 148 6.4 10 76 A 32.0 221 0.85 1.48354.0-T62 to 6061-T6 4043 30.8 212 19.0 131 9.3 39 62 C 28.7 198 0.93 1.51354.0-T62 to 5456-H321 5556 37.7 260 24.6 170 3.6 5 75 A 37.7 260 1.00 1.53C355.0-T61 to 6061-T6 4043 28.9 199 19.3 133 7.1 32 66 C 34.5 238 1.19 1.79C355.0-T61 to 5456-H321 5556 35.4 244 24.4 168 3.6 5 81 A 40.5 279 1.15 1.66NTS, notch tensile strength; TS, tensile strength; YS, yield strength. (a) For joint yield strength, offset = 0.2%, over a 2 in. gage length. (b) Location of fracture of unnotched specimens: A,through weld; B, 1⁄2 to 21⁄2 in. from weld; C, edge of weld
Chapter 8: Properties and Performance of Aluminum Castings / 107ness than do welds made with 4043; this is also consistent with the band for wrought alloys; a notable exception is when the 4043 weldcase for wrought alloys. In low-strength, high-toughness alloy in 6061-T6 was heat treated and aged after welding.A444.0-F, choice of ﬁller alloy made little difference. Notch Toughness at Subzero Temperatures. The results of The notch toughness of most welds as measured by NYR is notch tensile tests of several aluminum casting alloys at subzerogenerally somewhat less than that for parent metal of the same temperatures are presented in Table 8.19. Data from these tests arestrength, the principal exceptions being welds made with the 5xxx plotted in Fig. 8.14 as a function of test temperature for sand castseries ﬁller alloys. Many data for 4043 welds fall well below the alloys at subzero temperatures (Fig. 8.14a and b), permanent mold cast alloys (Fig. 8.14c), and premium-strength sand cast alloys (Fig. 8.14d). From Fig. 8.14, it can be seen that the 3xx.0 and 4xx.0 casting alloys rather consistently retain most or all of their toughness at subzero temperatures, even to –423 °F (–253 °C) and –452 °F (–269 °C). Alloy A444.0-F (Fig. 8.14c), with its relatively low yield strength, showed an exceptionally high NYR, at or above 2.5, even at –320 °F (–196 °C). From the notch tensile data in Fig. 8.14(d), it is also clear that A356.0-T61 performed quite well even at –452 °F (–269 °C). Other casting alloys, notably the 2xx.0 and 5xx.0 series, generally show a consistent and more rapidly decreasing toughness with decrease in temperature. When the notch-yield ratios for cast alloys are viewed on the basis of yield strength level (Fig 8.15), A444.0-F exhibits exceptionally high toughness and, among the higher-strength alloys, the premium- strength cast alloys have the most consistently superior strength- toughness combination, similar to the case at room temperature. The performance of the permanent mold castings is generally nearly as good as the premium-strength castings and, in fact, B535.0Fig. 8.10 Relative rankings of notch toughness of aluminum casting alloys based upon notch-yield ratio. (a) Sand castings. (b) Permanent mold castings. (c) Premium engineered castings
108 / Aluminum Alloy Castings: Properties, Processes, and ApplicationsFig. 8.11 Notch-yield ratio versus tensile yield strength for selected aluminum alloy castingsand A356.0 permanent mold castings essentially match the per- When selecting cast alloys for cryogenic service, it seems es-formance of the premium-strength castings. The conventionally pecially important to pay careful attention to the casting process ascast sand castings rather consistently exhibit the poorest perfor- well as the alloy itself; high-quality casting processes yield superiormance. combinations of strength and toughness. Data for welds in cast alloys at subzero temperatures are pre- sented in Table 8.20, and the NYRs are plotted as a function of temperature in Fig. 8.16. Both 4043 and 5556 welds exhibited NYRs about the same at temperatures down to –320 °F (–196 °C) as at room temperature. At lower temperatures, both ﬁller alloys exhibited some signiﬁcant reduction, but in all cases, NYRs were above 1.0, even at –452 °F (–269 °C).Fig. 8.12 Rankings of notch toughness of welds in aluminum casting alloys Fig. 8.13 Notch-yield ratio versus tensile yield strength for welds in alu- based upon notch-yield ratio for combinations of casting alloys minum alloy castings for combinations of casting alloys and ﬁllerand ﬁller alloys (middle number) alloys (middle number)